Research, Development, and Technology

Turner-Fairbank Highway Research Center

6300 Georgetown Pike

McLean, VA 22101-2296

Identifying Incompatible 

Combinations of Concrete Materials:

Volume I—Final Report

PUBLICATION NO. FHWA-HRT-06-079 AUGUST 2006
FOREWORD 

Unexpected interactions between otherwise acceptable ingredients in portland cement concrete 

are becoming increasingly common as cementitious systems become more and more complex 

and demands on the systems are more rigorous. Such incompatibilities are exhibited as early 

stiffening or excessive retardation, potential for uncontrolled early-age cracking, and unstable or 

unacceptable air void systems. 

Based on the experimental work described in this volume, a protocol has been developed to 

allow product manufacturers, concrete producers, contractors and owners to monitor their 

materials and concrete systems. The protocol is phased to allow relatively simple field tests to 

provide early warnings of potential problems, and central laboratory tests to support and confirm 

the field work. Tests conducted before beginning construction allows users to plan for changes in 

materials and environment. By monitoring materials with relatively simple field tests during 

construction, the users can detect when significant changes have occurred, indicating potential 

construction problems. 

 Gary Henderson 

 Director, Office of Infrastructure 

 Research and Development 

Notice 

This document is disseminated under the sponsorship of the U.S. Department of Transportation 

in the interest of information exchange. The U.S. Government assumes no liability for the use of 

the information contained in this document. This report does not constitute a standard, 

specification, or regulation. 

The U.S. Government does not endorse products or manufacturers. Trademarks or 

manufacturers’ names appear in this report only because they are considered essential to the 

objective of the document. 

Quality Assurance Statement 

The Federal Highway Administration (FHWA) provides high-quality information to serve 

Government, industry, and the public in a manner that promotes public understanding. Standards 

and policies are used to ensure and maximize the quality, objectivity, utility, and integrity of its 

information. FHWA periodically reviews quality issues and adjusts its programs and processes to 

ensure continuous quality improvement. 
Technical Report Documentation Page 

1. Report No. 

FHWA-HRT-06-079 

2. Government 

Accession No. 

3. Recipient's Catalog No. 

5. Report Date 

August 2006 

4. Title and Subtitle 

Identifying Incompatible Combinations of Concrete Materials: 

Volume I—Final Report 6. Performing Organization Code: 

7. Author(s) 

Peter C. Taylor Vagn C. Johansen 

Luis A. Graf Ronald L. Kozikowski 

Jerzy Z. Zemajtis Chiara F. Ferraris 

8. Performing Organization Report No. 

9. Performing Organization Name and Address 10. Work Unit No. 

CTLGroup 

5400 Old Orchard Road 

Skokie, IL 60077 

11. Contract or Grant No. 

DTFH61-03-X-00102 

12. Sponsoring Agency Name and Address 13. Type of Report and Period Covered 

FHWA and 

Portland Cement Association (24 percent) 

5420 Old Orchard Road 

Skokie, IL 60077 

14. Sponsoring Agency Code 

15. Supplementary Notes 

Chiara F. Ferraris of NIST worked under separate contract to FHWA. 

The Contract Officer’s Technical Representative was Peter Kopac, HRDI-12. 

16. Abstract 

Unexpected interactions between otherwise acceptable ingredients in portland cement concrete are becoming 

increasingly common as cementitious systems become more and more complex and demands on the systems are 

more rigorous. Such incompatibilities are exhibited as early stiffening or excessive retardation, potential for 

uncontrolled early-age cracking, and unstable or unacceptable air void systems. 

A number of test methods have been reviewed to assess their usefulness in detecting incompatibility early to help 

prevent problems with pavements in the field. A protocol has been developed to allow product manufacturers, 

concrete producers, contractors, and owners to monitor their materials and concrete systems. The protocol is 

phased to allow relatively simple field tests to provide early warnings of potential problems and then central 

laboratory tests to support and confirm the field work. 

This is the first of two volumes. The other volume in this series is: 

FHWA HRT-06-080, Identifying Incompatible Combinations of Concrete Materials: Volume II—Test Protocol. 

17. Key Words 

Cement, fly ash, slag, incompatibility, admixture, early stiffening, 

cracking, air void system 

18. Distribution Statement 

19. Security Classif. (of this report) 

Unclassified 

20. Security Classif. (of this page) 

Unclassified 

21. No. of Pages 

159 

22. Price 

Form DOT F 1700.7 (8-72) Reproduction of completed page authorized
ii 

SI* (MODERN METRIC) CONVERSION FACTORS 

APPROXIMATE CONVERSIONS TO SI UNITS

Symbol When You Know Multiply By To Find Symbol 

LENGTH 

in inches 25.4 millimeters mm 

ft feet 0.305 meters m 

yd yards 0.914 meters m 

mi miles 1.61 kilometers km 

AREA 

in2 square inches 645.2 square millimeters mm2

ft2 square feet 0.093 square meters m2

yd2 square yard 0.836 square meters m2

ac acres 0.405 hectares ha

mi2 square miles 2.59 square kilometers km2

VOLUME 

fl oz fluid ounces 29.57 milliliters mL 

gal gallons 3.785 liters L 

ft3 cubic feet 0.028 cubic meters m3 

yd3 cubic yards 0.765 cubic meters m3 

NOTE: volumes greater than 1000 L shall be shown in m3

MASS 

oz ounces 28.35 grams g

lb pounds 0.454 kilograms kg

T short tons (2000 lb) 0.907 megagrams (or "metric ton") Mg (or "t") 

TEMPERATURE (exact degrees) o

F Fahrenheit 5 (F-32)/9 Celsius oC 

or (F-32)/1.8 

ILLUMINATION 

fc foot-candles 10.76 lux lx

fl foot-Lamberts 3.426 candela/m2 cd/m2

FORCE and PRESSURE or STRESS 

lbf poundforce 4.45 newtons N 

lbf/in2 poundforce per square inch 6.89 kilopascals kPa 

APPROXIMATE CONVERSIONS FROM SI UNITS 

Symbol When You Know Multiply By To Find Symbol 

LENGTH

mm millimeters 0.039 inches in 

m meters 3.28 feet ft 

m meters 1.09 yards yd 

km kilometers 0.621 miles mi 

AREA mm2

 square millimeters 0.0016 square inches in2 

m2 square meters 10.764 square feet ft2 

m2 square meters 1.195 square yards yd2 

ha hectares 2.47 acres ac

km2 square kilometers 0.386 square miles mi2 

VOLUME 

mL milliliters 0.034 fluid ounces fl oz 

L liters 0.264 gallons gal 

m3 cubic meters 35.314 cubic feet ft3 

m3 cubic meters 1.307 cubic yards yd3 

MASS 

g grams 0.035 ounces oz

kg kilograms 2.202 pounds lb

Mg (or "t") megagrams (or "metric ton") 1.103 short tons (2000 lb) T 

TEMPERATURE (exact degrees) o

C Celsius 1.8C+32 Fahrenheit oF 

ILLUMINATION 

lx lux 0.0929 foot-candles fc 

cd/m2 candela/m2 0.2919 foot-Lamberts fl

FORCE and PRESSURE or STRESS 

N newtons 0.225 poundforce lbf 

kPa kilopascals 0.145 poundforce per square inch lbf/in2

*SI is the symbol for th International System of Units. Approp e riate rounding should be made to comply with Section 4 of ASTM E380. 

(Revised March 2003)
iii 

TABLE OF CONTENTS 

CHAPTER 1. INTRODUCTION................................................................................................ 1

Overview ..................................................................................................................................... 1 

Background ................................................................................................................................. 1 

Study Goals, Objectives, and Scope............................................................................................ 3 

CHAPTER 2. LITERATURE REVIEW.................................................................................... 5

General ........................................................................................................................................ 5 

Need for Information Request Responses................................................................................... 5 

Construction Materials and Practices.......................................................................................... 6 

Findings on Rheology, Cracking, and Air void System.............................................................. 9 

Summary ................................................................................................................................... 33 

CHAPTER 3. PROJECT TASKS ............................................................................................. 35

TASK 2.1.1—EARLY SETTING OR EXCESSIVE RETARDATION.................................. 35 

Test Matrix for Paste and Mortar Systems................................................................................ 40 

Testing Concrete ....................................................................................................................... 51 

Test Methods Discussion .......................................................................................................... 57 

Observations.............................................................................................................................. 64 

Summary ................................................................................................................................... 85 

TASK 2.1.2—CRACKING....................................................................................................... 91 

Mix designs ............................................................................................................................... 95 

TASK 2.1.3—AIR VOID SYSTEM....................................................................................... 115 

CHAPTER 4. SUMMARY....................................................................................................... 135

Introduction ............................................................................................................................. 135 

Early Setting and Excessive Retardation ................................................................................ 135 

Protocol ................................................................................................................................... 140 

Implementation Plan ............................................................................................................... 141 

ACKNOWLEDGEMENTS ..................................................................................................... 143

REFERENCES.......................................................................................................................... 145
iv 

LIST OF FIGURES 

Figure 1. Example plot with a strong relationship between data sets........................................... 58 

Figure 2. Example plot of data sets with little or no relationship................................................. 58 

Figure 3. A plot comparing sets of initial setting time measurements determined by 

different methods. ................................................................................................................... 59 

Figure 4. Correlation between initial and final set for concrete tests. .......................................... 60 

Figure 5. Correlation between initial and final set for paste tests................................................. 60 

Figure 6. Device used at NIST to lift the mold for the minislump test......................................... 67 

Figure 7. A plot of minislump data for mixtures tested in round 1. ............................................. 68 

Figure 8. A plot of minislump data for mixtures tested in round 2. ............................................. 71 

Figure 9. A plot of minislump data for mixtures tested in round 3. ............................................. 72 

Figure 10. A plot of minislump data for mixtures tested in round 4. ........................................... 73 

Figure 11. A plot of minislump data for mixtures tested in round 5. ........................................... 74 

Figure 12. A plot of minislump data for mixtures tested in round 6. ........................................... 75 

Figure 13. Stress growth measurement......................................................................................... 81 

Figure 14. Typical plots of yield stress versus time for accelerated, untreated, and 

retarded cementitious systems. ............................................................................................... 81 

Figure 15. A photograph of the rheometer used at NIST. ............................................................ 82 

Figure 16. Die set for squeezing pore solution from hardened cement paste specimens. ............ 85 

Figure 17. Pore fluid being collected from die set........................................................................ 85 

Figure 18. Equation. Solubility product of gypsum...................................................................... 86 

Figure 19. Equation. Ion activity product of gypsum. .................................................................. 86 

Figure 20. Equation. Pulse velocity. ............................................................................................. 90 

Figure 21. Compressive strength development........................................................................... 102 

Figure 22. Modulus of elasticity development. .......................................................................... 103 

Figure 23. Splitting tensile strength development. ..................................................................... 103 

Figure 24. Early age properties for mix WRA1.......................................................................... 105 

Figure 25. Early age properties for mix WRA2.......................................................................... 105 

Figure 26. Long-term properties for mix WRA1........................................................................ 106 

Figure 27. Long-term properties for mix WRA2........................................................................ 106 

Figure 28. Early age properties for mix FA1.............................................................................. 107 

Figure 29. Early age properties for mix FA2.............................................................................. 107 

Figure 30. Long-term properties for mix FA1............................................................................ 108 

Figure 31. Long-term properties for mix FA2............................................................................ 108 

Figure 32. Early age properties for mix 25FA90........................................................................ 109 

Figure 33. Early age properties for mix 4FA90.......................................................................... 110 

Figure 34. Long-term properties for mix 25FA90...................................................................... 110 

Figure 35. Long-term properties for mix 4FA90........................................................................ 111 
v 

Figure 36. Conduction calorimetry plot of paste system for mixture 25FA90 

conducted at 32 °C (90 °F). .................................................................................................. 112 

Figure 37. Early age properties for mix 25FA70........................................................................ 113 

Figure 38. Early age properties for mix 4FA70.......................................................................... 113 

Figure 39. Long-term properties for mix 25FA70...................................................................... 114 

Figure 40. Long-term properties for mix 4FA70........................................................................ 114 

Figure 41. Foam drainage procedure. ......................................................................................... 119 

Figure 42. Equation. Foam drainage........................................................................................... 119 

Figure 43. Equation. Percent drained.......................................................................................... 119 

Figure 44. Rating 0–No clustering present. Visual rating guide for analysis of air 

void clustering severity (PCA R&D Serial No. 2789).......................................................... 124 

Figure 45. Rating 1, Minor clustering Visual rating guide for analysis of air void 

clustering severity (PCA R&D Serial No. 2789).................................................................. 124 

Figure 46. Rating 2, Moderate clustering. Visual rating guide for analysis of air 

void clustering severity (PCA R&D Serial No. 2789).......................................................... 125 

Figure 47. Rating 3, severe clustering. Visual rating guide for analysis of air void 

clustering severity (PCA R&D Serial No. 2789).................................................................. 125 

Figure 48. Example of clustering rating for a cylinder............................................................... 126 

Figure 49. Correlation between pressure meter and AVA-generated fresh air contents. ........... 128 

Figure 50. Correlation of total air contents between pressure meter and ASTM C 457............. 131 

Figure 51. Correlation of total air contents between AVA and ASTM C 457. .......................... 131 

Figure 52. Correlation between AVA and ASTM C 457 generated spacing factors.................. 132 

Figure 53. Spacing factor versus air content relationship for ASTM C 457 and AVA.............. 132 

Figure 54. Reactions in hydrating cement. ................................................................................. 138 
vi 

LIST OF TABLES 

Table 1. Commercial portland cement characteristics used in Task 2.1.1.................................... 36 

Table 2. Oxide analyses of cements.............................................................................................. 37 

Table 3. Oxide analyses of supplementary cementing materials.................................................. 38 

Table 4. Particle size distributions of cementitious materials....................................................... 38 

Table 5. Tests conducted on paste systems in all rounds.............................................................. 41 

Table 6. Summary of paste and mortar data from round 1. .......................................................... 43 

Table 7. Summary of data from round 2....................................................................................... 45 

Table 8. Summary of data from rounds 3 and 4. .......................................................................... 47 

Table 9. Summary of all paste and mortar data. ........................................................................... 48 

Table 10. Test plan for early stiffening and normal concrete systems. ........................................ 51 

Table 11. Test plan for retarding and normal concrete systems. .................................................. 51 

Table 12. Physical properties of aggregates. ................................................................................ 52 

Table 13. Nominal concrete mix proportions (SSD). ................................................................... 52 

Table 14. Temperature, air content, unit weight, slump, and impedance results.......................... 54 

Table 15. Slump loss and mortar flow loss................................................................................... 55 

Table 16. Setting time, NDT, and semi-adiabatic cell results. ..................................................... 56 

Table 17. Minislump test data for round 1.................................................................................... 68 

Table 18. Minislump test data for round 2.................................................................................... 70 

Table 19. Minislump test data for round 3 and 4.......................................................................... 76 

Table 20. Minislump test data for investigating effect of w/cm. .................................................. 77 

Table 21. NIST test data for round 1. ........................................................................................... 78 

Table 22. NIST test data for round 2. ........................................................................................... 79 

Table 23. NIST Test Data For Round 3 and 4. ............................................................................. 80 

Table 24. Oxide analyses of cements............................................................................................ 93 

Table 25. Oxide analyses of supplementary cementing materials................................................ 94 

Table 26. Physical properties of aggregates. ................................................................................ 94 

Table 27. Concrete mixtures......................................................................................................... 95 

Table 28. Concrete mix proportions. ............................................................................................ 96 

Table 29. Fresh concrete properties.............................................................................................. 97 

Table 30. Setting time data. .......................................................................................................... 97 

Table 31. Results of ASTM ring tests........................................................................................... 98 

Table 32. Hardened concrete properties for mix WRA1. ............................................................. 99 

Table 33. Hardened concrete properties for mix WRA2. ............................................................. 99 

Table 34. Hardened concrete properties for mix FA1. ............................................................... 100 

Table 35. Hardened concrete properties for mix FA2. ............................................................... 100 

Table 36. Hardened concrete properties for mix 25FA90. ......................................................... 101 

Table 37. Hardened concrete properties for mix 4FA90. ........................................................... 101 
vii 

Table 38. Hardened concrete properties for mix 25FA70. ......................................................... 101 

Table 39. Hardened concrete properties for mix 4FA70. ........................................................... 102 

Table 40. Results of minislump tests conducted on 25FA90 pastes........................................... 112 

Table 41. Air entraining admixtures and related properties. ...................................................... 116 

Table 42. Cementitious materials composition and fineness...................................................... 116 

Table 43. Coarse aggregate grading............................................................................................ 117 

Table 44. Fine Aggregate Grading.............................................................................................. 117 

Table 45. Concrete test matrix used in stages 2 and 3 of subtask 2.1.3...................................... 122 

Table 46. Base concrete mixture................................................................................................. 123 

Table 47. Corresponding calculations for average clustering rate............................................. 126 

Table 48. Foam drainage results. ................................................................................................ 127 

Table 49. Fresh concrete properties............................................................................................ 129 

Table 50. Hardened concrete properties. .................................................................................... 130 

Table 51. Compounds of calcium sulfate in cement................................................................... 136 

1 

CHAPTER 1. INTRODUCTION 

OVERVIEW 

The objectives of this project were to develop practical test protocols and procedures with 

criteria in the following three areas to assess the effects of combinations of materials for concrete 

pavements: 

• Early stiffening and excessive retardation that can affect workability, placeability, 

consolidation, and finishing. 

• Potential for early-age cracking including plastic shrinkage; and possibly the ability 

to attribute the cause of cracking to chemical, physical, and environmental 

phenomena. 

• Characteristics of the air void system including nonuniformity, insufficient air, 

coalescence of air voids around aggregate, and excessive large voids, all of which 

influence strength or durability, or both. 

This study considered the following materials: 

• Portland cement and blended cements. 

• Fly ash, slag, silica fume, and other pozzolans. 

• Chemical admixtures. 

• Aggregates. 

The research also considered the following effects of production and placement methods: 

• Factors influencing segregation. 

• Bleeding and cohesiveness relative to finishability. 

• Influence of environmental conditions such as temperature and humidity. 

The developed procedures have been incorporated into guidelines for evaluating and qualifying 

combinations of materials for use in pavements. An implementation plan with recommendations 

and materials for dissemination of the information (e.g., technical summaries, presentations) 

appears in this volume in Chapter 4, Summary, and in Volume II. 

The protocol is phased to allow combinations of materials to be filtered through a set of 

relatively accessible tests. Potentially problematic combinations then can be subjected to more 

rigorous investigation. 

BACKGROUND 

Premature pavement distress can result from causes such as alkali-silica reactivity, D-cracking, 

and materials contamination, all problems that have been researched extensively and solutions 

are known. Other incidents of premature pavement distress have led to questions about the 
2 

ability of concrete pavement to achieve a desired service life.(1) Examples of these types of 

distress are early stiffening, poor consolidation, early-age cracking, and lack of proper air 

entrainment. Little is known about these early pavement distresses, mainly because of a lack of 

tests to determine the susceptibility of materials combinations to these distresses. 

Lack of compatibility among various cementitious materials and admixtures can lead to early 

stiffening, which could account for many other problems. The tendency to early stiffening may 

be attributed not only to the individual cementitious materials, but also to interactions among the 

various cementitious materials and the chemical admixtures. Early stiffening may be caused by 

excessive calcium sulfate in the form of hemihydrate (plaster) in the cement (false set) or the 

uncontrolled early hydration reactions of the tricalcium aluminate (C3A) (flash set). False set 

may be overcome by continued mixing of the concrete. Early stiffening is not reversible and 

leads to loss of workability. When concrete is hard to place, it is likely water will be added, 

which reduces both strength and durability and increases the potential for shrinkage and 

cracking. The addition of some admixtures improves workability without these negative effects, 

but the admixtures also add considerably to the cost of the concrete, and they may retard setting. 

Early stiffening depends on several factors, including C3A content and reactivity; alkali content; 

and the form, content, and distribution of sulfates in the cement. C3A hydrating in the presence 

of sulfate ions forms ettringite on its surface. The ettringite acts as a barrier, further limiting 

reactivity. If supplementary cementing materials, particularly Class C fly ash, contain aluminate 

phases, and the sulfate is not well distributed in the cement paste, the concrete may experience 

early stiffening. A balance among the ions in plastic concrete is necessary to prevent early 

stiffening. Some chemical admixtures, particularly Type A water reducers, may disturb this 

balance. 

Early stiffening can be deleterious to pavement performance. If the concrete cannot be 

thoroughly consolidated, loss of strength and durability can result, as well as early development 

of cracking and pavement failures.(2) If extraordinary consolidation efforts are used to achieve 

the required concrete density, the entrained air-void system may be altered, leading to decreased 

freeze-thaw durability.(3,4)

Cracking in concrete can also be caused by a host of factors. Shrinkage can occur in fresh or 

hardened concrete. The major cause of plastic shrinkage cracking is thought to be the tensile 

stress developed as water evaporates from the surface of the concrete, leaving the capillaries 

partially filled and creating a disjoining pressure caused by surface tension effects. The risk of 

cracking may be higher in concretes that exhibit early stiffening because the mix does not remain 

fluid long enough to allow a layer of bleed water to remain on the surface. While bleeding is 

generally thought of as detrimental to concrete, bleeding may also have some benefit with 

relation to the potential for plastic cracking: drying of the surface cannot occur if it is covered 

with bleed water. Precautions to prevent plastic shrinkage cracking include (1) strict adherence to 

specifications regarding evaporation rates and cessation of concrete placement if relative 

humidity is low and temperatures and wind speeds are high, (2) use of fog sprays, and (3) use of 

evaporation retarding admixtures during and immediately after finishing. 
3 

Cracking can also occur because of autogenous shrinkage, drying shrinkage, thermal effects, and 

external loads. Cracking occurs when and where the maximum principal tensile stress exceeds 

the tensile strength of the concrete. 

A number of paving projects have experienced problems related to use of synthetic air-entraining 

agents resulting in accumulations (coalescence) of air voids around the aggregate particles. In 

addition to this problem, the quality of the air void system in the hardened concrete continues to 

be a matter of concern. The spacing factor and specific surface are the main parameters of the 

concrete air void system that indicate the ability of the concrete to resist the damaging effects of 

frost. In recent years, it has been observed that marginal air void systems may result from 

incompatibility between certain water reducers and air-entraining agents. 

STUDY GOALS, OBJECTIVES, AND SCOPE 

The primary goal of the study was to develop reliable tests or standards to predict potential 

incompatibility of concrete materials that adversely affect the properties of concrete at early 

ages. The availability of such tests and standards will allow material suppliers, concrete 

producers, and users to identify undesirable material combinations so that use of marginal 

concrete for paving can be avoided. A secondary goal of the study was to understand the 

mechanisms behind the observed behaviors. 

Following is a list of the specific objectives for the research in this project: 

• Develop or refine test procedures that can be used to evaluate the potential of 

materials and combinations of materials to contribute to early stiffening in concrete 

pavement mixtures. After test procedures are refined, develop test protocols and 

guidelines for evaluating job materials using the proposed procedures. 

• Develop or refine test procedures that can indicate the potential for cracking of 

concrete mixtures including plastic shrinkage cracking and cracking resulting from 

restraint of drying shrinkage and temperature shrinkage. Develop test protocols and 

guidelines. 

• Develop or refine tests to determine characteristics of the air void system in concrete, 

preferably while the concrete is still fresh. 

A suite of phased tests has been developed into a protocol of relatively simple tests to assess the 

potential for incompatibility in a given set of concrete materials. If the results of these tests 

indicate possible problems, a more sophisticated set of tests can then be applied to more firmly 

establish the risk of problems and possible remedial actions. 

Following is a list of components in the scope of this project: 

• Conduct a literature review. 

• Conduct the research in accordance with the approved work plan. 
4 

• Develop guidelines and test protocols for identifying the effects of incompatible 

concrete materials. 

• Submit a final report documenting the work performed. 

• Develop a comprehensive implementation and technology transfer plan. 
5 

CHAPTER 2. LITERATURE REVIEW 

GENERAL 

An extensive review of literature was conducted pertinent to the three areas of interest—early 

stiffening and retardation (rheology), premature cracking, and air void systems in concrete. The 

review focused on the following three objectives: 

• Identify the extent of field problems and various manifestations of these problems. 

• Determine if material incompatibility was the identified or suspected cause of these 

problems. 

• Review test procedures identifying concrete material incompatibility. 

In addition to the literature review, the study included a survey of highway officials, technical 

support staff from cement companies, and field office staff from the American Concrete 

Pavement Association (ACPA) to collect information on highway paving projects that was not 

reported in the literature. The following section summarizes responses and discusses construction 

materials and practices that may result in premature failures or unacceptable pavement and 

specific findings related to concrete rheology, premature cracking, and air void systems. A 

discussion on construction materials and practices distinguishes problems related to individual 

materials and construction practices from the problems related to use of incompatible materials. 

NEED FOR INFORMATION REQUEST RESPONSES 

The following field problems were reported in response to a request for field experience 

information: 

• Excessive void system caused by angular fine aggregate movement during placement 

and finishing operations. 

• Longitudinal joint deterioration attributed to poor air void systems. 

• Premature cracking in pavements, prestressed elements, and bridge decks, possibly 

related to incompatibility among admixtures, Class C fly ash, and cements. 

• A mix exhibiting retardation attributed to incompatibility between the cement and 

water reducer, causing the no set in the concrete and cracking. The problems 

occurred in both cool and warm weather and disappeared with a change in the water 

reducer. 

• Serious retardation in concrete that contained low-alkali Type I cement and 

30 percent Class C fly ash. One Type-A lignosulfonate water reducer was used at a 

dosage of 2 ounces (59 milliliters) per 100 pounds (45 kilograms) of cement. 
6 

Testing indicated that the effect of the admixture on cement hydration was an 

important factor. 

• Excessive slump loss and air loss within about 15 min at a paving site during 

November 2000. The concrete mix used 350 kilograms per cubic meter (kg/m3) 

(517 pounds per cubic yard (pcy)) of cement and no fly ash. The slump and air loss 

at the project and in the laboratory were attributed to the cement. 

• Early stiffening problems such as excessive slump loss from the plant to the paving 

train resulted in poor strength results from field cast specimens. The water reducer 

used had no beneficial effect on the workability of the cement-Class C fly ash blend 

paste and, in fact, resulted in early stiffening. A change in the chemical admixtures 

was found to be effective. 

• Material incompatibility may have caused some of the problems attributed to 

requirements for smoother pavements, high production placement, use of Class C fly 

ash, poor mixing cycles, and poor air void system. 

• Early transverse shrinkage cracking in a concrete pavement and cracking were 

observed adjacent to several transverse joints during joint sawing. The early cracking 

was attributed to a retarded mix, possibly caused by overdosing the water reducer. 

The problem was corrected by increasing the cement content to 60 percent and 

reducing the slag and fly ash components to 30 percent and 10 percent, respectively. 

• Low strength and air void clustering were observed frequently in one construction 

season. The problem was attributed to a lack of cement dispersion (measures to 

ensure effective dispersion of cement, use of water reducers, proper mixing action, 

and use of vinsol resin to achieve necessary air in relatively stiff mixes), cement 

composition (use of high dosage of air-entraining agent with low alkali cement), 

aggregates (use of blended aggregates and higher amount of fine aggregate to 

achieve required air void characteristics), and ambient temperature (routine use of 

water reducers and retarders under high ambient temperature conditions minimizes 

retempering the concrete with water when slump loss occurs). Clustering of air voids 

and low compressive strength can occur when concrete is retempered with water. 

• Excessive slab warping and curling were observed in a pavement. A task force is 

looking at ways to specify reduced concrete shrinkage. 

• Air void stability on a project where low alkali cement was used with high dosages 

of air-entraining admixtures. 

CONSTRUCTION MATERIALS AND PRACTICES 

A survey of highway officials, technical support staff from cement companies, and field office 

staff from ACPA collected information on highway paving projects not reported in the literature. 

The survey also provided insights into current construction practices. The Pooled Fund Study, a 

statistical analysis of the histories of pavements in several States, provided additional 
7 

information about combinations of materials and practices associated with premature 

deterioration.(5) The association between materials and practices on one hand and poor 

performance on the other was generally anecdotal from the people surveyed and statistical from 

the Pooled Fund Study. 

Construction Materials 

Class C Fly Ash 

Jennings et al. cited the use of Class C fly ash as one of the factors most strongly associated with 

pavement deterioration.(5) Numerous respondents to the informal survey also implicated Class C 

fly ash as the cause of premature deterioration. One State highway department no longer allows 

the use of fly ash in highway pavements because of this association. The exact causes of 

problems associated with certain combinations of portland cement and Class C fly ash are not 

known; however, the possibilities include available alkalis, CaO, and aluminates.(1) Free lime 

increases water demand, contributing to the loss of workability of the fresh concrete. Alkalis, 

CaO, and aluminates all affect setting. Alkalis accelerate the hydration reactions of the 

cementitious materials. Cement contains sulfates to control the hydration of the aluminates; 

however, if fly ash is added at the batch plant, the sulfates in the cement may not be sufficient to 

control the hydration of the additional aluminates from the fly ash. Several respondents to the 

survey associated the combination of Class C fly ash and hot weather placements with early 

stiffening. 

Cement 

Alkalis in fresh concrete accelerate the hydration of the cementitious materials, and thus the 

setting of the concrete, making it difficult to place and consolidate the concrete. In addition, the 

loss of slump causes a loss of entrained air. Jennings et al. correlated incidents of premature 

deterioration with alkali contents of the cementitious materials.(5)

Sulfate is added to the cement to control the hydration of the aluminates (C3A) to prevent early 

stiffening. The department of transportation in one State limits the sulfate content of the cement 

to a maximum of 3 percent, regardless of the C3A content. The ASTM C 150 (2004) 

specification sets maximum sulfate contents of 3 percent for Type I cements with C3A contents 

up to 8 percent, and 3.5 percent for contents exceeding 8 percent. The specification allows higher 

sulfate contents provided that the mortar-bar expansion (ASTM C 1038) remains below 

acceptable limits. Lower limits set by some departments of transportation may result in cements 

in which control of the hydration of the C3A is only marginal. Additional aluminates from 

supplementary cementing materials would only increase the possibility of early stiffening. 

Aggregate Grading 

In a well-graded aggregate, the smaller particles efficiently fill up the spaces between the larger 

particles so that the void space remaining is minimized. Gress also emphasized the importance of 

using the largest maximum aggregate size compatible with other requirements.(1) A continuous 

uniform aggregate grading minimizes the content of cement paste, which in turn minimizes the 

cost of the concrete, the heat of hydration, the volume of entrained air required to achieve an 

acceptable air void system, and the shrinkage of the hardened concrete. With a poorly graded 
8 

aggregate, the concrete is difficult to mix, place, consolidate, and finish. Aggregates with 

insufficient fines may result in excessive bleeding. 

Sometimes only poorly graded aggregates are available, or the larger aggregate particles must be 

removed because they are subject to D-cracking. In that case, adjustments must be made to the 

mix design to compensate. These adjustments may include increasing the quantity of cement, 

using supplementary cementing materials, and increasing the volume of entrained air. 

Construction Practice 

Concreting in Hot Weather 

Hot weather or high placement temperatures were cited by several respondents to the survey, as 

well as by Jennings et al.(5) Because the construction season spans the summer months, hot 

weather placements are unavoidable. In times of high demand for cement, it is shipped 

immediately after it is produced, still warm from the plant, increasing the temperature of the 

concrete. Elevated mix temperatures make mixing, placement, consolidation, and finishing more 

difficult. Loss of slump is associated with loss of entrained air. Rapid hydration of the cement 

increases the rate of heat evolution. Thermal gradients within the concrete may cause early 

cracking. Hot windy weather may result in plastic shrinkage cracking. The rapid loss of slump 

may tempt the crew to add water to the concrete, reducing strength and durability and increasing 

the risk of air void agglomeration. Increasing mix temperatures means that additional airentraining admixture will be required to achieve the same air content. 

Mixing 

If concrete is mixed briefly and subsequently not remixed, it may exhibit stiffening known as 

“brief mix set.”(6) Several survey respondents mentioned very short mixing times as a potential 

cause of early pavement distress. The low slumps (typically 1 inch or less) of today’s pavement 

concretes would make them difficult to mix thoroughly. Air-entraining admixtures need 

sufficient time to develop an adequate air void system. Because most pavement concretes are 

transported to the site in dump trucks, the only mixing they receive is at the central batch plant. 

Whiting and Nagi found greater variations in air content with short mixing times, and 

recommended that concrete be mixed at least 75 seconds (s) to obtain an adequate air void 

system.(7)

Delays in Placement 

Long haul times or delays in placement also contribute to the loss of entrained air. Whiting and 

Nagi reported that the loss of air content is typically 0.5 to 1 percentage points per hour, but that 

the rate of loss is greater for air contents higher than 6 percent.(7) When concrete is transported to 

the site in nonagitating trucks, the loss of air content ranges from 1 to 4 percentage points, 

depending on the haul time and consistency of the concrete. Placement techniques also can cause 

loss of air content. Whiting and Nagi recommended that the exact loss for equipment and 

techniques be established by test to compensate for the loss of air. One survey respondent cited 

this practice as a remedy for low air contents in the pavements in his State. 
9 

Vibration 

Vibration to consolidate the concrete also can result in loss of air, as seen in vibrator trails along 

the length of the pavement. Stutzman found that the air void systems of deteriorated pavements 

were worst in the vibrator trails.(8) Stark found that higher vibration frequencies had the most 

pronounced effect.(3) Concretes with low water-to-cement ratios (w/c) lost less air than those 

with higher w/c. Resistance to frost damage was related to both spacing factor (thus vibration) 

and w/c. Simon et al. also found that near the vibrator, the total volume of air was reduced by 

removal of the entrapped air and a portion of the entrained air, which was not necessarily 

detrimental to frost resistance.(9) Whiting and Nagi recommended that for slip-form paving, 

vibration frequency should be limited to 8,000 vibrations per minute (vpm) for paver speeds 

greater than 0.9 m/min (3 ft/min), and frequencies should be reduced for lower speeds.(7)

Tymkowicz and Steffes identified excessive vibrator frequency at 12,000 vpm in one project, 

and excessive vibration locally when the paver speed was reduced to half that of normal with a 

vibrator frequency of 8,000 vpm.(4) Two survey respondents indicated that vibration frequencies 

are monitored continuously in their States. 

Control Joints 

Concrete is subject to drying shrinkage and thermal expansions and contractions. A pavement 

slab will crack when such contractions occur unless contraction joints (also known as control 

joints) are provided as appropriate. Kosmatka et al. indicate that control joints should extend to a 

depth of one-fourth of the slab thickness.(10) Control joints may be formed in the fresh concrete 

with hand groovers or by placing strips of wood, metal, or preformed joint material at the joint 

locations. Control joints also may be cut into the concrete as soon as it is strong enough to resist 

damage from the saw blade, usually 4 to 12 h after the concrete hardens. Supplementary 

cementing materials generally slow the early strength gain of the concrete. Thus, they may 

necessitate longer waits before the joints can be cut. Four of the survey respondents reported 

cracking resulting from delayed or improper cutting of control joints. 

Curing 

Curing provides the conditions of moisture and temperature that allow the concrete to develop 

strength and water-tightness. Senbetta and Malchow(11) found that proper curing could increase 

the abrasion resistance of concrete by 50 percent or more compared to air-drying. When curing 

cannot be applied sufficiently early, plastic shrinkage cracking may develop. It is essential to 

prevent moisture loss (e.g., by fogging, monomolecular layer, or—after finishing—application of 

a curing compound). Effective curing methods reduce the rate and magnitude of early shrinkage. 

For paving projects, the most practical method of curing is the application of a membraneforming curing compound. These compounds prevent loss of water from the concrete. 

FINDINGS ON RHEOLOGY, CRACKING, AND AIR VOID SYSTEM 

Many practices in the construction of highway pavements are less than ideal. Placement during 

hot weather, short mixing times, transport in nonagitating trucks, excessive or insufficient 

vibration, and poor timing of control joint sawing all contribute to unsatisfactory performance. 

Some materials and combinations of materials are more sensitive to these practices than others. 
10 

In particular, combinations of cement with Class C fly ash and cementitious materials with 

chemical admixtures have the potential for incompatibility, leading to early stiffening, increased 

cracking, and inadequate air void systems. The information collected on these issues is 

highlighted in the following paragraphs. The test program discussed later takes into account the 

findings from the literature review and the conditions encountered in pavement construction. 

Rheology Findings 

The workability of fresh concrete is defined as the ease and homogeneity with which concrete 

can be mixed, placed, consolidated, and finished. Concrete loses workability, consistency, and 

other attributes with time. The rate of this loss is of paramount interest in paving because the 

concrete is usually mixed at the plant and transported to the site in nonagitating trucks. 

Interactions between concrete constituents can contribute to loss of workability. 

Cementitious Materials and Early Stiffening 

When slump loss is so rapid as to interfere with the normal placing and finishing of concrete, it is 

often described as “early stiffening.” The stiffening of concrete could result from either the 

excessive amounts of calcium sulfate as hemihydrate (plaster) in the cement (false or plaster set) 

or the uncontrolled early hydration reactions of the aluminate component (early stiffening or 

“flash set”). False set is generally associated with short concrete mixing times and delivery 

without subsequent agitation. Although false set can be overcome by continued mixing of 

concrete through the stiffening phase, stiffening caused by inadequate control of aluminate 

hydration is not recoverable. Early stiffening is encountered more frequently in the presence of 

water-reducing and set-controlling admixtures. 

Two ASTM standard test methods, ASTM C 451 and C 359, are intended to identify the early 

stiffening behavior of portland cement. 

Depending on the chemistry of the system, the severity of false set or early stiffening may vary. 

Dehydration of the gypsum during milling may result in severe false setting. Hansen provided an 

extensive discussion of false set in portland cement. Lost plasticity is often regained on further 

mixing.(12)

Early stiffening depends on several factors. The form, size, distribution, and type of sulfate 

source control the release of sulfate ions in the pore solution. A balance is usually achieved 

through the reaction between the sulfate ions and C3A. Although this reaction controls the 

reactivity by forming ettringite around the C3A grains, analysis of the cement oxide composition 

does not provide any information on sulfate solubility characteristics of a cement.(13)

A proper C3A-sulfate control is critical to hydrating cement paste and the performance of 

admixtures addition.(14) Improper aluminate control typically results in poor admixture 

efficiency, workability loss, and reduced strength. Wadso demonstrated the use of a multichannel 

conduction calorimeter for detecting cement-admixture incompatibility and to quantify 

retardation in hydrating cements in the presence of added sulfates and chemical admixtures.(15)

He concluded that this device was efficient, easy to use, and required small size samples. 
11 

Marginally controlled and sometimes uncontrolled cements are sometimes encountered. 

Uncontrolled cements exhibit early stiffening tendencies even in the absence of admixtures. 

Marginally controlled cements generally do not exhibit abnormal stiffening behavior in the 

absence of chemical admixtures; however, in the presence of admixtures, the delicate balance 

between the soluble sulfate and C3A may be disturbed. Well-controlled cements in general 

exhibit improved workability in the presence of water-reducing admixtures. 

Water-reducing admixtures improve workability through the absorption of organic molecules on 

the surface of cement particles, reducing the interparticle forces and increasing dispersion. While 

the sugar content of the lignin-based, water-reducing admixtures may result in set retardation and 

air entrainment, a higher dosage of water-reducing admixtures may also affect strength 

development.(16) Type F high-range water-reducing admixtures have less effect on cement 

hydration and setting. The occurrence of cement-admixture incompatibility with high-range 

water-reducing admixtures is less than with water-reducing admixtures. In some combinations of 

cement with high-range water-reducing admixtures, severe slump loss has been encountered at 

higher dosages.(16) Because high-range water-reducing admixtures generally are not used in 

paving concrete, emphasis is given in this project only to water-reducing admixtures. In many 

cases, the incompatibility between some cements and water-reducing admixtures can be 

overcome by delaying the addition of the admixture by as little as half a minute. In some cementadmixture combinations, air-entraining admixtures may lead to early stiffening. 

Supplementary cementing materials such as fly ashes and ground, granulated blast-furnace slag 

may also affect stiffening. Fly ash may contain reactive aluminate phases such as C3A and 

Klein’s compound (calcium sulfoaluminate), which may not be adequately controlled by the 

sulfates in the cement. If there is an incompatibility, the stiffening can be severe. Slag generally 

does not contain any such fast hydrating phases; however, jagged slag particles may reduce 

workability. On the other hand, fly ash may improve workability.(17,18)

False setting, if not overcome by remixing, and early stiffening of concrete, may affect the 

performance of concrete in the plastic and hardened states. If concrete is mixed briefly, and it is 

not remixed subsequently, it may also stiffen. This stiffening is also known as “brief-mix-set,” 

which is different from early stiffening.(6) When cement incompatibility leads to stiffening, the 

water demand increases. The problems generally associated with early stiffening are related to 

workability, bleeding, setting time, and finishability of the plastic concrete. Subsequently, 

strength development and durability of the hardened concrete are also affected. For paving 

concrete with slump less than 50 mm, the incompatibility may cause inefficient consolidation, 

which may lead to honeycomb and lower strengths. In addition, durability may also be affected 

because the air content and the spacing factor may be adversely affected.(16)

Incompatibility between Materials 

Incompatibility between materials may arise from chemical and physical causes. When the 

incompatibility is of chemical origin, it is generally caused by some combination of cement, 

supplementary cementitious materials, and chemical admixtures, often at elevated temperatures. 

Physical incompatibility may arise from the mix proportions of the concrete. For example, a 

cement with normal setting characteristics may show stiffening behavior depending on the 

amount of cement and the type of aggregates used.(19) When chemical incompatibility is 
12 

combined with physical incompatibility, the early stiffening behavior may be compounded. 

Chemical incompatibility may be evaluated in cement paste and physical incompatibility in 

concrete. The paste can be evaluated before testing the concrete for physical incompatibilities. 

The concrete can be tested both at the plant and in the field, providing quality control measures 

before and during the paving job. 

Techniques to Measure Workability of Cement Paste and Concrete 

Workability of concrete is most indicated by slump; however, if the slump is less than 50 mm, 

measurement of workability loss will lack the precision needed to diagnose incompatibility. In 

recent years several researchers applied rheological principles and methods to concrete for better 

characterization of the concrete workability. Rheological measurements determine the 

relationship among shear stress, shear strain, and time. For a simple (Newtonian) liquid, the 

shear stress is directly proportional to the shear rate, and the constant of proportionality is called 

the “coefficient of viscosity.” A Bingham fluid flows only when a certain shear stress is 

overcome, after which it flows at constant rate with increasing shear rates. This rate, or the slope 

of the curve, is called “plastic viscosity.”(20) In general, concrete exhibits a behavior similar to 

that described by the Bingham model. 

Rheological Evaluation of Cement Paste System 

Kantro developed a minislump cone test as a rapid, simple method for evaluating the influence of 

water-reducing admixtures on the workability of neat cement paste.(21) A high-intensity mixer is 

used to make cement paste that is rheologically similar (i.e., comparable shear history) to that 

found in a typical concrete mix.(19,22) Researchers familiar with the minislump test routinely use 

the mixing protocol developed by Helmuth(22) and Tang and Bhattacharja(19) to evaluate cement 

paste rheology.(18,23) To predict the behavior of concrete, the cement paste should be mixed with 

high shear. (See references 18, 19, 22, 23.) 

Ferraris and her collaborators have been evaluating cement paste using viscometers with parallel 

plate geometry.(18,23,24) Rheology of concrete depends on the gap between the aggregates, and 

parallel plate geometry allows them to vary the gap to simulate different interaggregate spacings 

in concrete. The interaggregate distance modifies the shear environment during concrete mixing, 

and it depends on the volume of the paste fraction. To avoid slippage, the faces of the parallel 

plate rheometer used by Ferraris and coworkers were serrated. Parallel plate rheometers are 

commonly used in asphalt laboratories at State departments of transportation (DOTs), 

commercial asphalt testing facilities, and asphalt concrete contractors. With some modification 

of the software and perhaps the hardware, this viscometer can be used to evaluate cement paste 

rheology. 

Rheological Evaluation Methods 

To test the flow characteristics of concrete, it is necessary to apply shear stress. The schemes that 

have been used to generate shear stress in the existing methods can be divided into four 

categories: (1) free flow, (2) free flow under confinement, (3) rotational, and (4) vibrational.(20)

These rheometers and the associated physical principles have been discussed at length by 

Ferraris et al. (18,25) and Wong et al.(26) The stiffness of concrete commonly used in pavement 
13 

applications is far above the application range of rheometers. The limitations of these rheometers 

have been discussed in several papers. (See references 18, 25, 27, 28.) Vibration has been used to 

test concretes with stiffness similar to that used for pavements. Some of these are Ve-Be time or 

remolding test (ASTM C 1170), and vibrating slope apparatus.(26) Vibration is commonly used 

during paving operations, and the concrete flows when the vibrational force transferred exceed 

the yield stress of the concrete. 

Even though vibration makes it flow, low-slump paving concrete cannot be assumed to behave 

like a fluid. The calculation of a plastic viscosity from measurements taken under vibration is 

complex. Vibration also alters the rheological characteristics to such an extent that the behavior 

of vibrated concrete is very different from that of unvibrated concrete.(29) Only one rheometer is 

capable of measuring the rheological parameters while concrete is vibrated.(30) Because only a 

limited number of tests using vibration were performed with this instrument, the results may not 

correlate with field performance. 

Thermal Methods for Evaluating Cement-Admixture Incompatibility 

A proper aluminate control is critically related to the performance of admixture in the early age 

behavior of hydrating cement paste. Insufficient aluminate control often results in reduced 

admixture efficiency, loss of workability, and poor strength development. Cement-admixture 

interaction is often complicated and difficult to predict by current standards. Sandberg and 

Roberts reviewed the application of isothermal calorimetry for cement hydration related to 

aluminate-sulfate interaction in the presence of admixtures.(14) They found the heat signatures to 

be suitable for observing the hydration characteristics of combinations of additional soluble 

sulfates, supplementary cementing materials, and chemical admixtures. 

Earlier, Wadso (2004) also demonstrated the use of conduction calorimetry as a convenient 

method for detecting cement-admixture incompatibility and to quantify retardation in hydrating 

cements in the presence of added sulfates and chemical admixtures.(15) The calorimeter used was 

designed to have multichannels for simultaneously testing 14 samples of cement pastes and 

mortars. This device had advantages over the semi-adiabatic calorimeters because it requires 

small-size samples, effectively makes use of the heat released, and is easier to use. 

Early Stiffening Tests 

Cement Paste Tests 

To diagnose incompatibility, the rheological measurements should be performed on cement 

pastes similar to those found in a typical concrete mix. This will require high-shear mixing of 

cement paste under controlled temperature conditions. Cement paste rheology can be tested 

using either parallel plate or coaxial cylindrical viscometer. Both perform reasonably well for 

cement paste. 

Although parallel plate viscometers are generally available at DOT laboratories, the coaxial 

cylindrical viscometer is very common. During experimental development, the gap in the parallel 

plate viscometer may be modified to simulate the interaggregate spacing between aggregates. 

For industry to use such a method, the gap must be standardized to avoid any misleading results 

and conclusions. The gap between the spindle and cup in a coaxial cylindrical viscometer is 
14 

generally not varied. To minimize the effect of bleeding, a parallel plate viscometer is used with 

lower w/c ratios. Some chemical admixtures and supplementary cementing materials may 

increase bleeding, which may interfere with the rheological measurements. This is of less 

concern for a coaxial cylindrical viscometer, but the results can still be influenced by a 

concentration of particles at the bottom of the container; nevertheless, these two well-established 

rheological tools are best suited to evaluate cement paste. 

Concrete Tests 

In paving operations, concrete is generally mixed in a batch plant and transported to the job site 

in a dump truck. If concrete suffers from false set or plaster set, the little agitation generated 

during transport and dumping may not be adequate. During unloading at the job site, the 

agitation may be adequate to regain some plasticity, but the concrete is likely to lack uniformity. 

After unloading, the concrete sits idle until the paver reaches it. The concrete is thoroughly 

agitated when the paver passes it through the auger. At this stage, the agitation is adequate, and 

false setting concrete may regain its plasticity. Considering this sequence of paving operations, 

false set appears not to be a problem. The stiffening behavior becomes an important issue if the 

concrete cannot be properly consolidated even with vibration. 

Because vibration is always used for placement and consolidation of pavement concrete, 

concrete that does not achieve the desired quality under these conditions must be identified. The 

effect of combinations of the vibrational parameters (frequency and amplitude within the range 

practiced in the field) on the consolidation characteristics of concrete must be evaluated. If a 

concrete cannot be consolidated within the available range of vibrational parameters, it may be 

identified as early stiffening. 

A concrete testing techniques that appears appropriate for paving concrete is the vibration testing 

apparatus, in which remolding or consolidation characteristics of the concrete are measured.(31)

The settlement of the concrete is measured from the loss of concrete height as a function of 

vibration time. 

Cracking Findings 

In several reported cases of cracking in pavement concrete, incompatibility between two or more 

of the concrete ingredients contributed to cracking. In other cases, the influence of other factors 

such as weather, design factors, and construction practices caused, or at least contributed to, the 

cracking. It is not always appropriate to examine these factors in isolation because a particular 

combination of ingredients may work well at some temperatures and not in others. Also, a 

particular combination of materials may be more sensitive to construction variables such as 

mixing time or curing practices. 

Importance of Cracking 

Permeability of concrete is the key to durability. One of the most important strategies in 

protecting concrete from the action of aggressive agents is not to prevent deterioration (which 

may be impossible), but to retard it by limiting the ability of these agents to enter the concrete. 

Cracking dramatically increases permeability. Aldea et al. measured the permeability of concrete 

loaded under controlled conditions and found that the coefficient of permeability increased with 
15 

increasing crack width by several orders of magnitude.(32) While concrete having cracks less than 

100 micrometers (μm) (0.004 inch) wide exhibited a decrease in permeability over time, the 

permeability of concrete with cracks 200 μm (0.008 inch) or higher remained unchanged. 

Early cracks widen over time because of mechanical- and environment-induced stresses. The 

cracks become channels for the ingress of water and other harmful species; therefore, minimizing 

early cracking is important to the service life of the concrete. Chatterji identified four 

mechanisms responsible for cracking in concrete at early ages: (1) differential plastic shrinkage, 

(2) self desiccation, (3) desiccation, and (4) temperature differences between the interior and 

surface concrete.(33) Frequently the conditions that give rise to one of these mechanisms also 

favor another, and the combined effect is greater than the sum of individual effects. 

Springenschmid et al. pointed out that cracks do not occur because of high temperatures, but 

because of the thermal stresses caused by the heat of hydration and the restrained deformations 

of the concrete.(34) In addition, strains unrelated to thermal effects (for example, self desiccation) 

often have an important influence. Springenschmid and Breitenbücher cited two parameters that 

must be considered in the assessment of cracking potential:(35)

• Cracking sensitivity of a concrete mix that depends on constituents, mix 

composition, and fresh concrete temperature. 

• Boundary conditions (dimensions of a member, degree of restraint, temperatures). 

Cracking from Autogenous, Plastic, and Drying Shrinkage 

When the evaporation rate is higher than the rate of bleeding, the air-water interface penetrates 

into the concrete. Capillary menisci form, compressing the concrete mix and causing plastic 

shrinkage. Because of differential rates of plastic shrinkage in different parts of a concrete 

section, cracks appear. Plastic shrinkage cracking can be avoided by preventing the formation of 

menisci, that is, by preventing the evaporation of water from the surface.(33)

Long before cracks are visible, extensive microcracking occurs even on relatively mild drying. 

Drying can occur even in cold temperatures if the concrete temperature is considerably warmer 

than the ambient temperature. With the passage of cold air over the warm surface, air 

temperature is raised, lowering the relative humidity. The reduction in relative humidity dries the 

concrete surface, possibly enough to cause cracking. In this situation, covering the concrete with 

a plastic sheet prevents evaporation without affecting the thermal behavior(33) Powers et al. 

subjected hydrated cement paste specimens to extended drying at 93 percent relative humidity 

(RH), followed by further drying at 79 percent RH and then resaturation.(36) They found that the 

water permeability of these specimens increased by a factor of about 70 compared with 

companion specimens, which were never dried. Chatterji(33) attributes this behavior to the 

formation of microcracks in the paste on drying. 

Krauss and Rogalla found that drying shrinkage could be reduced by reducing the total paste 

volume and the water content, maximizing the aggregate volume, using Type II cement, and 

using an aggregate with low shrinkage.(37) They also found that extended moist curing does not 

necessarily decrease the total shrinkage, but may reduce the rate of shrinkage. 
16 

During the hydration of cement, the volume of the cement paste decreases. The change in 

volume depends on the original w/c and the degree of hydration. Continued hydration after the 

concrete sets can result in self-desiccation, in some cases causing cracks even before forms are 

removed.(33) Holt emphasized the importance of early-age shrinkage in the development of 

cracks.(38) Standard test methods measure the shrinkage of concrete from an age of 24 hour (h) 

onward. However, Holt reported that shrinkage in the first 24 h might exceed all shrinkage that 

takes place after that time. 

Heat of Hydration and Thermally-Induced Cracking 

Traditionally, temperature differences between surface and interior have been limited to 

minimize the stresses (and cracking) due to thermal gradients. However, as Bernander pointed 

out, “there is no generally valid proportionality between temperature difference and stress.”(39)

Stress calculations which take into account the nonuniform development of maturity in the 

concrete at different locations within a section show that the assumption of a linear relationship 

between the temperature distribution and the resulting stress distribution is simply not valid. 

However, in practice the assessment of risk of cracking is often based solely on temperature 

criteria. 

Initially, the heat of hydration of the cement generates thermal expansion in the concrete. 

However, at early ages the modulus of elasticity is low, so that the restraint of this expansion 

does not generate significant compressive stresses. In addition, such compressive stresses that do 

develop are reduced by a high degree of relaxation. By the time the concrete cools off, the 

modulus of elasticity increases and the tendency to creep reduces, so that the tensile stresses 

generated by the restraint of thermal shrinkage are higher to begin with and do not relax as 

much.(35)

Thermal cracks may appear either in the heating or the cooling phase after the concrete is placed. 

Very early cracks that appear during the heating phase tend to close at the end of the cooling 

period. These cracks are generally surface cracks, which may or may not adversely affect 

performance. Cracks that occur in the cooling phase generally extend through the thickness. 

Depending on the geometry and the environmental conditions, these cracks may appear weeks, 

months, or even years after placement.(39)

Bernander recommended the use of cement with a low cracking sensitivity.(39) When this 

property cannot readily be determined, the use of low heat cements would be appropriate. In 

addition, the cement content can be reduced by the use of water reducers (which reduce the 

amount of paste required for good workability), replacement of some of the cement by 

supplementary cementing materials, and the use of a large maximum size of aggregate. In hot 

weather, Krauss and Rogalla recommended avoiding placement temperatures greater than 27 °C 

(80 °F), maintaining the placement temperature of the concrete at least 11 °C (20 °F) lower than 

ambient, placing the concrete during late afternoon or evening rather than morning or early 

afternoon, minimizing solar radiation during placement, and allowing lower early strengths by 

specifying 56- or 90-day strengths.(37)
17 

Factors Affecting the Tendency of Concrete to Crack 

Analytical studies performed by Krauss and Rogalla showed that the modulus of elasticity of the 

concrete, adjusted for the effects of creep, affects both thermal and shrinkage stresses more than 

any other property of concrete.(37) The higher the modulus of elasticity, the higher the stresses 

associated with a given thermal or shrinkage strain. The use of aggregates with low modulus of 

elasticity, increased paste contents, and reduced concrete strengths would all reduce the modulus 

of elasticity of the concrete. These measures would also increase the total shrinkage. 

Krauss and Rogalla recommended the following measures to reduce the tendency of concrete to 

crack: low modulus of elasticity at early ages; low early strength; high early creep; low cement 

content; good quality, low-shrinkage aggregates; low hydration temperatures; pozzolans with 

low heat of hydration; low coefficient of thermal expansion; minimum paste volume and free 

shrinkage; Type II cement; shrinkage-compensating cement.(37) The use of fine cement, silica 

fume, and other admixtures that give high strength and modulus of elasticity should be avoided. 

Springenschmid and Breitenbücher summarized the relative effectiveness of measures that might 

be taken to reduce the tendency of concrete to crack.(35) Following the European practice, these 

are quantified in terms of their effects on the cracking temperature of the concrete. Measurement 

of the cracking temperature is described below. Simultaneous use of more than one of these 

measures generally results in effects that are less than the sum of the individual effects. Both the 

net effectiveness and the costs must be evaluated case-by-case. Springenschmid et al. considered 

it unreasonable to specify the maximum cracking temperature acceptable for a concrete.(34)

Rather, the measures required to prevent cracking should be specified. 

As Bernander pointed out, measures designed to avoid early-age cracking are directed primarily 

toward reducing the cement content. Such measures may jeopardize the mentioned materials 

requirements with regard to strength and durability.(39) As these requirements may vary with type 

of structure and environment, different measures for controlling cracking are necessary. The 

selection of a specific strategy for control of cracking in a given project will depend on the 

associated costs and benefits. 

Construction Variables. The tendency of concrete to crack increases with the placement 

temperature of the fresh concrete. Springenschmid and Breitenbücher cited two reasons for this: 

(1) A high placement temperature will accelerate hydration of the cement, which generates heat 

and increases the temperature of the interior of the member, so that the temperature gradient is 

increased, and (2) high curing temperatures result in lower tensile strengths resulting from the 

type of microstructure that develops under these curing conditions.(35)

The placement temperature and the ambient temperature strongly influence the temperature 

distribution in the concrete. The interaction between them can be decisive for the tendency to 

crack at early ages. A suitable choice of placement temperature in relation to ambient 

temperature allows the possibility of optimizing prestress in the surface layers as well as of 

avoiding adverse conditions that cause surface cracking.(39)

Some measures used to control temperature are not always compatible with the goal of reducing 

cracking.(39) For example, a very low placement temperature on a hot summer day may actually 
18 

favor the formation of surface cracks caused by nonuniform maturity of the concrete through the 

thickness of the section. The warmer surface concrete develops strength and stiffness first, while 

the cooler interior concrete hydrates more slowly. When the interior portion of the concrete does 

begin to hydrate, generate heat, and expand, the surface concrete is already starting to cool and 

contract, generating tensile stresses at the surface. For pavement slabs, Bernander recommended 

reducing the placement temperature of the concrete, using cement with low cracking sensitivity, 

and optimizing the cement content to control the temperature rise. Control of drying shrinkage 

by the use of moist curing or curing compounds is essential. Joint spacing should be determined 

to minimize restraint. The concrete should be protected from solar radiation. 

Cracking at early ages may be exacerbated by simultaneous exposure to low ambient 

temperatures, high surface temperatures (from solar radiation), and drying shrinkage. The risk of 

cracking caused by thermal expansion of the interior is greatest during the heating phase, when 

avoidance of exposure to drying and low temperatures is critical. For this reason, curing with 

water or curing compounds and protecting from direct sun are recommended.(39)

Van Breugel pointed out that the effect of wind on temperature development could exceed that of 

solar radiation.(40) Rapid cooling of the surface because of wind may result in steep temperature 

gradients between surface and interior. He warned that ignoring the effect of wind on 

temperature might completely invalidate the interpretation of otherwise sophisticated 

calculations. Holt measured the shrinkage of concrete specimens from the time of casting and 

found that if the concrete were allowed to dry with no wind, the shrinkage for the first 24 h was 

equal to the shrinkage in the next 3 months.(38) In the case of concrete allowed to dry with wind, 

the shrinkage during the first 24 h was seven times that of the long-term shrinkage. Thus, it is 

essential to begin curing as soon as possible. 

Roper and Anderson observed that in slabs on grade the permeability of the base material has an 

important effect on cracking.(41) Their experiments showed that bleed water remained on the 

surface of concrete cast on an impermeable base far longer than for the same concrete cast on a 

granular base, making it less susceptible to plastic shrinkage cracking; however, tests of the 

quality of the concrete placed showed it to be inferior to that of the concrete cast on a permeable 

base. 

Materials Factors. Krauss and Rogalla summarized the material properties of concrete that 

affect cracking tendency: cement content and composition, modulus of elasticity at early ages, 

creep, aggregate type, placement temperature, heat of hydration, and drying shrinkage.(37) They 

found that mix design factors affecting the tendency to crack include aggregate type and grading, 

cement type and amount, water content, supplementary cementing materials, silica fume, and 

chemical admixtures. 

Aggregate with a low coefficient of thermal expansion will provide less restraint for the 

concrete, reducing its cracking sensitivity. Springenschmid and Breitenbücher considered 

crushed aggregates to be advantageous because their rough surface improves the tensile strength 

of the concrete.(35) A high maximum size reduces the amount of cement paste required for 

workability. The reduced cement content results in reduced temperature rise caused by the heat 

of hydration. With a high maximum aggregate size, the tensile strength may be somewhat 

reduced. 
19 

Cements that develop a modulus of elasticity relatively quickly would reduce the sensitivity of 

concrete to cracking because the concrete could develop some compressive prestress during the 

initial thermal expansion. As Springenschmid and Breitenbücher pointed out, it is not known 

how to implement this theoretical requirement.(35) It is clear that different cements give different 

sensitivities to cracking. Springenschmid and Breitenbücher reported that portland cements with 

low cracking sensitivity have relatively low alkali contents and high sulfate contents in relation 

to their C3A contents, and they are not too fine.(35) Also, high early strength results in increased 

tendency to crack. 

Thomas and Mukherjee found that slag is effective in reducing the initial rate of heat 

development and the maximum temperature rise.(42) These effects increased with the slag 

content; however, these benefits are at least partially offset by concomitant reductions in the 

tensile strength and tensile strain capacity of slag concrete at early ages. Thus, the replacement of 

portland cement by slag may not be effective in mitigating thermal cracking without the use of 

additional measures. Chan et al. found that the presence of slag in the concrete increased the 

autogenous shrinkage, while the presence of fly ash reduced it.(43) Ternary concretes containing 

both supplementary cementing materials behaved similarly to the slag concretes. 

Thomas et al. investigated the effects of 12 different fly ashes on the temperature rise and earlyage tensile strain capacity of concrete.(42) They found that the rate and amount of heat evolved 

increased with the calcium content of the fly ash; however, increasing fly ash contents reduced 

the heat evolved for all of the fly ashes tested. Thus, even high-calcium fly ashes are effective in 

reducing the heat evolved if used in sufficiently large doses. The flexural strength of the concrete 

decreased with higher dosages of fly ash. The strain capacity at one day was reduced for many of 

the fly ash concretes compared to the control. The strain capacity of the fly ash concretes was 

similar to or slightly higher than that of the control concrete at 3 and 7 days. Thus, the beneficial 

effect of the fly ash in reducing temperature rise is not necessarily offset by reductions in the 

capacity to resist thermal strains. The authors did not consider the effects of creep and stress 

relaxation in their analysis. 

Springenschmid et al. recommended that concrete strengths higher than necessary be avoided 

because high strengths often lead to higher cracking tendency.(34) Specifiers may prefer to 

specify a 56- or 90-day strength rather than a 28-day strength to reduce cementitious content, and 

therefore, the cracking tendency. 

Ziegeldorf et al. tested the mechanical properties of cement pastes at early ages and found that 

those with lower w/c exhibited a rapid increase in tensile strength at about 7 h and little change 

in tensile strength between 15 and 75 h.(44) The compressive strength increased rapidly at first 

and continued to increase at later ages. The development of the modulus of elasticity was similar 

to that of the tensile strength. The development of strain to fracture was not uniform. Pastes with 

higher w/c showed a steep decrease with age up to 10 h, with a minimum at about 30 h. Pastes 

with lower w/c also showed a minimum at about 7 h. 

To reduce the stresses caused by drying shrinkage, the water content should be kept as low as 

possible. A large maximum size aggregate and optimized particle size distribution of the 

aggregates, particularly for the sand, will minimize the amount of cement paste (and water) 
20 

needed for good workability. Further reductions in water content can be achieved by the use of 

water reducers, and by keeping the placement temperature low.(34)

Springenschmid and Breitenbücher reported that air entrainment increases the ultimate tensile 

strain by about 20 percent and reduces the modulus of elasticity and the consequent stresses 

caused by restraint.(35) Both effects reduce the cracking sensitivity of the concrete. 

Test Methods for Evaluating the Tendency of Concrete Mixtures to Early Cracking 

Cracking Rings. Krauss and Rogalla developed a test method in which concrete is cast in the 

annulus between a stiff inner steel ring and an outer steel ring.(37) The restraint supplied by the 

inner ring to the shrinkage of the concrete is comparable to that encountered in full-depth bridge 

decks, while the outer ring provides little restraint to expansions. Water is ponded on the 

concrete surface. At the end of the curing period, the water and the outer steel ring are removed, 

and heavy plastic sheeting attached to the top surface to prevent loss of water. Strain gauges 

attached at the quarter points on the inside of the inner ring indicate when the concrete cracks. 

Sellevold et al. have used a similar test apparatus.(45)

This test method provides a close approximation of the conditions encountered in concrete 

bridge decks; however, it is impossible to simulate the effects of delayed or negligent curing 

within the first hours (before final set). The test can be of long and highly variable duration; 

Whiting and Detwiler found that their silica fume concrete specimens took from 18 to 51 days to 

crack, and some did not crack at all.(46) More important, it is not clear what constitutes a good or 

acceptable result in terms of performance in the field; one can simply conclude that one concrete 

is more or less prone to crack than another. 

The ASTM International has published a test method (ASTM C 1581) to determine the age of 

cracking in mortars and concrete under restrained shrinkage. The procedure can be used to 

determine the relative effects of cementitious materials properties on the risk of drying shrinkage 

cracking. 

RILEM Cracking Frame. The International Union of Testing and Research Laboratories for 

Materials and Structures (RILEM) cracking frame consists of a closed insulated frame with two 

crossheads and two invar steel bars 100 mm (4 inches) in diameter. The fresh concrete is placed 

directly into the formwork of the frame. Thus, deformations are restrained from the beginning, 

with the degree of restraint being at least 75 percent. Strain gauges on the steel bars allow for 

continuous measurement of the deformations, and thus, the forces in the bars and in the concrete 

specimen.(47)

The information provided by the cracking frame data, that is, the stresses developed under 

conditions of restraint, is probably more useful than the time required to crack the concrete. This 

test method has the additional advantage of allowing for simulation of a wider variety of 

conditions of curing, including drying conditions beginning at the time of casting. The main 

disadvantage of this method is the high cost of the invar steel bars. 

ICBO Method: Cracking of Slab Under Restraint. The International Conference of Building 

Officials (ICBO) Test Method for Evaluating Plastic Shrinkage Cracking of Restrained Concrete 

with Synthetic Fibers specifies a test panel 356 by 559 by 102 mm (14 by 22 by 4 inches) deep. 
21 

Immediately following casting and screeding, the finished surface is subjected to a wind 

generated by a fan. Internal restraints and a stress riser are cast into the panel to initiate cracking. 

This test provides a reasonable simulation of conditions likely to be encountered in the field on 

hot, windy days when cracking is most problematic; however, because it includes all of the 

conditions at once, it does not provide insights into the causes of cracking in a particular 

concrete. 

Japan Concrete Institute Method: Unrestrained Shrinkage. The tendency to crack is closely 

related to shrinkage. If the concrete is completely unrestrained, it may shrink or expand freely 

and no stresses develop. If the concrete is restrained from shrinking, tensile stresses develop. 

This is particularly critical at early ages because the concrete has little or no tensile strength to 

resist the stresses, and thus, it is vulnerable to cracking. Tests such as ASTM C 157, Standard 

Test Method for Length Change of Hardened Hydraulic-Cement Mortar and Concrete, can be 

used to measure the free shrinkage of concrete at later ages (normally after 28 days curing), but 

ignore the critical first few days. 

The Technical Committee on Autogenous Shrinkage of Concrete of the Japan Concrete Institute 

(JCI) reported on a new test method that measures the autogenous shrinkage or expansion of 

concrete specimens from the time of casting.(48) The specimens are 100 by 100 by 400 mm (4 by 

4 by 16 inches). Gauge plugs are cast into each end to allow for measurement of any changes in 

length using dial gauges or other sensors. The bottom plate of the mold is covered with a 

polytetrafluoroethylene sheet and all surfaces of the mold are then covered with polyester film to 

prevent any restraint of the concrete specimen. After 24 h, the specimens are removed from the 

mold and sealed on all sides with aluminum adhesive tape. Length changes are monitored up to 

28 days. 

Holt and Leivo pointed out a difficulty inherent in this test method in relation to anchoring gauge 

plugs in fresh concrete.(49) At very early ages, the concrete may settle under its own weight. 

Because the embedded gauge plugs move with the concrete, the sensors could register settlement 

as a length change; however, this problem is expected to be minimized in the case of the low- or 

no-slump concretes used for paving. This test has the advantage that test conditions such as 

temperature and curing could be modified as needed to simulate conditions in the field. 

Researchers who have used the test have indicated that precision and reliability of the test was 

poor. 

Fundamental Properties of Concrete Related to Cracking 

For modeling, heat of hydration curves indicate the rate and amount of heat developed over time. 

These can be used to predict the temperature of the concrete at different locations and different 

times. Van Breugel considered that the various types of hydration curves—adiabatic, semiadiabatic, or isothermal—to be equally useful for modeling.(40) The selection depends on the 

experimental difficulties in obtaining the data and the size of the concrete elements to be 

analyzed. Adiabatic curves for the first 72 h of hydration can be determined accurately using an 

adiabatic calorimeter. These have the advantage of being possible to determine for the concrete 

mix to be used on site, and they are most appropriate for simulating conditions in mass concrete. 

Semi-adiabatic curves are generally easy to determine for concrete. In smaller sections from 
22 

which some heat loss can be expected, these would simulate the hydration conditions reasonably 

well. Isothermal hydration curves usually apply to cement paste rather than concrete, and thus, 

they may not fully represent the hydration of cement in concrete. In any case, isothermal 

hydration would not be expected in concrete structures. The data generated from these tests can 

be used in modeling to predict the thermal history of the concrete at early ages. 

The times of initial and final set can be determined by ASTM C 403, Standard Test Method for 

Time of Setting of Concrete Mixtures by Penetration Resistance. In this test, mortar is sieved 

from a representative sample of concrete, placed in a container, and stored at a specified ambient 

temperature. The resistance of the mortar to penetration by a set of standard needles is measured 

at regular time intervals. From a plot of penetration resistance versus elapsed time, the times of 

initial and final set are determined. This test has distinct advantages over tests on cement paste or 

mortar made expressly for the measurement of setting times. Testing cement paste is 

inappropriate because the shearing experienced by cement paste in concrete is very different 

from that imposed by the standard mixing procedure. Shearing has a significant effect on the rate 

of hydration of the cement at early ages, so it is essential to simulate the mixing conditions as 

closely as possible. The mortar test is preferable from the standpoint of mixing, but it is 

somewhat different from that of mixing in concrete. In addition, a large batch of concrete can be 

used to cast several types of test specimens, so that the data from different tests can be directly 

compared. Setting times could be determined for more than one ambient temperature to simulate 

different weather conditions in the field. 

The basic mechanical properties of the concrete—compressive and tensile strength and modulus 

of elasticity—change rapidly within the first 24 h. The modulus of elasticity determines the 

stress developed when a volume change such as autogenous shrinkage, thermal expansion, or 

contraction is restrained. The tensile strength measures the ability of the concrete to resist 

cracking under these stresses; thus, it is essential to measure these properties at frequent intervals 

from the time of final set, particularly within the critical first 24 h. Standard ASTM tests for all 

of these properties are well established. As with the other tests, different specimens should be 

maintained at different temperatures so that the effect of weather can be included as a variable. 

The mechanical properties of concrete would be difficult to monitor in the field by the methods 

described in the previous paragraph; however, they can be correlated with appropriate 

nondestructive test data for field use. Ultrasonic pulse velocity measurement has not been 

successful in determining the quality of early-age concrete, principally because of the attenuation 

of signal strength through the relatively thick units. A more recent approach to record the 

evolution of fresh concrete while still in the formwork (or molds) is described by Rapoport et 

al.(50) This approach concentrates on the interface between the formwork or mold and the 

concrete, and relies on the ultrasonic shear wave reflection from this interface. The reflection 

energy is measured, and it has been shown to be directly related to properties such as setting 

action between 1 and 6 h and modulus of elasticity after 12 h. The equipment used in those 

studies operates at a much higher frequency range than the direct transmission method (between 

1 and 10 megahertz (MHz)). This is in the frequency range normally applied to steel weld 

testing, and is made possible by the relatively small signal penetration depths required. 

Repeatability and sensitivity are thereby enhanced. Laboratory specimens in metal molds can be 

monitored at the same time intervals used for the conventional mechanical tests and the data 

correlated. For field monitoring, metal boxes could be cast as inserts into the concrete. 
23 

See et al. outlined a procedure to quantify concrete behavior under restrained shrinkage using a 

ring specimen.(51) Cracking resistance of concrete is a combination of shrinkage potential, 

shrinkage rate, tensile creep, and tensile strength. Tensile creep was shown to be important in 

evaluating the risk of cracking under restraining conditions. It was also realized that shrinkage–

reducing admixtures significantly improved the cracking resistance of concrete by reducing the 

shrinkage potential and the shrinkage rate. The data also showed that tensile creep under 

restrained shrinkage was lower than under a constant stress—suggesting the data on tensile creep 

obtained under classical constant load may lead to nonconservative predictions on concrete 

performance. 

Hossain et al. developed a simple stress solution for the ring test data as an attempt to make the 

ring test more quantitative.(52) Their procedure incorporates restrained ring test with acoustic 

emission, which can be used in evaluating stress development and cracking tendency for various 

concrete bridge decks, patching, or paving mixtures. 

Air Void System Findings 

Purpose and Mechanism of Air Entrainment 

Concrete used in pavements in cold regions of the country, such as the Midwest and the 

Northeast, is exposed to severe winter conditions. This includes heavy snowfall, the application 

of large quantities of deicing agents, and many cycles of freezing and thawing while concrete is 

in a saturated condition. Concrete is susceptible to frost damage because it is porous. Porosity of 

concrete consists of an interconnected pore system (capillary pores) representing the space 

occupied by mix water that did not become part of the hydrated portland cement. When 

subjected to freezing, concrete may be degraded because of the pressure generated by the 

movement of water or ice through the internal pore system. The mechanisms of frost damage are 

driven by the freezing of water in the capillary pores; however, the exact mechanism of frost 

damage is still not completely understood, even though it has been extensively studied for more 

than 50 years. It has been established that concrete with a proper air void system will sustain 

many cycles of freezing and thawing without serious damage, as the inclusion of entrained air 

provides empty space within the paste to which the excess water can move and freeze without 

damage. 

While a minimum amount of entrained air certainly is needed, the quality of the air void system 

in the hardened concrete is the most important factor in its ability to withstand a severe freezing 

and thawing environment. Theoretical work has indicated that the minute air voids introduced 

into the concrete during mixing must, in the final hardened state, be of such a size and spacing 

that disruptive forces induced by migration of water during freezing can be relieved so that the 

tensile strength of the concrete is not exceeded.(2) Spacing factor and specific surface are the 

main parameters of the concrete air void system controlling frost resistance. The spacing factor is 

a measure of the distance water must travel before reaching an air void.(36) Specific surface is a 

measure of air void size. Higher specific surfaces are associated with a system consisting of a 

large number of small voids. The air bubbles, if properly spaced, act as safety valves to protect 

all the paste. 
24 

Air-entraining agents have been used in concrete for more than 50 years to produce an entrained 

air system that protects the concrete from frost damage. Air on the surfaces of cement and 

aggregate particles is normally entrapped in concrete on mixing, but it is of limited value because 

the air voids are too large and widely spaced. The addition of a suitable surfactant entrains 

additional air in the form of a stable foam that persists in the hardened concrete as a system of 

finely divided air voids well dispersed throughout the cement paste. Taylor describes airentraining admixtures generically as long-chain molecules with a polar group at one end, which 

becomes concentrated at the air-liquid interface with their polar parts in the liquid and nonpolar 

parts in the air.(53) The air-entraining agent lowers the surface tension of the water, stabilizing the 

air bubbles. The inner surfaces of the air bubbles are composed of hydrophobic material formed 

by the nonpolar parts of the molecules. This material acts as a barrier to the entry of water during 

mixing or placement of the fresh concrete, or when the hardened concrete is saturated. 

Until the early 1980s the majority of air-entraining agents were based solely on the salt of wood 

resin (neutralized vinsol resin). This material is a by-product of a process for recovering various 

solvents and rosins from pine wood stumps. These were originally marketed as vinsol, short for 

“very insoluble,” and later were known as vinsol resin. Because they are highly insoluble, they 

are neutralized with sodium hydroxide to form a soluble sodium soap, which is the basis of 

commercial formulations.(2,7) Neutralization allows the admixture to form films around air 

bubbles immediately after addition to and subsequent agitation of the concrete mix because it 

does not require any further reaction with alkalis generated by cement hydration. For this reason, 

entrained air is generated quickly with vinsol resin air-entraining agents, and there is a temporary 

minor increase in air content with continued mixing, followed by air loss with prolonged mixing. 

In addition to neutralized vinsol resin, several groups of air-entraining admixtures were available 

but not widely used in highway construction. However, because of the limited supplies of vinsolbased admixtures and their relatively high cost, other types of air-entraining admixtures have 

been used more frequently in highway construction in the last few years. 

It is difficult to define the exact components of an air-entraining admixture because of their 

complexity and the proprietary nature of manufacturers’ formulations. In addition to vinsol resin, 

air-entraining admixtures available in the market generally include wood-derived acid salts such 

as tall oil, vegetable oil acids, synthetic detergents, and others. Each class of these admixtures 

will generate air void systems somewhat different from the others. For example, tall oil-based 

agents will generate very small air bubbles, while vegetable oil acid-based air-entraining agents 

will create coarser air bubbles. A complete evaluation of the air void system is important when 

any new air-entraining agent is used, even though all other materials in the mix have remained 

the same. 

Factors Affecting Air Entrainment 

In addition to air-entraining agents, all materials used in concrete (portland cement, 

supplementary cementing materials, water, chemical admixtures, sand, and aggregate) to a 

certain degree influence the air void system.(7) Production procedures, construction practices and 

field conditions also affect the air void system of concrete. The effects of these factors on the air 

void system have been studied extensively over the years. Recently the focus of research has 
25 

been on specific issues such as the effect of chemical admixtures and their compatibility with airentraining admixtures and supplementary cementing materials. 

Certain combinations of water reducers and air-entraining admixtures can be incompatible, 

resulting in unacceptable air void systems. Plante et al. indicated that increasing the dosage of 

water reducers influences the air void system.(54) Doubling the recommended dosage of any of 

three water reducers in their study negatively influenced the stability of the air void system. 

There was no consistent relationship between the change in admixture dosage and the resulting 

air content. 

Accelerating admixtures have a minor effect on the air void system. Stott et al. studied the effect 

of both calcium chloride and nonchloride accelerating admixtures on frost durability.(55) They 

found that the air content and spacing factor of mixes containing accelerating admixtures did not 

differ from those of the control mixes. Attiogbe et al. indicated that properly air-entrained 

concrete containing superplasticizer could have adequate frost resistance even if the spacing 

factors were relatively high.(56) Spacing factors exceeding the American Concrete Institute (ACI) 

recommended maximum values of 0.20 mm (0.008 inch) were determined in their concretes, yet 

the frost resistance was acceptable. 

Increases in the water content will increase the air content up to a point as the workability 

increases, but air may be lost from very fluid concrete. While increasing the cement content 

produces a greater number of smaller air bubbles, an increase in water generates coarser bubbles. 

Because air-entraining admixtures are surfactants (surface-active agents), the fineness of the 

cement influences the air content of the concrete. The introduction of more surface area with 

increasing fineness of the cement increases the required dosage of air-entraining admixture. Air 

content is decreased by increasing the cement content of a given concrete mix; therefore, a 

higher dosage of air-entraining agent (per unit mass of cement) is needed to maintain the 

required air content. 

An overview also summarized the basic principles and influences of pore formation, 

manufacturing, and evaluation of air-entraining concretes.(57) Resin-based soaps and mixtures of 

both nonionic and ionic tensides are commonly used in developing air-entraining agents for 

concretes. The influence of cement type, additives, and aggregates, and a number of other factors 

needs to be considered for producing air-entrained concrete. 

The chemical and mineralogical compositions of cement types (for example, intermixed 

substances, sulfate carriers, grinding aids) play a role in the air pore characteristics. Each cement 

needs to be evaluated for the amount of air-entraining agent to be used for a specific application. 

Fine particle additives can have detrimental effect on the formation and stability of air voids. 

Particle size and shape (spherical or pointed) of the additives also play a role. It is pointed out 

that additives that are not compatible with air-entraining agents may not develop the air pores at 

all, or they may destroy the already existing air pores. 

Also, a change in aggregate sources such as sand and gravel pits can lead to variation in particle 

size distribution—especially in the range < 1 mm (0.04 inch) can have a pronounced effect on air 

void system. A large proportion of < 0.25-mm (0.01 inch) particles make formation of air voids 

difficult, whereas the presence of a high proportion of particles between 0.25 and 1 mm (0.01 
26 

and 0.04 inch) favors the formation of air voids. It is also recommended that only fresh water be 

used as mix water for concrete because the recycled water containing fine particle suspensions 

can cause uncontrollable changes in air void systems. 

Pigeon et al. indicated that an increase in the soluble alkali content of the cement significantly 

improved the stability of the air void system, especially when superplasticizer is used.(58) They 

also found that the use of superplasticizer with a low-alkali cement can increase the spacing 

factor. Whiting and Nagi reported that alkalis allow more of the air-entraining agent to remain in 

solution during the mixing process, making it more effective.(7) The higher the alkali content of 

the cement, the lower the required dosage of air-entraining admixture. 

Air content increases with increasing sand content; therefore, the dosage of air-entraining agent 

needs to be decreased as the sand content is increased to maintain the same air content. Coarse 

sand also increases the air content; however, spacing factors may be higher than acceptable. 

Pavements in Nebraska and Kansas, where coarse sands were used in concrete mixtures, 

exhibited freeze-thaw failure (in the form of scaling) even though the air contents were higher 

than specified. (59) 

The use of supplementary cementing materials in concrete will affect its air void system. High 

carbon content in fly ash decreases the air content because carbon adsorbs the air-entraining 

agent and prevents it from acting to stabilize the air bubbles in fresh concrete; therefore, higher 

dosages of air-entraining agent are needed to form stabilized air void systems. Gebler and 

Klieger indicated that the air void system of concrete containing ASTM C 618 Class C fly ash is 

generally more stable than that of concrete containing Class F fly ash.(60) Their study showed that 

while fly ash affects the volume of air, it has less influence on the air void system parameters 

(spacing factor and specific surface). Studies showed that concretes containing up to 50 percent 

fly ash (percent by mass of total cementitious material) can have adequate frost resistance.(61)

Their research indicated that different sources of fly ash did not have a significant effect on the 

concrete air void system. It has been found that silica fume does not have a significant influence 

on the production and stability of the air void system, but because of its fineness, higher amounts 

of air-entraining agent are needed. 

Construction practices such as retempering (adding water to restore consistency), working in 

high temperatures, prolonged vibration (or over-vibration), and pumping may lead to alterations 

in the air void system of concrete. Compared with other construction factors, placement 

temperature can be more critical and difficult to control. Higher temperatures will require higher 

dosages of air-entraining admixtures to maintain a given air content.(7) However, Saucier et al. 

found that, while changes in temperature lead to changes in the total air content, the spacing 

factor of the hardened concrete is not significantly affected.(62) It has been observed recently that 

at high placement temperatures, some new air-entraining admixtures can cause the air bubbles to 

accumulate at the surfaces of aggregate particles, weakening the concrete. This phenomenon is 

discussed in the next section in more detail. If considerable air is lost because of any of the above 

factors, there may be insufficient air bubbles left to achieve the necessary spacing factors that are 

required to ensure good freeze-thaw durability. 

Gardner and others have attributed several effects of elevated temperature on concrete.(63) This 

may include rapid setting because higher temperature facilitates faster formwork turnover; 
27 

elevated mix temperatures results in higher 28-day compressive strengths; elevated mix and 

curing temperatures lead to increase in pore diameter. 

Pang and others developed a modified lignosulfonate superplasticizer to positively influence the 

hydration temperature and the resulting microstructure. It was found that the admixture could 

remarkably retard the cement heat of hydration.(64) With the dosage of 0.35 percent, the 

temperature dropped by 13 °C; thus, the amount of thermal crack reduced and the population of 

smaller pores increased. The growth of ettringite became refined as the crystal size turned small, 

which made the concrete denser, less permeable, and more corrosive resistant. 

Khayat and Assaad evaluated the influence of mix proportioning on the stability of air void 

system in self-consolidating concrete (SCC) when subjected to agitation.(65) Several samples 

were tested at different time intervals to analyze the variation in air void system upon agitation. 

A modified point-count method was used to determine the air voids. The corresponding 

parameters evaluated were Bingham rheological parameters (plastic viscosity and yield stress), 

slump flow, filling capacity, V-funnel flow time, and surface settlement. Data indicated that the 

air void characteristics in SCC could be similar to those in normal-slump concrete. Greater air 

void stability could be achieved when the SCC had a higher content of cementitious materials 

and a lower water-to-cementitious materials ratio (w/cm). For mixtures with a relatively low 

cementitious material content and a high w/cm, air void stability may still be obtained by 

incorporating a viscosity-modifying admixture. It was pointed out that to avoid coalescence of 

small air bubbles during agitation, the plastic viscosity and yield stress values should not exceed 

10 N·m·s (88.5 lbf·in·s) and 2 N·m (17.7 lbf·in·s), respectively. Such limits also yield greater air 

void stability in occasionally agitated concrete. 

Recent Problems With Air-Entrainment in Concrete Pavements 

A survey conducted by Nagi and Whiting, found that 85 percent of the respondents indicated 

having experienced some problems with control of air content.(66) Over the years concrete users 

have learned to overcome most of these problems. In the last 10 years, numerous incidents 

related to use of air-entraining agents in highway concrete were reported in many States. The 

most common problem was the loss of strength associated with the use of synthetic air-entraining 

agents. Loss of air caused by excessive vibration of concrete during paving procedures was also 

reported. 

Air Void Clustering. Loss of strength associated with the use of new air-entraining admixtures 

(mainly synthetic admixtures) was noticed in several States in the last few years. Interviews with 

DOT personnel, researchers, and concrete producers in the Midwestern and Eastern States 

confirmed the occurrence of such problems. Strength reductions of 20 percent or more have been 

observed in concrete pavements. The strength loss is usually manifested when the 28-day 

compressive strength is found to be less than the design strength. 

An increase in air content by a percentage point leads to an average reduction of 3 to 5 percent in 

compressive strength. Strength reductions recently have been noted in concretes having normal 

air contents. When neutralized vinsol resin air-entraining agents were replaced by synthetic 

admixtures, the 28-day compressive strengths dropped even for comparable air contents. Most of 

the States reported more than usual debonding of aggregate particles during compression testing. 
28 

A failure mode of mostly shear at the interface between aggregate and paste was noticed, with 

very few fractured aggregate particles. Microscopic examination indicated accumulations of air 

voids around the aggregate particles. The presence of excessive voids around the aggregate 

obviously reduces the bond strength between the aggregate and surrounding mortar, leading to 

this type of failure. 

The effect on strength of clustering air voids around aggregate particles is not a new concept; 

however, few cases were reported in the past. Hover reported a case study in which the 

accumulation of air bubbles at the mortar/coarse aggregate interface led to debonding of 

aggregate particles and reduction in strength.(67) The South Dakota DOT conducted a 

comprehensive investigation to define the causes of compressive strength reduction observed 

during the construction season of 1997.(68) The strength reduction was caused by poor bond 

between paste and aggregate, and it was attributed to the change from the traditional vinsol resin 

air-entraining agents to new synthetic admixtures. The report stated that the incompatibility 

between low-alkali cement and synthetic admixtures, along with high summertime temperatures 

aggravated the problem. Thinner-walled air bubbles formed by these admixtures caused more 

flocculation than would be observed with vinsol resin admixtures. As a result of this study, the 

South Dakota DOT banned the use of synthetic air-entraining admixtures. 

A research project sponsored by the New Jersey DOT is studying similar strength loss problems 

associated with the use of the new generation of air-entraining admixtures. The New York State 

DOT (NYSDOT) has experienced similar problems. During summer construction when certain 

synthetic air-entraining admixtures were used, the compressive strengths went down even though 

the air contents remained within the normal range. As a result, NYSDOT banned the use of some 

these admixtures. The State of Delaware also encountered strength reductions on one pavement 

project. Personnel in the Delaware DOT materials laboratory indicated difficulties with synthetic 

air-entraining admixtures in passing the strength requirements of ASTM C 260. ASTM requires 

the concrete strength when the new admixture is used to be at least 90 percent of that of a 

reference concrete. In some cases compressive strengths of 80 percent or less were obtained 

when synthetic air-entraining admixtures were used. Based on these observations, the State of 

Delaware banned the use of synthetic air-entraining admixtures. A representative of the 

Michigan DOT indicated that the State had had problems with incompatibility among synthetic 

air-entraining admixtures, cement, and water reducers. Strength loss associated with aggregate 

debonding was observed. On the other hand, this problem was not a major concern in Illinois, 

Kentucky, Maryland, Missouri, and Ohio. 

The effect of the use of synthetic air admixtures was more noticeable at higher air contents. As 

mentioned, an increase in air content by 1 percent decreases the strength by 3 to 5 percent, but, 

when a synthetic air-entraining agent is used, the strength reduction may be greater. 

Admixture manufacturers have indicated that the problem with air void systems and the 

associated strength loss may be caused by short mixing times. At least one manufacturer 

recommended the use of neutralized vinsol resin in concrete pavements. Other factors such as the 

condition of aggregate (e.g., moisture content) and mixing speed may also contribute to the 

problem. In applications other than pavement, synthetic air-entraining admixtures did not appear 

to be problematic. Some ready-mix suppliers prefer to use synthetic admixtures. Air loss 
29 

resulting from haul time and agitation is lower when synthetic air-entraining admixtures are 

used. Air contents are sometimes increased by the longer mixing times. 

Kozikowski et al. investigated the factors causing the air void clustering.(69) They studied mix 

design variations, mode of mixing, slump, and strength in concrete samples prepared with a 

variety of cements, aggregates, admixture types, and w/c. Microscopic means were used to 

assess the degree of clustering. Following is a summary of the results: 

• A late addition of water to concrete mixes using nonvinsol admixtures would result 

in air void clustering. Retempering concrete mixes containing these types of 

admixture will exacerbate the clustering problem. The severity of clustering 

increases when the retempered concrete is mixed for longer periods. A later addition 

of water enhances the formation of air content regardless of the admixture type used. 

• The potential for air void clustering may be greater in finer air void systems. 

• The timing of air-entraining admixtures (AEA) addition (i.e., before or after cement 

is added) did not influence the air void clustering. 

• Moisture in aggregate did not influence the formation of air void clustering. 

Based on the data obtained, a useful rating system was developed to relate the severity of air void 

cluster to the strength of concrete. 

Consolidation. Normally consolidation is carried out by vibration, which reduces the friction 

between the aggregate particles and makes the concrete more flowable.(7) For slip-form paving, 

internal vibrators are usually spaced at a maximum of 450 to 600 mm (18 to 24 inches) and 

operate at frequencies from 5,000 to 10,000 vpm. The purpose of vibration is to remove pockets 

of entrapped air generated in fresh concrete; however, vibration also can cause a loss of entrained 

air from fresh concrete, especially if the vibrator is held in place for extended periods. The loss 

of air content caused by vibration depends on the concrete slump, initial air content, vibration 

frequency, and amount of vibration. Studies have shown that for a given vibration frequency and 

vibration time, the loss of air increases with slump.(70) An increase in vibration frequency also 

has a significant effect on the air void system. The spacing factor significantly increased for 

concrete subjected to 20 s of vibration at frequencies of 11,000 and 14,000 vpm; however, for 

frequencies of 8,000 vpm or less, even though the air content is decreased, the spacing factor 

remains relatively unchanged. 

In some cases of concrete pavement construction, scaling caused by cycles of freezing and 

thawing is observed in paths following the vibrator heads on the paving machine. This is to the 

result of excessive vibration. The Iowa DOT has observed an increase in premature deterioration 

in concrete pavements related to overvibration. This problem has been noticed on several 

portland cement concrete pavement projects across the State. Tymkowicz and Steffes reported 

that cores taken from longitudinal cracks in I–80 in Iowa contained 3 percent air in the top half 

and 6 percent in the bottom half.(4) Iowa DOT attributed this behavior to excessive vibration, 

saying that excessive vibration occurred at lower paver speeds even though the frequency was at 

middle range (8,000 vpm). As a result, Iowa DOT recommends that for vibration frequencies 
30 

from 5,000 to 8,000 vpm, the paver speed should be greater than 1 meter per minute (m/min) 

(3 feet per minute (ft/min)). The investigation indicated that the radius of effective consolidation 

of the vibrator was smaller than is commonly believed. Cores taken between vibrator trails 

showed significant entrapped air within 4 inches of the vibrator location. Stutzman conducted a 

similar study on Iowa pavements and found that the air void systems of deteriorated pavements 

were worse in the visible vibrator trails.(8) 

Test Methods for Air Void System 

The preceding discussion summarizes the many factors that can influence the air void systems of 

concrete and lead to changes in its air content from design values. All highway agencies specify 

limits for air contents of concretes. These limits account for the possible changes in air content 

resulting from the factors mentioned above; however, all current specifications are based on 

measuring the air content of fresh concrete. 

ASTM C 231, Air Content of Freshly Mixed Concrete by Pressure Method. This is the most 

commonly used test. This test serves as a very good quality control tool to assure frost resistance 

of millions of cubic meters (m3) (cubic yards (y3)) of concrete each year used in pavements and 

other infrastructure; however, the total air content in itself does not guarantee frost resistance. 

One reason is that the total air content includes entrapped air, which does not contribute to frost 

resistance. In addition, many contractors target the lower limit of air content to maximize 

strength. This sometimes may not leave enough entrained air to protect the concrete, especially 

in severe exposures. As mentioned above, some concretes with high air content will not tolerate 

repeated cycles of freezing and thawing because of high spacing factors. Much of the air may 

exist in larger entrapped voids, which can protect only a small portion of the paste. The number 

of air voids in concretes having the same air content may vary dramatically. In one experiment, 5 

to 6 percent air was incorporated into concrete by using each of five different air-entraining 

agents.(71) The resultant numbers of were 24,000, 49,000, 55,000, 170,000, and 800,000 voids 

per cubic centimeter (390, 803, 900, 2,790, and 13,100 million air voids per cubic inch). 

ASTM C 457, Microscopical Determination of Parameters of the Air void System in 

Hardened Concrete. The measurement of the air void system parameters, as opposed to total air 

content, is a more realistic prediction of concrete performance under repeated cycles of freezing 

and thawing. It would be desirable to have a rapid test that could give concrete users a quick 

indication of the air void system so that corrections could be made without incurring extensive 

delays in the construction process. The only ASTM method for such measurements is ASTM 

C 457, Microscopical Determination of Parameters of the Air void System in Hardened 

Concrete. In this method, entrained air is measured microscopically on a cut and polished section 

of concrete. While modern computer-assisted techniques make the measurement somewhat more 

efficient, it is still time consuming and tedious, and concrete must be sufficiently mature to 

withstand polishing for examination. It may be possible to accelerate the hydration by heat 

curing the specimens. 

Torrens and Ivey developed a test in which the air in a mortar sample is displaced by excess 

water in a conical glass container.(72) By tracing the area of bubbles that adhere to the glass plate, 

an estimate of the surface area can be obtained to compute a void-spacing indicator. The 

relationship between the void-spacing indicator factor and the spacing factor depends on the ratio 
31 

between the air contents of the fresh and hardened concrete. Because this ratio cannot be known 

in advance, predicting the spacing factor from the void-spacing indicator factor is difficult. 

ASTM Type A Air Meter. Another technique to evaluate fresh concrete air void system has 

been developed by Norwegian investigators using an ASTM Type A air meter.(73) The meter is 

filled with concrete and subjected to external vibration. The rate of air loss with time is 

determined. From the rate of air loss and certain assumption related to the rheological properties 

of concrete, the void size distribution is calculated. The test assumes ideal behavior of air 

bubbles regarding their movement through the cement paste. 

Air Void Analyzer. A more promising technique was developed in Europe in the mid 1980s to 

measure the air void parameters of concrete. The equipment for this test, known as an Air Void 

Analyzer (AVA), is commercially available. The main advantage of this technique is that the test 

is conducted on fresh concrete and takes less than 30 min to complete.(74) The method is based on 

Stoke’s Law. Large bubbles rise through a column of liquid faster than small bubbles do, and 

therefore, bubble size can be accurately inferred from the time it takes the bubble to rise. Mortar 

is extracted from a concrete sample taken from the as-placed concrete and injected by means of a 

syringe into the base of the AVA. The mortar sample is stirred into a viscous liquid to release the 

air voids. The bubbles rise through the viscous liquid and water in the glass cylinder, and then, 

they are gathered on a petri dish suspended from a bracket attached to a sensitive balance. From 

the viscosity of the system and using Stoke’s Law, the sizes of the air bubbles with time are 

computed and the air void parameters are calculated. The parameters obtained with this method 

are the air content, spacing factor, and specific surface. 

Since 1993, the AVA has been used commercially in Denmark, Sweden, Iceland, Germany, 

Belgium, Switzerland, Italy, and Spain. Recently the AVA was used on the E6 Motorway in 

Sweden.(75) In this project, approximately 1,453 m3 (1,900 y3) of concrete were produced daily. 

The concrete was transported on trucks and placed using a slip-form paver. The AVA was used 

for quality assurance to achieve frost resistance. In addition, cores were taken for ASTM C 457 

test. The specific surface and spacing factor results of the two methods to determine the were 

almost identical. 

Magura evaluated the practicality of the AVA and compared it to ASTM C 457.(76) He listed 

several disadvantages of some parts of the AVA procedure such as the sensitivity of the test to 

vibration and changes in temperature. 

An evaluation of the AVA also was conducted by the Maine DOT. The equipment was evaluated 

during the 1998 construction season. Redmond reported, “this is a remarkable technology and 

should definitely be developed further.”(77) When comparing AVA data with ASTM C 457 

measurements, the report stated that the difference in the readings occurred when air voids larger 

than 3 mm (0.12 inch) (mostly entrapped air) were included in the ASTM C 457 measurement 

but excluded from the AVA data. The report mentioned the sensitivity of equipment to vibration 

and temperature. 

More recently, an automated linear traverse system has also been developed by Zhang et al. to 

determine entrained air void in hardened concrete.(78) The technique has several analytical 

components including an image analysis system for surface images through a microscope, 
32 

methodology for detecting and identifying the air voids, and a computer-controlled twodimensional actuator for bringing the sampling points in line with the microscope. The technique 

requires pigmenting of the sample for color contrast between the voids and matrix. Data are 

analyzed automatically, and air void parameters for air content, specific surface, spacing factor, 

void frequency are displayed and stored. After the sample is prepared for analysis, the process 

for the complete determination of air void parameters takes approximately 15 min. 

Test Methods for Air Void Stability 

In a search for simpler techniques to evaluate the air void stability of concrete, most researchers 

looked into the use of foam theories. Several testing procedures were developed over the years to 

evaluate the effectiveness of an admixture or effect of combinations of materials on air void 

system stability. The earliest technique was used by Bruere in the 1950s.(79) He used the cylinder 

flotation test to evaluate the stability of foams produced by different air-entraining admixtures. 

Foam Index Test. The foam index test(80) has been successfully used by various researchers.(7)

Gebler and Klieger used the test to evaluate the stability of the air void system of concrete 

containing different types of fly ashes and measure the relative air-entraining admixture 

requirements for fly ash concretes.(60) The stability of the air bubbles formed during mixing a 

paste suspension may be an indication of the air void stability in concretes made with the same 

materials. In this test, 50 milliliters (mL) (1.7 fluid ounces (fl oz)) of water are placed in a 500 

mL (17 fl oz) wide-mouth jar. Then, 20 grams (g) (0.7 oz) of the appropriate proportions of 

cement and fly ash are hand-blended and added to the water. The jar is capped and vigorously 

shaken for 15 s. A quantity of air-entraining admixture is then added, and the jar is shaken for an 

additional 15 s. The jar is then placed upright for 45 s, and then the cap is removed. The foam 

index is the minimum amount of air-entraining admixture (in mL or oz) needed to produce a 

stable foam, which is defined as the state where bubbles exist over the entire surface of solution 

in the jar. An unstable state is recognized by discontinuities in the foam, where a stable state is 

indicated by no breaks in the foam. The foam index has been used as a relative indication of the 

amount of air-entraining agent needed in the concrete, assuming that the dosage for a comparable 

concrete without fly ash has been determined. This dosage is then multiplied by the ratio of the 

foam index for the fly ash mix to the foam index of the control concrete to estimate the dosage 

needed for the fly ash concrete. 

Foam Drainage Test. A more promising technique known as foam drainage test, has been 

selected by Cross et al.(68) in the recent South Dakota study to evaluate the stability of air void 

system. The foam drainage test was originally used by Gutmann.(81) He used a kitchen blender to 

mix air-entraining admixtures with water and then poured the foam into a graduated cylinder. 

The level of water drained from the foam was measured after 1 h. In the Gutmann test, only 

water and admixtures were used; the test did not include cement. Also, as indicated by Cross et 

al., the single measurement at 1 h does not allow the determination of the kinetic nature of the 

foam drainage.(68)

By contrast, Cross et al. included cement in their mixture. 300 mL (10 oz) of water is mixed with 

10 mL (0.3 oz) of air-entraining admixture and 5 g (0.18 oz) of cement in a blender.(68) The 

resultant foam is poured into a 1,000 mL (34 oz) graduated cylinder. The amount of water 

drained as a function of time is fit to kinetic equations and the values of V0 and –1/k are 
33 

calculated. V0 is the amount of liquid in the foam at the start of drainage and –1/k is a mixture 

parameter. The percent of water drained and the percent of water in the foam are also calculated. 

These three parameters define the stability of void system formed by a given air-entraining 

admixture. The test data presented by Cross et al. indicate that the foam drainage test provides a 

rapid method for screening air-entraining admixtures. 

SUMMARY 

Concrete mix designs are becoming more complex with the use of supplementary cementing 

materials and combinations of chemical admixtures. The likelihood of incompatibility among 

cementitious materials and admixtures increases with the number of ingredients added to the 

mix. Incompatibility may manifest itself as early stiffening, retardation of setting and strength 

gain, coalescence of entrained air voids, loss of air, or early-age cracking. These problems in turn 

reduce the durability of the pavement, increasing the life-cycle cost that must ultimately be borne 

by the taxpayer and imposing costly delays on the driving public. 

Because of the complexity of concrete, it is not possible to predict incompatibility from tests of 

the individual materials. Combinations of the specific materials to be used on the job must be 

tested using methods that appropriately simulate job conditions. Numerous test methods already 

available could lend themselves to the prediction of various aspects of incompatibility. Some of 

these methods are established ASTM standards, while others are in various stages of 

development. 

35 

CHAPTER 3. PROJECT TASKS 

TASK 2.1.1—EARLY SETTING OR EXCESSIVE RETARDATION 

Introduction 

One of the greatest difficulties experienced by the paving construction industry is when a 

concrete does not stiffen and set at the right time. Early stiffening makes it impossible to move 

the concrete through a slipform paving machine, resulting in poor consolidation and an 

unacceptable surface finish. This is particularly prone to occur during hot weather and when 

certain combinations of cementitious materials and chemical admixtures are used in the concrete 

mixture. Early setting may result in cracks appearing because of drying shrinkage before sawcuts can be made. At the other extreme, slow strength gain and setting can also result in a higher 

risk of cracking because of plastic shrinkage, and difficulties with applying curing compounds, 

which should be conducted soon after texturing but after bleeding has stopped. 

Systems that exhibit unpredictable stiffening and setting are therefore a matter of serious 

concern, and methods to detect such problems well before the concrete is batched are needed. 

The work conducted in this task was to develop such methods, as well as to better understand the 

mechanisms behind the observed problems. 

The work conducted is described first, followed by the data collected and a discussion of its 

meaning and application. 

Six portland cements were tested in this program, with a wide range of C3A and alkali contents. 

Three different supplementary cementing materials (SCM) were included, a slag, and two fly 

ashes including a Class C with a high C3A content. Two Type A water-reducing admixtures 

(WRA), one lignin and one sugar-based, were included in the matrix. All of these materials are 

discussed in more detail in the following sections. 

A large suite of tests was conducted on a matrix of the materials to assess the ability of the tests 

to detect early stiffening and retardation type incompatibility. Some of these tests were 

conducted at 10 °C (50 °F) and 32 °C (90 °F) as well as at the standard 21 °C (70 °F). 

Following is a summary of the rounds of the test matrix: 

• Round 1. Every cement, with a single dose of every SCM and a single dose of the 

lignin-based WRA (24 mixtures), all at 21 °C (70 °F). 

• Round 2a. Selected cement/SCM combinations (Early Stiffening) with no WRA, and 

at a double dosage of the lignin-based admixture (7 mixtures) at 21 °C (70 °F). 

• Round 2b. Selected cement/SCM combinations (Normal and Early Stiffening) with 

sugar-based WRA at a single dose (6 mixtures), 21 °C (70 °F). 
36 

• Round 3. Selected cement/SCM/WRA combinations (Normal and Early Stiffening) 

(8 mixtures) at 32 °C (90 °F). 

• Round 4. Selected cement/SCM/WRA combinations (Normal and Delayed 

Stiffening) (8 mixtures) at 10 °C (50 °F). 

In addition, concrete mixtures were prepared and tested using selected cementitious/admixture 

systems at all three temperatures (36 mixtures). 

Details of the materials and the selections of combinations for the various rounds are discussed 

in the next two sections. Discussion of the test methods and results follows. 

Materials Selection and Characterization 

To cover a reasonable number of material combinations, six commercial portland cements, 

described in table 1, were identified based on analyses of samples received from manufacturers. 

North American cements contain different proportions of gypsum and hemihydrate, and the 

cements in table 1 provide a representative selection. To address the solubility of natural 

anhydrite and gypsum, cements containing anhydrite were incorporated in the program. Both 

retarding and early stiffening characteristics of these cements were evaluated with and without 

WRAs. One cement from Task 2.1.2 was also used in this task as indicated in table 1. The 

cements came from six plants and five manufacturers. 

Table 1. Commercial portland cement characteristics used in Task 2.1.1. 

Cement 

Type 

Percentage of C3A 

Content 

(High is > 6) 

Percentage of 

Alkali Content 

(High is > 0.6%) 

Gypsum-toHemihydrate Ratio 

(High is > 1) Comment 

High High Low Contains natural 

anhydrite 

High High Low – 

High Low High – 

Type I 

High Low Low – 

Low Low Low From Task 2.1.2 

Type II Low Low Low Contains natural 

anhydrite 

A Class C fly ash was selected with a relatively high C3A content (11.4 percent) based on the 

experiences reported from the field that this type of material is most commonly associated with 

setting and stiffening problems. 

The Class F fly ash used was selected with moderate to high loss-on-ignition (LOI) content 

(4 percent). 

A commercially available ASTM C 989 grade-100 slag was selected from a local supplier. 

Type A WRAs generally are made using three basic chemical forms: (1) lignins with setbalancers, (2) sugars or polymers, and (3) combinations of 1 and 2. Most of the work was 
37 

conducted using a lignin-based material (WRA A), but some mixtures were prepared using a 

sugar-based system (WRA B). 

Materials Characterization 

The procured cements and SCMs were characterized for their phase and oxide compositions and 

fineness as shown in tables 2, 3, and 4. The analytical tools used were X-ray diffraction, X-ray 

fluorescence, differential scanning calorimetry (DSC), and thermogravimetric analysis (TGA). 

Analysis and characterization of the materials used in the study involved the use of X-ray 

diffraction analysis and selective dissolution techniques, some of which were specially 

developed at the contractor’s laboratory for this project. The six portland cements used for this 

study consisted of Type I and Type II cements with compositions ranging from low to high C3A 

and varying alkali contents. The supplementary cementing materials used in preparing the 

cement blends were Class C and Class F fly ash, and granulated slag. Both fly ashes were used at 

a replacement level of 20 percent by mass, while the blend made with the slag was at 40 percent. 

Table 2. Oxide analyses of cements. 

Percentage of Mass 

Analyte Cement 1 Cement 2 Cement 3 Cement 4 Cement 5 Cement 6

SiO2 20.51 19.06 20.29 19.48 19.22 20.83 

Al2O3 4.46 6.03 5.48 5.95 5.56 4.20 

Fe2O3 3.19 2.13 2.8 2.68 2.66 3.3 

CaO 63.43 62.45 65.59 64.42 61.63 62.55 

MgO 2.99 2.67 1.02 0.85 2.34 3.23 

SO3 2.72 3.87 2.63 3.32 4.42 2.75 

Na2O 0.13 0.23 0.19 0.18 0.27 0.13 

K2O 0.65 1.25 0.3 0.53 0.99 0.65 

TiO2 0.23 0.26 0.26 0.51 0.29 0.30 

P2O5 0.07 0.31 0.16 0.24 0.21 0.09 

Mn2O3 0.07 0.07 0.06 0.04 0.18 0.53 

SrO 0.1 0.25 0.16 0.24 0.07 0.05 

Cr2O3 <0.01 <0.01 <0.01 0.01 <0.01 <0.01 

ZnO <0.01 <0.01 0.01 0.02 0.04 0.22 

L.O.I. (950 oC) 1.44 1.23 0.9 1.41 2.11 1.45 

Total 99.99 99.82 99.86 99.88 99.99 100.24 

Alkalies as Na2O 0.56 1.06 0.38 0.53 0.92 0.56 

Gypsum plaster ratio 1.5 0.08 0.07 1.05 4.11 0.58 

Anydrite Yes No No No No Yes 

Calculated Compounds per ASTM C 150-02a 

C3S 60 55 65 61 51 56 

C2S 13 13 9 10 17 18 

C3A 6 12 10 11 10 6 

C4AF 10 6 9 8 8 10 

Blaine Fineness, m2/kg 392 395 411 442 431 392 
38 

Table 3. Oxide analyses of supplementary cementing materials. 

Analyte Percentage of Mass 

Material Slag Class C 

Fly ash 

Class F 

Fly ash 

SiO2 37.6 32.26 52.56 

Al2O3 7.95 17.38 20.26 

Fe2O3 0.87 6.06 11.46 

CaO 38.91 26.8 4.29 

MgO 10.87 7.87 1.00 

SO3 2.49 2.65 0.64 

Na2O 0.33 2.03 1.32 

K2O 0.37 0.35 1.92 

TiO2 0.84 1.37 0.97 

P2O5 <0.01 0.90 0.28 

Mn2O3 0.53 0.04 0.05 

SrO 0.04 0.47 0.08 

Cr2O3 0.01 0.02 0.02 

ZnO <0.01 0.01 0.04 

L.O.I. (950 oC) −0.99 0.24 4.22 

Total 99.84 98.47 99.1 

Alkalies as Na2O 0.58 2.26 2.58 

Thermogravimetric Analysis (as-received basis) 

Free moisture (Ambient −105 °C) 0.06 0.08 

L.O.I. (105 °C–750 °C) 0.21 4.26 

L.O.I. (750 °C–950 °C) 0.03 −0.04 

Table 4. Particle size distributions of cementitious materials. 

Size Percentage Passing 

(micron) Cement 1 Cement 2 Cement 3 Cement 4 Cement 5 Cement 6 Slag Class C Class F 

45 90.22 87.42 87.74 89.15 88.53 90.20 97.97 74.47 84.14 

30 77.51 72.49 72.43 74.71 73.58 77.74 90.96 64.51 74.09 

10 41.24 36.30 34.81 37.79 36.94 37.90 56.21 39.00 40.38 

7 32.05 28.67 27.46 29.96 29.34 28.62 44.93 31.71 30.34 

3 16.47 14.58 14.27 15.69 15.23 13.75 23.07 16.73 12.48 

1 5.41 4.72 4.73 5.17 4.99 4.03 7.11 5.12 3.10 

Cement 1 

This cement had low free lime (CaO) and moderate to high level of periclase (MgO) with high 

ferrite phase (C4AF) and low C3A. Alite (C3S) and belite (C2S) were present in normal amounts 

with only slight prehydration as indicated by the presence of small amounts of Ca(OH)2. The 

total alite and belite was estimated at 78 percent by mass of the cement using selective 

dissolution techniques. Anhydrite (CaSO4) was the predominant form of calcium sulfate present 

in the cement, followed by hemihydrate or plaster (CaSO4·1⁄2H2O) and gypsum (CaSO4·2H2O). 

The clinker sulfate was mainly present in the form of K3Na(SO4)2. 
39 

Cement 2 

In contrast to Cement 1, Cement 2 contained high C3A and low ferrite phase. It was also with 

low free lime and moderate amounts of periclase. The alite and belite were present in normal 

proportions with an estimated total of 73 percent. There was slight prehydration of the silicates, 

as indicated by the presence of small amounts of Ca(OH)2. Hemihydrate or plaster was the 

predominant form of calcium sulfate present in the cement, mixed with only a small amount of 

gypsum. Alkali sulfates in the form of both K2SO4 and K3Na(SO4)2 were present in significant 

amounts in this cement. 

Cement 3 

This high C3A cement contained both low free lime and periclase. Again, alite and belite are 

present in normal proportions with an estimated total of 77 percent. No indication of 

prehydration was found in this cement. Hemihydrate or plaster was the predominant form of 

calcium sulfate form present in this cement mixed with small amount of gypsum. K2SO4 and 

K3Na(SO4)2 were also detected in the cement but only in small amounts. 

Cement 4 

This cement was high in C3A content and low in both free lime and periclase contents. Alite and 

belite also appeared to be present in normal proportions with an estimated total of 74 percent. No 

indication of prehydration was found in the cement. Gypsum was the predominant form of 

calcium sulfate present in the cement mixed with small amounts of hemihydrate or plaster. Both 

K2SO4 and K3Na(SO4)2 in moderate amounts were detected in the cement. 

Cement 5 

This cement was moderately high in C3A with low free lime and moderate amount of periclase. 

The alite and belite in the cement appear to be present in normal proportions with an estimated 

total of 72 percent. There was slight prehydration of the C3S as indicated by the presence of 

small amounts of Ca(OH)2 in the cement. Gypsum was the predominant form of calcium sulfate 

present in the cement mixed with very small amounts of anhydrite and hemihydrate or plaster. 

High amounts of clinker sulfate in the form of arcanite, aphthitalite, and calcium langbeinite 

were detected in the cement. This cement had been received from the field (see section on 

cracking), and it had been in sealed storage for some time before testing. 

Cement 6 

As with Cement 1, this cement had a high ferrite content and the lowest level of C3A of the six 

cements. It also had low free lime and contained moderate amounts of periclase. As in the case 

of the other five cements, alite and belite were also present in normal proportions at an estimated 

total of 78 percent. No indication of prehydration of the silicates was found. Anhydrite was the 

predominant form of calcium sulfate form present, followed by hemihydrate or plaster and 

gypsum. The only clinker sulfate detected in the cement was K2SO4 in small amounts. 
40 

Granulated Slag 

The granulated slag was completely amorphous (glassy). The characteristic amorphous peak in 

the diffractogram was at about 0.29 nanometers (nm), a significantly lower D-spacing than that 

found in Class C fly ash. The slag had an estimated glass content of 99 percent as obtained using 

an acetic acid selective dissolution method. 

Class C Fly Ash 

The Class C fly ash consisted mainly of an amorphous phase (glassy phase) along with 

crystalline compounds that include alpha-quartz (SiO2), C3A, MgO, CaO, CaSO4, C2S, C2AS, 

and ferrite. Further testing of the fly ash gave the following additional information: C3A = 11.4 

percent, CaSO4 = 4.0 percent, and acid insoluble residue = 28 percent. The acid insoluble residue 

was primarily composed of alpha-quartz (SiO2), anorthite (CAS2), sillimanite (Al2SiO5), coesite 

(SiO2), cristobalite (SiO2), and a glassy phase that was not acid-soluble. 

Class F Fly Ash 

As with the Class C fly ash, the Class F fly ash also was composed primarily of an amorphous 

phase and some crystalline components that include alpha-quartz, Fe3O4, Al2SiO5, (Mg,Fe)2SiO4, 

and CaO. The main difference was that Class F fly ash contains no reactive crystalline reactive 

component such as C3A. The acid-insoluble residue (89 percent) of the fly ash consisted virtually 

of the same phases detected before treatment except for CaO. 

Chemical Admixtures 

The chemical admixtures used for this study are identified according to ASTM C 494 as Type A. 

Water-reducer Type A was reported by the manufacturer to be lignin-based and water-reducer 

Type B was reported by the manufacturer to be sugar-based. Both products were obtained from 

the same manufacturer. 

TEST MATRIX FOR PASTE AND MORTAR SYSTEMS 

Fifty-two sets of cement pastes and mortars were tested in four rounds. For each of the mixtures 

prepared in the four rounds described below, a number of tests were conducted as summarized in 

table 5 (described below). All of the paste tests were conducted in duplicate. Details of the 

methods are provided in the discussion in the next section. 

Following is a list of labeling conventions used: 

• First character=cement number (1 through 6). 

• Second character=SCM added (P=plain, C=Class C fly ash, F=Class F fly ash, 

S=slag). 

• D (where present) indicates a double dose of admixture. 

• A or B identifies water-reducing admixture. (No label means no admixture.) 
41 

Table 5. Tests conducted on paste systems in all rounds. 

Information to Obtain Test Method 

Yield stress and plastic viscosity to diagnose 

stiffening characteristics 

Minislump (Contractor, National Institute of 

Standards and Technology (NIST)) 

Rotational rheometer (NIST) 

Heat generation behavior of the cementitious 

system Isothermal conduction calorimetry 

Setting behavior Penetration of 2 mm diameter vicat needle 

(AASHTO T 131)( Contractor, NIST) 

Bleeding 

Mass and volume of water decanted after 

initial set from a known volume and mass of 

cement paste (NIST) 

Mortar cube strength ASTM C 109 (Contractor) 

Mortar air content ASTM C 185 (Contractor) 

Mortar stiffening ASTM C 359 (Contractor) 

Pore solution chemistry 

Periodically up to 24 h. Analyses were 

conducted for sulfate, calcium, alkali and 

hydroxyl ion concentrations, and pH 

(Contractor) 

Supplementary cementing materials were dosed at the following cement replacement levels: 20 

percent for Class C and Class F fly ash, and 40 percent for ground granulated blast furnace slag 

(GGBFS). All paste and mortar tests were prepared at a fixed w/cm of 0.5, unless otherwise 

indicated. Admixture dosages were fixed as 325 and 650 mL/100 kg (5 and 10 oz/cwt) for 

WRA A at single dose and double dose, respectively, and 163 mL/100 kg (2.5 oz/cwt) for 

WRA B. 

Discussion of the test methods and their data interpretation is given in a later section. 

Round 1 

Mixtures. Mixtures made with the six cements shown in table 1 were tested at room temperature 

with and without a single dosage of each of the three supplementary cementing materials. The fly 

ashes were used at 20 percent cement replacement, and the slag at 40 percent cement 

replacement. All of the mixtures were made with a lignin-based Type A lignin-based WRA, and 

they were dosed at the manufacturer’s maximum recommended dosage (24 mixtures). All tests 

were conducted in duplicate. 

Data. All results have been consolidated into a single table (table 6). Limiting values were 

selected to indicate early stiffening systems, and those outside these limits are shaded. The limits 

were selected based on the following criteria: 

• Where current specifications provide pass/fail limits, these were used. 

• For some test methods, the experience and expertise of the team were used. 

• For other tests, values were selected that flagged a limited number of the tests in 

round 1. 
42 

The shaded cells in table 6 indicate potentially rapid stiffening systems, while speckled cells 

indicate potentially delayed or retarded systems. The number of shaded cells for each system was 

counted, as shown in the right-most columns of table 6. 

Based on the number of shaded cells, systems 2PA, 2CA, 4PA and 5PA were selected as “early 

stiffening” and 1PA, 1CA, and 6PA as “normal.” 

Discussion. A significant difference between the approaches by the contractor and the National 

Institute of Standards and Technology (NIST) was that the contractor concentrated on the 

stiffening that occurs in the first few minutes as a result of C3A and/or sulfate effects. These tests 

have indicated several cases of false set, and in Cement 2, a lot of apparent instability. NIST, 

which concentrated on the instability and C3S-based stiffening effects, flagged Cements 3 and 4. 

In reviewing the complete set of data, the contractor took the viewpoint of a user who observes 

something happening to the concrete, and who does not know or care about the chemical 

reactions that are causing the problem. It is, therefore, appropriate that the tests represent both 

types of problem and exclude cement 3 and 4 from the “normal” set. The systems without 

supplementary cementing materials that exhibited the least number of fast hits were 1P and 6P, 

and that 1C was selected as the system with Class C fly ash to pair with its control. 

At least one system containing a SCM was included in both sets; therefore, the choice of 2C is 

appropriate because problems in the field often are associated with high C3A Class C fly ash, 

depending on the cement with which it is combined. 
43

Table 6. Summary of paste and mortar data from round 1. 

Note: Shaded cells indicate potential rapid stiffening or setting.  Speckled cells indicate potential delayed or retarded stiffening or setting. Unit conversions: 

1mm =0.0394 inch 1 mL = 0.0338 oz 1 mm2 = 0.00155 in21 megapascal (MPa) = 145.0 pounds per square inch (psi) 
44 

Rounds 2a and 2b 

Mixtures. Four of the mixes that exhibited early stiffening in round 1 were repeated with no 

WRA and at double the manufacturer’s maximum recommended dosage using the same 

admixture (8 mixtures) (round 2a). 

The early stiffening cementitious systems tested in round 2a, along with three that did not exhibit 

accelerated stiffening, were repeated using a second (sugar-based) WRA at the manufacturer’s 

maximum recommended dose (7 mixtures) (round 2b). 

Fifteen combinations were tested at room temperature. The same tests were conducted in this 

round as in round 1. 

Data. All of the results from this round are consolidated into table 7. As before, the same 

limiting values were used to indicate “Early Stiffening” systems, and those outside these limits 

are shaded. Again, the approach was to count the number of shaded cells for each system as 

shown in the last columns on the right. 

Based on the number of shaded cells in tables 6 and 7, the following systems were selected for 

testing in rounds 3 and 4: 

• Early stiffening: 2PA, 5PA, 5P, 5PB. 

• Normal: 1PA, IPB, 1CA, 6PA. 

• Delayed stiffening: 2CA, 2FA, 2CDA, 1CB. 

Discussion. Cements 2 and 5 have indicated problems with early stiffening including when they 

contain different admixtures. Three versions of the Cement 5 system were selected as “Early 

Stiffening,” along with one from Cement 2. 

As before, Cements 1 and 6 appeared to be the least prone to problems, and they were selected as 

the control materials: three from Cement 1 and one from Cement 6. 

Selection of the “Delayed Stiffening” set was the most open-ended because there was no 

obviously retarded system in the materials tested. Class C fly ash appears to have slowed setting, 

despite its propensity to also cause slump loss, and therefore, it was included in three of the 

selected systems. One system with Class F fly ash was also chosen as a companion to one of the 

Class C fly ash selections. 

The overlap of materials selected was considered desirable to help with comparing the effects of 

each component on the systems. 
45 

Table 7. Summary of data from round 2. 

Notes: Shaded cells indicate potential rapid stiffening or setting.  Speckled cells indicate potential delayed or retarded stiffening or setting. Unit conversions: 

1 mL = 0.0338 oz 1 mm2 = 0.00155 inch2

1 MPa = 145.0 psi 
46 

Rounds 3 and 4 

Eight mixes were tested in round 3 at an approximate paste temperature of 32 °C (90 °F) to 

simulate hot weather conditions. The eight mixtures were selected based on the stiffening rates 

measured in rounds 1 and 2. Four were the fastest stiffening mixes from rounds 1 and 2, and the 

other four were those with intermediate stiffening rates. This set was selected to model the effect 

of high temperature on the risk of loss of workability and early setting (eight mixtures). 

In round 4, eight paste mixes were tested at 10 °C (50 °F). The eight mixes were selected based 

on the stiffening rates measured in rounds 1 and 2. Four were the slowest stiffening mixes from 

rounds 1 and 2, and the other four were the same set as used in round 3 with intermediate 

stiffening rates. This set was selected to model the effect of low temperature on the risk of 

retardation (eight mixtures). 

Data. The results from the last two rounds were consolidated into table 8. The same limiting 

values were used to indicate “Early Stiffening” systems, and those outside these limits are 

shaded. Based on the data from all four rounds of tests conducted on pastes, eight systems were 

selected for testing in concrete. 

It was decided that the three selected for the “Delayed Stiffening” paste tests should also be used 

for concrete tests. Noting that 1C is in the “Delayed Stiffening” set, the remaining two were 

selected for the “Normal” concrete mixtures. The set of “Early Stiffening” systems in round 3 

has only two materials; therefore, a third system was selected based on its performance in 

rounds 1 and 2: 

• Early Stiffening: 2P, 5P, 4P. 

• Normal: 1P, 6P. 

• Delayed Stiffening: 2C, 2F, 1C. 

Discussion. Again, the overlap of materials selected should help with the comparison of the 

effects of each component on the systems and concrete performance with paste and mortar. 

All data from rounds 1 through 4 are summarized in table 9 in sets of cement type to allow 

comparison of the effects of chemical admixture types and dosages. 
47 

Table 8. Summary of data from rounds 3 and 4. 

Notes: Shaded cells indicate potential rapid stiffening or setting.  Speckled cells indicate potential delayed or retarded stiffening or setting. Unit conversions: 

1 mL = 0.0338 oz 1 mm2 = 0.00155 inch2

1 MPa = 145.0 psi 
48 

Table 9. Summary of all paste and mortar data.

Round Mixture Temperature Bleed 

2-mm 

Vicat 

Final 

Set 

Calorimeter 

Set 

Minislump 

False Set 

Index 

(Area5/Area2)

Minislump 

Stiffening 

(Area30/Area5)

Minislump 

Pat Area 

Initial 

Peak 

Silicate 

Peak 

24 Hour 

Cube 

Strength 

Air 

Content

Stiffening 

(ASTM C 

359) 

Minislump, 

Time to 

 < 48mm 

V

Ini

 °C mL min min in^2 J/gh J/gh MPa % Min 

4 1PA 10 6.0 720 1.1 0.9 17480 1.24 28 244 1 1PA 21 5.0 330 390 1.2 1.0 17390 44.2 13.0 7.17 27 245 3 1PA 32 5.6 192 1.2 1.0 16650 10.41 27 304 4 1PB 10 8.0 720 1.4 1.2 22320 3.03 21 244 2 1PB 21 630 510 1.3 0.9 15950 45.9 13.0 11.10 17 304 3 1PB 32 5.6 210 1.1 0.8 15290 13.17 17 335 

C 1PDA 10 C 1PDA 21 C 1PDA 32 

4 1CA 10 5.0 720 1.0 0.9 17160 0.34 27 302 

C 1CA 10 

1 1CA 21 5.0 510 540 1.1 0.9 19280 40.4 9.4 3.10 27 

C 1CA 21 

3 1CA 32 2.0 300 1.1 0.7 16000 6.07 23 304 4 1CB 10 3.5 720 1.1 1.0 22060 0.55 20 303 2 1CB 21 840 630 1.1 0.9 19450 38.7 10.3 4.34 17 362 

C 1CDA 10 C 1CDA 21 

1 1FA 21 7.0 390 420 1.1 0.9 17070 45.6 10.6 3.72 19 305 1 1SA 21 8.0 450 510 1.2 1.1 17130 26.5 8.5 2.07 25 304 2 2P 21 300 270 1.6 1.9 11910 66.3 14.5 16.82 15 False 123 1 2PA 21 10.0 390 480 0.9 0.6 6980 87.0 14.7 7.45 30 False 13 

C 2PA 21 

3 2PA 32 4.1 210 1.0 0.5 7100 15.24 22 Dry 12 

C 2PA 32 

2 2PB 21 450 510 1.0 0.4 8800 78.3 15.6 15.31 17 False 13 2 2PDA 21 630 570 1.9 1.0 11080 73.3 12.9 2.14 39 13 

C 2PDA 21 C 2PDA 32 
49 

Table 9. Summary of all paste and mortar data (continued).

Round Mixture Temperature Bleed 

2-mm 

Vicat 

Final 

Set 

Calorimeter 

Set 

Minislump 

False Set 

Index 

(Area5/Area2)

Minislump 

Stiffening 

(Area30/Area5)

Minislump 

Pat Area 

Initial 

Peak 

Silicate 

Peak 

24 hour 

Cube 

Strength 

Air 

Content

Stiffening 

(ASTM C 

359) 

Minislump, 

Time to 

 < 48mm 

V

Ini

 °C mL min min in^2 J/gh J/gh MPa % Min 

2 2C 21 420 390 1.1 1.0 16680 65.1 13.3 24.13 15 305 4 2CA 10 2.3 720 1.2 1.1 20000 33 123 

C 2CA 10 

1 2CA 21 6.0 630 630 1.1 0.8 15570 77.3 12.0 1.86 32 64 

C 2CA 21 

2 2CB 21 630 690 1.2 0.7 15940 58.7 12.1 10.82 18 64 4 2CDA 10 0.5 720 1.2 1.1 18970 39 365 

C 2CDA 10 

2 2CDA 21 690 840 1.2 0.8 7520 49.8 9.7 2.41 37 423 

C 2CDA 21 

4 2FA 10 9.0 720 1.2 0.8 18450 28 183 

C 2FA 10 

1 2FA 21 5.5 450 540 1.1 0.9 15530 75.4 11.1 3.59 24 False 197 

C 2FA 21 C 2FDA 10 C 2FDA 21 

1 2SA 21 5.0 450 480 1.2 0.8 12380 48.1 10.2 2.28 27 123 1 3PA 21 4.5 330 360 1.1 1.0 14180 65.2 10.4 5.38 21 False 185 1 3CA 21 7.5 570 660 1.1 0.9 18580 61.0 9.9 2.83 23 307 1 3FA 21 6.5 390 480 1.1 1.0 15070 73.4 9.0 4.55 13 False 183 1 3SA 21 7.0 390 450 1.2 1.0 15050 45.9 8.6 2.41 21 False 243 2 4P 21 270 270 1.2 1.1 15930 87.3 14.7 13.79 16 False 183 1 4PA 21 4.0 330 420 1.3 1.1 16610 84.0 12.2 10.48 22 False 94 

C 4PA 21 C 4PA 32 

2 4PB 21 300 480 1.2 0.9 14300 87.5 14.0 12.07 17 False 182 2 4PDA 21 420 600 1.6 1.1 13360 87.7 12.1 5.24 35 False 93 

C 4PDA 21 C 4PDA 32 

1 4CA 21 6.5 450 600 1.2 1.0 18490 75.7 10.9 5.03 24 184 
50 

Table 9. Summary of all paste and mortar data (continued).

Round Mixture Temperature Bleed 

2-mm 

Vicat 

Final 

Set 

Calorimeter 

Set 

Minislump 

False Set 

Index 

(Area5/Area2)

Minislump 

Stiffening 

(Area30/Area5)

Minislump 

Pat Area 

Initial 

Peak 

Silicate 

Peak 

24 hour 

Cube 

Strength 

Air 

Content

Stiffening 

(ASTM C 

359) 

Minislump,

Time to 

 < 48mm 

V

Ini

 °C mL min min in^2 J/gh J/gh MPa % Min 

1 4FA 21 6.5 390 570 1.2 1.1 16520 85.0 10.5 7.38 15 False 180 1 4SA 21 6.5 390 510 1.4 1.3 15400 58.6 10.6 3.31 21 False 186 2 5P 21 270 270 1.1 0.9 14800 64.5 15.6 12.34 14 Rapid 125 3 5P 32 114 1.0 0.5 7940 15.72 13 184 1 5PA 21 5.0 300 390 1.1 0.8 14730 74.0 13.9 11.17 26 False 94 

C 5PA 21 

3 5PA 32 3.5 180 1.0 0.5 9160 6.69 30 False 187 

C 5PA 32 

2 5PB 21 360 390 0.9 0.4 8390 76.8 14.6 17.79 16 Rapid 124 3 5PB 32 0.7 180 0.8 0.4 7100 11.79 19 False 124 2 5PDA 21 390 480 1.3 0.7 9810 72.7 11.8 5.03 32 False 64 

C 5PDA 21 C 5PDA 32 

1 5CA 21 5.0 450 480 1.1 0.8 16290 66.3 10.7 6.41 29 123 1 5FA 21 5.5 390 450 1.1 0.9 15110 71.1 10.3 5.79 20 False 187 1 5SA 21 6.0 420 450 1.3 1.0 14560 48.0 8.9 4.07 25 243 4 6PA 10 5.0 720 1.1 1.0 17940 0.55 32 186 1 6PA 21 5.0 330 420 1.3 1.1 16730 39.6 13.3 5.17 30 242 3 6PA 32 6.9 174 1.3 0.9 14580 9.31 29 184 2 6PB 21 570 510 1.1 0.8 17170 37.3 14.7 7.79 20 False 304 

C 6PDA 10 C 6PDA 21 C 6PDA 32 

1 6CA 21 4.0 510 600 1.3 1.0 18090 33.3 10.4 2.28 30 243 1 6FA 21 7.5 390 570 1.2 1.0 17070 35.8 11.0 2.76 20 363 1 6SA 21 6.0 480 570 1.3 1.1 15860 22.2 9.1 1.65 26 424 

Unit conversions: 

1 mL = 0.0338 oz 1 mm2 = 0.00155 inch2

1 MPa = 145.0 psi 
51 

TESTING CONCRETE 

The matrix of concrete mixtures and tests is given in tables 10 and 11.

Table 10. Test plan for early stiffening and normal concrete systems. 

Mix 

Behavior 

Cementitious 

System WRA 

Test 

Temperature Tests 

Early 

Stiffening 2P, 5P, 4P 

WRA A at 2 

dosage levels, 

325 and 650 

mL/100 kg 

(5 and 10 

oz/cwt) 

Normal 1P, 6P 

WRA A at 650 

mL/100 kg (10 

oz/cwt) 

Nominal 

temperatures of 

21 and 32 °C 

(70 and 90 °F) 

Slump and flow time 

(vibrating-slope apparatus) 

immediately, 30-min, and 60-

min after mixing. 

Extracted mortar to perform 

AASHTO T 197 for setting 

time and mortar flow 

following ASTM C 230 flow 

table. 

Change in temperature of 

concrete in adiabatic cell with 

time. 

Table 11. Test plan for retarding and normal concrete systems. 

Mix 

Behavior 

Cementitious 

System WRA 

Test 

Temperature Tests 

Retarding 2C, 2F, 1C 

WRA A at 2 

dosage levels, 

325 and 650 

mL/100 kg 

(5 and 10 

oz/cwt) 

Normal 1P, 6P 

WRA A at 650 

mL/100 kg (10 

oz/cwt) 

Nominal 

temperatures of 

21 and 10 °C 

(70 and 50 °F) 

Change in temperature of 

concrete in adiabatic cell with 

time. 

Setting time. 

Coarse aggregate used in the concrete mixtures was a crushed limestone from the Chicago area. 

Fine aggregate was a siliceous river sand also from the Chicago area. The physical properties of 

the materials are given in table 12. The nominal concrete mix proportions used for all the mixes 

are given table 13. 
52 

Table 12. Physical properties of aggregates.

 Limestone Coarse 

Aggregate 

Siliceous Fine 

Aggregate 

Sieve Analysis 

Sieve Percentage Passing 

2.54 cm (1inch) 100.00 

1.9 cm (0.75 inch) 92.30 

1.27 cm (0.5 inch) 46.50 

0.95 cm (0.375 inch) 25.10 

number 4 8.70 100.00 

number 8 90.70 

number 16 71.30 

number 30 49.30 

number 50 16.20 

number 100 3.00 

number 200 0.60 

Pan 0.00 0.00 

Fineness Modulus 2.69 

Density 

Bulk Specific Gravity (SSD) 2.69 2.67 

Absorption 1.40 1.77 

Dry Rodded 

Unit Weight, kg/m3

1,633.00 1,794.00 

Unit conversions: 

1 kg/m3

 = 1.69 pcy 

Table 13. Nominal concrete mix proportions (SSD). 

Material Mass (kg/m3) Mass (pcy) 

Cementitious Materials 335 564 

Fine Aggregate 994 1,676 

Coarse Aggregate 961 1,619 

Water 141 237 

All concrete materials were conditioned in rooms controlled at the target temperatures for 24 h 

before mixing. Mixes were prepared in a 0.056 m3

 (2 ft3), Type SW counter current mixer in a 

room controlled at 21°C (70 °F). Immediately after samples were made they were transported 

back to the appropriate temperature-controlled rooms. 

The following tests were conducted on samples of the concrete mixtures: 

• Slump loss in concrete every 15 min up to 60 min, ASTM C 143. Samples were all 

molded as soon as mixing was complete, covered with plastic sheeting, and left until 

the cones were lifted at the designated times. 

• Slump loss of mortar sieved from the concrete every 15 min up to 60 min, Modified 

ASTM C 1437. 

• Unit weight, ASTM C 138. 

• Air content, ASTM C 231. 
53 

• Temperature, ASTM C 1064. 

• Setting time, ASTM C 403. 

• Consolidation monitoring. 

• Ultrasonic P-wave monitoring. 

• Temperature monitoring using a semi-adiabatic cell. 

Concrete slump, unit weight, air content, and temperature measurements for every concrete mix 

are presented in table 14. Slump loss and mortar flow determinations conducted on some (rapid 

stiffening and control mixtures) are shown in table 15. Setting time results, as well as data 

obtained from nondestructive testing (NDT) measurements and the semi-adiabatic cell, are 

combined in table 16. 
54 

Table 14. Temperature, air content, unit weight, slump, and impedance results.

Cementitious 

System 

WRA A 

Dosage 

(mL/100 

kg) 

Mix 

Temperature 

(°C) 

Air 

content 

(%) 

Unit 

Weight 

(kg/m3

) 

Initial 

Slump 

(mm) 

Impedance, 

Initial 

(Ω) 

Impedance, 

Final 

(Ω) 

Cement 1 

No SCM 

650 

650 

650 

21.7 

33.9 

13.6 

7.0 

4.8 

9.0 

2342 

2396 

2284 

70 

20 

120 

220 

300 

300 

190 

150 

220 

Cement 1 

20%C-Ash 

325 

650 

325 

650 

20.0 

19.5 

15.0 

14.6 

5.2 

8.5 

5.0 

7.8 

2380 

2291 

2390 

2307 

65 

135 

50 

100 

160 

390 

170 

170 

140 

220 

110 

150 

Cement 2 

No SCM 

325 

650 

325 

650 

23.0 

23.9 

35.3 

34.6 

4.6 

5.2 

6.0 

4.0 

2385 

2355 

2243 

2451 

5 

15 

0 

0 

260 

185 

340 

245 

190 

110 

320 

130 

Cement 2 

20% C-Ash 

325 

650 

325 

650 

23.1 

23.6 

14.2 

14.3 

4.2 

6.7 

5.5 

6.7 

2411 

2315 

2364 

2331 

20 

85 

65 

70 

245 

150 

165 

210 

140 

115 

120 

160 

Cement 2 

20% F-Ash 

325 

650 

325 

650 

22.9 

22.1 

15.2 

14.8 

3.5 

4.0 

3.4 

4.8 

2409 

2358 

2396 

2355 

5 

15 

20 

45 

250 

130 

250 

200 

180 

80 

160 

150 

Cement 4 

No SCM 

325 

650 

325 

650 

21.7 

23.5 

33.6 

35.7 

3.5 

4.2 

4.9 

5.1 

2428 

2409 

2352 

2302 

5 

25 

5 

0 

340 

390 

405 

455 

140 

220 

275 

305 

Cement 5 

No SCM 

325 

650 

325 

650 

23.1 

23.9 

32.7 

33.7 

4.9 

6.0 

5.3 

5.4 

2364 

2361 

2368 

2390 

0 

15 

15 

40 

200 

130 

180 

130 

140 

80 

140 

80 

Cement 6 

No SCM 

650 

650 

650 

21.7 

32.3 

13.4 

8.5 

5.3 

8.5 

294 

2377 

2319 

160 

30 

75 

220 

230 

220 

190 

170 

190 

Unit conversions: 

1 °C = (X – 32)/1.8 °F 

1 mL/100 kg = 0.0154 oz/cwt 

1 kg/m3 = 1.69 pcy 

1mm =0.0394 inch 
55 

Table 15. Slump loss and mortar flow loss. 

Percentage Slump Loss 

(at time, m) 

Percentage Mortar 

Flow Loss 

Cementitious (at time, m) 

System 

Mix 

Temp. 

(°C) 

WRA 

Dosage, 

(mL/100 

kg) 

Slump 

(mm) 0 15 30 60 15 30 60 

Cement 1 

No SCM 

21 

32 

10 

650 

650 

650 

70 

20 

120 

0 

0 

– 

27 

100 

– 

64 

100 

– 

82 

100 

– 

0 

0 

– 

12 

5 

– 

26 

24 

– 

Cement 2 

No SCM 

21 

21 

32 

32 

325 

650 

325 

650 

6 

15 

0 

0 

0 

0 

0 

0 

0 

100 

0 

0 

100 

100 

0 

0 

100 

100 

0 

0 

0 

0 

0 

0 

-5 

4 

0 

-4 

-15 

13 

0 

30 

Cement 4 

No SCM 

21 

21 

32 

32 

325 

650 

325 

650 

5 

25 

5 

0 

0 

0 

0 

0 

100 

50 

100 

0 

100 

100 

100 

0 

100 

100 

100 

0 

0 

0 

0 

0 

22 

6 

36 

10 

14 

3 

54 

45 

Cement 5 

No SCM 

21 

21 

32 

32 

325 

650 

325 

650 

0 

15 

15 

40 

0 

0 

0 

0 

0 

50 

100 

83 

0 

50 

100 

100 

0 

100 

100 

100 

0 

0 

0 

0 

62 

33 

22 

11 

94 

39 

51 

21 

Cement 6 

No SCM 

21 

32 

10 

650 

650 

650 

160 

30 

75 

0 

0 

– 

84 

100 

– 

92 

100 

– 

100 

100 

– 

0 

0 

– 

11 

15 

– 

22 

32 

– 

Unit conversions: 

1 mL/100 kg = 0.0154 oz/cwt 

1 kg/m3 = 1.69 pcy 

1mm =0.0394 inch 
56

Table 16. Setting time, NDT, and semi-adiabatic cell results. 

Setting Time (min) 

Impedance 

(Ω) ASTM C 403 Ultrasonic P-Wa

Cementitious 

System 

Temp 

(°C) 

WRA 

Dosage 

(mL/100kg) 

Max 

Temp 

(°C) Initial Final Initial Final Initial Fin

Cement 1 No SCM 

21 32 10 

650 650 650 

34.3 50.3 20.4 

220 300 300 

190 150 220 

398 277 673 

486 348 880 

325 175 733 

6845

129

Cement 1 20%C-Ash 

21 21 10 10 

325 650 325 650 

32.2 31.8 21.5 21.1 

160 390 170 170 

140 220 110 150 

450 486 513 716 

556 625 728 963 

460 589 512 707 

82

102

83

114

Cement 2 No SCM 

21 21 32 32 

325 650 325 650 

40.6 41.1 53.3 53.9 

260 210 340 245 

190 130 320 130 

235 340 124 196 

350 436 204 263 

215 231 220 230 

1984343

Cement 2 20% C-Ash 

21 21 10 10 

325 650 325 650 

38.7 37.1 21.7 20.8 

245 150 165 210 

143 115 123 163 

429 541 776 

1081 

496 597 886 

1447 

345 576 758 

1115 

7499

139175

Cement 2 20% F-Ash 

21 21 10 10 

325 650 325 650 

36.8 37.7 20.6 21.0 

250 130 248 203 

180 

80 

160 150 

283 368 534 735 

410 497 832 

1015 

314 383 630 626 

5966

133100

Cement 4 No SCM 

21 21 32 32 

325 650 325 650 

37.3 39.0 51.5 52.9 

340 390 405 455 

140 220 275 305 

251 328 186 232 

332 419 221 298 

270 388 184 211 

5865659

Cement 5 No SCM 

21 21 32 32 

325 650 325 650 

38.0 40.5 52.6 53.3 

200 130 180 130 

140 

80 

140 

80 

263 237 174 246 

338 303 227 297 

297 245 158 

n/d 

57525572

Cement 6 No SCM 

21 32 10 

650 650 650 

34.5 48.3 20.2 

220 230 220 

190 170 190 

435 247 642 

539 344 869 

378 304 691 

7057

123

Unit conversions: 

1 °C = (X – 32)/1.8 °F 1 mL/100 kg = 0.0154 oz/cwt 1 kg/m3 = 1.69 pcy 1mm =0.0394 in. 
57 

TEST METHODS DISCUSSION 

Each test method is discussed below, including details of the test method if it is not standardized, 

the relevance of the results to assessment of stiffening and setting, and how to interpret the data. 

As indicated above, there is no single mechanism causing so-called incompatibility; therefore, no 

single test will determine if a problem exists. It was observed that all tests are effective for some 

mechanisms, but not for others. Another confounding issue was that no single incompatible 

system could be used as a reference point to calibrate the data from the 24 sets of test data 

collected. This meant that decisions regarding the validity of using a given test method were 

based on data from other test methods that were likewise being questioned. 

A general observation is that in many test methods there is no simple threshold or pass/fail limit. 

A value obtained for one cementitious system may be satisfactory, but a clear indication of 

trouble for another. Rather, a change between batches of materials or between loads of concrete 

will act as the required warnings. This means that data must be collected for a given mix design 

to establish appropriate values for that concrete. 

Many tests that are more suited to field application will be particularly useful in monitoring 

variability. Regular and frequent testing of materials and the concrete system will allow the user 

to develop a familiarity with the product. A sudden change in results of any test discussed below 

will clearly indicate that something has changed in the raw materials, the proportions, or the 

environment. Such a change may signal potential problems in the concrete, and test results will 

warn the user that changes may be required in proportioning or practice. Details of what to do 

will depend on the situation, and the situation may require additional investigation and possibly 

expert advice. A decision to proceed with work during this additional investigation will need to 

be based on balancing the risk of failure against the cost of stopping or changing materials or 

processes. 

Selecting test methods also will be governed by equipment availability. For example, a number 

of methods can be used to assess initial setting time. Any of those tests would be appropriate if 

used consistently, depending on the circumstances at the site and the needs of the project. 

This discussion begins with a brief summary of the hydration processes that are believed to occur 

in the first hours after mixing. The relative rates of these processes cause the observed effects, 

and it is necessary to be able to interpret the data presented in tables 9 through 16. 

A technique used to review the data was to plot two different sets of results to observe whether a 

relationship existed between them. The plots, generated semi-automatically in a spreadsheet, 

were not saved. The plots compared 24 variables, but because the purpose was to see 

relationships, the plots were not generated with axis labels. An example plots with both a clear 

relationship and another with little relationship appear in figures 1 and 2. These plots are the 

basis of the discussion of the usefulness of data sets. 
58 

Figure 1. Example plot with a strong 

relationship between data sets. 

Figure 2. Example plot of data sets with little or 

no relationship. 

Bleeding 

The total bleed water removed from 250-gram (g) (8.8-oz) paste samples was recorded for some 

of the systems. The mixtures used were the same as those prepared to make minislump samples. 

Little useful information was obtained from the bleed tests. There was little correlation between 

these data and any other data collected. 

Setting Time 

Setting time was determined in paste in the contractor’s laboratory using a 2-mm (0.08-inch) 

diameter needle attached to a vicat apparatus. The time to achieve a zero indentation was used to 

indicate the time of final set. The mixtures used were the same as those prepared for minislump 

tests. Tests were cut off at 12 h for systems that had not set in this time. 

Vicat Initial Set vs. Vicat Final Set

0

100

200

300

400

500

600

700

800

900

0 100 200 300 400 500 600 700 800

Air content vs. Minislump Pat Area

0

5

10

15

20

25

30

35

40

45

0 5 10 15 20 25 30 35 40
59 

Setting time in paste was conducted at NIST in accordance with the ASTM C 191 standard using 

the same mixtures as the minislump tests. Data include both initial and final setting times. 

Setting time was also determined using isothermal calorimetry in paste and penetrometer (ASTM 

C 403), ultrasonic P-wave, and semi-adiabatic temperature data in concrete. The initial set was 

taken to be the time when heat or stiffness started to increase after the dormant period. 

Attempts were made to determine the final set based on some variation of when the rate of 

increase in temperature or stiffness flattened out, but, not surprisingly, a poor correlation with the 

penetrometer data existed because final set determined using ASTM C 403 is an arbitrary 

pressure value not necessarily related to the time when hydration rates slow. 

Correlation of the various determinations of initial set was fair, as shown in figure 3. 

The horizontal axis is the average of the various methods for each mixture. 

Figure 3. A plot comparing sets of initial setting time measurements determined 

by different methods. 

Correlation between initial set and final set was also found to be reasonably good for any test 

method, as shown in figures 4 and 5. This means that final set can be estimated with some 

confidence after the initial set is determined using any of the described approaches. Following is 

a list of some of the general observations about the initial set: 

Set Time

0

200

400

600

800

1000

1200

0 200 400 600 800 1000 1200

Average, minutes

Measured, minutes

Calorimeter Set

Vicat Initial Set

Rheology

Concrete Init

Concrete Temp Init

Ultrasonic P-wave Init
60 

• Retarded with increasing dosage of WRA. 

• Retarded with decreasing temperature. 

• Retarded with the use of fly ash. 

• Longer in concrete than in the equivalent paste systems. 

These observations are consistent with reported trends. 

Vertical axis is the first parameter in the heading, horizontal axis is the 

second. Both axes are in minutes. 

Figure 4. Correlation between initial and final set 

for concrete tests. 

Vertical axis is the first parameter in the heading, horizontal axis is the 

second. Both axes are in minutes. 

Figure 5. Correlation between initial and final set 

for paste tests. 

Concrete Init vs. Concrete Final

0

200

400

600

800

1000

1200

0 200 400 600 800 1000 1200 1400 1600

Vicat Initial Set vs. Vicat Final Set

0

100

200

300

400

500

600

700

800

900

0 100 200 300 400 500 600 700 800
61 

The most rapid setting times were observed in the systems containing cements 4 and 5. In these 

systems, the silicate reactions were fastest. The slowest setting times were associated with the 

systems containing fly ash, despite the cement reactivity, largely as a result of changes to the rate 

of silicate hydration. Measurement of this parameter indicates silicate hydration rate and its 

associated effects on concrete properties. 

It appears that any of the tests would be applicable in the laboratory or in the field. Test selection 

depends on the availability of equipment and controlled environments. The cheaper field systems 

are prone to more scatter than more controlled laboratory-based sets. 

Knowledge of the setting time is useful for a number of reasons. Changes in setting time from 

batch to batch or day to day can signal changes in the concrete system. Setting time of concrete 

is sensitive to the environment and the chemistry of the reactive materials, and therefore, it 

provides a useful means to flag changes that have occurred. Changes in setting also affect the 

timing of protecting, finishing, and curing activities, plus the critical activity of saw-cutting 

joints to prevent random cracking in unreinforced pavements. Knowledge of when setting has (or 

will) occur enhances the probability of achieving a crack-free durable structure or pavement. 

Calorimetry 

Introduction. Isothermal conduction calorimetry was selected as a technique to monitor the 

cement hydration process. Cement hydration process is an exothermic reaction. Its intensity 

greatly depends on the cement composition, the w/c, the types of admixture added, and the 

fineness of tested material. The rate and amount of hydration of a hydraulic material, as a 

function of time, can be determined using conduction calorimetry. Conduction calorimetry also 

helps to understand the reactions that occur during the hydration process and their influence on 

strength development, setting time, and premature stiffening. This study used conduction 

calorimetry to assess the effect of supplementary cementing materials on the hydraulic properties 

of cement blends and investigate the effect of admixtures on cement hydration. 

Strength development and setting properties of cement, and subsequently concrete, largely 

depend of the hydration of different cement minerals. Conduction calorimetry monitors cement 

hydration under isothermal conditions as a function of time from the moment water is added to 

cement and the hydration process is initiated. 

Calorimetry is useful to track hydration of a cementitious system. The shape of the power/time 

plot can give clear indications of setting time, reactivity of the system, time when ettringite starts 

to be converted to monosulfate, and if slag or fly ash are present in the system in significant 

amounts. As with many test methods, calorimetry is most useful in detecting changes in the 

system. , The data are summarized as the magnitude of the silicate peak in table 9. 

Equipment. The calorimetry testing was performed using a differential heat flow calorimeter 

designed to monitor the heat of cement hydration as a function of time. A control unit and a 

calorimeter block are two major parts of the instrument. The control unit provides electronic 

temperature control for the heating of the calorimeter block, measures voltage of the thermosignal, and assists in calibration. The calorimeter block is actually a measuring cell that holds the 

specimen and the reference. 
62 

For the analysis, a test tube containing the specimen and a reference test tube containing inert 

material were placed inside the calorimeter block. A disposable syringe filled with mix water 

was placed above the specimen. At the beginning of the experiment, the syringe needle was 

embedded in the sample to deliver the mix water. After the thermal balance was reached, the 

specimen was injected with the mix water. The heat evolved after reactants were mixed was 

continuously measured, evaluated, and stored by a computer during the first 24 h after mixing. 

Current thinking among experts is that it is more important to control the amount of mixing 

applied to the paste at the expense of losing the data for the first 15 to 30 min of the test. This is 

in agreement with the data from this work in which little correlation was observed between the 

initial (wetting/aluminate reaction) peak and the performance of the material. Consistent mixing 

will reduce the scatter in the output of the test. 

Results and Observations. The conduction calorimetry analyses were performed using 5.0 g 

(0.18 oz) of a selected sample and a w/c or w/cm of 0.5. Tests were performed for 24 h at 

25 ± 1°C (77 ± 2 °F). The results for rounds 1 and 2 are discussed below. Tests were not 

conducted on rounds 3 and 4. 

Round 1—General. The intensities of the induction period peaks closely follow the chemistry 

of the tested cements, specifically the tricalcium aluminate (C3A) content. The most intense 

peaks are attributed to sample 2PA and 4PA, samples with the highest amount of C3A. 

Intermediate intensity peaks were observed for samples 3PA and 5PA, and the lowest intensity 

peaks are produced by samples 1PA and 6PA that contain the smallest amount of tricalcium 

aluminate. 

The beginning of tricalcium silicate (C3S) reaction occurs essentially within the same time frame, 

that is, 2 and 2.5 h, for all samples except for sample 2PA. The onset of the C3S reaction for this 

sample occurs almost 3 h after the start of the hydration process. The intensity of the C3S 

reaction for this sample is also the highest, followed by the sample 5PA. The C3S hydration 

profile for samples 1PA and 6PA is very similar; however, the C3S for 1PA peaks a little earlier. 

Samples 3PA and 4PA display a double C3S hydration peak normally occurring when there is an 

excess of C3A over that required combining with the sulfate. 

Calorimetry testing of this set of cements confirmed that hydration process significantly depends 

on the C3A and C3S content of the selected samples together with the sulfate form and content. 

Round 1—Cement and Fly Ash Blends. The hydration process of cement with fly ash 

additions differs from hydration of cements only. Other factors affecting the hydration process of 

cement-fly ash matrix include glass content of fly ash, particle size, amount of sulfate and alkali 

content of cement. The addition of fly ash to cement results in a decrease in the amount of 

calcium hydroxide formed during the cement hydration process; this reduction is caused by the 

pozzolanic reaction with fly ash. 

In this study, the addition of Class C fly ash overall had a retarding effect on all tested cements, 

with sample 3CA (highest C3S content) affected the most and 5CA influenced the least (lowest 

C3S content). For the rest of the samples, the intensity for C3A peaks decreased only slightly 

compared to cement-only samples. The effect of Class C fly ash addition was more evident in the 
63 

hydration of C3S, which was delayed for about 1 (sample 5CA) to 3 h (sample 3CA). 

Furthermore, the C3S hydration peaks became broader and more diffused and exhibited 

noticeable secondary C3A peaks, particularly for 5CA and 3CA samples. 

Overall, the addition of Class F fly ash delayed the hydration process of the sample compared to 

the cement-only samples, but it had a less retarding effect compared to samples with added 

Class C fly ash. Compared to the cement-only samples, the C3A peak intensity for 1FA and 3FA 

samples increased, and samples 4FA and 5FA showed about the same intensity. The C3A 

reaction for 2FA and 6FA samples were affected the most by the Class F fly ash addition 

compared to the respective cements (i.e., it diminished noticeably). Compared to the cement-only 

samples, the onset of C3S reaction was only slightly delayed for all samples with Class F fly ash 

except for 6FA. For this sample, the C3S reaction was retarded by almost 2 h. None of the 

samples containing Class F fly ash exhibit the secondary C3A peak evident in the calorimetry 

graphs for samples with Class C fly ash addition. 

Round 1—Cement and Slag Blends. The hydration process of cement with addition of slag is 

influenced by slag composition, glass content, and fineness. Other important factors influencing 

hydration of cements with slag addition are the dosage of slag and temperature of curing. In this 

study, the addition of slag in general had a retarding effect on both C3A and C3S hydration. The 

intensity of C3A and C3S peaks diminished for all cements containing slag compared to cementonly samples. All slag-containing cement samples except for 1SA exhibit a secondary C3S peak, 

which is most prominent in sample 4SA. 

Round 2a—Selected Cements and Blends with and without Admixture A. The effect of 

WRA on the hydration process of samples exhibiting early stiffening is assessed when 

comparing the hydration profiles of the same samples tested without admixture addition. It was 

evident that the use of admixture A noticeably enhanced the C3A reactivity for samples 2PA, 

2CA, and 5PA. In the case of sample 4P, the use of admixture had very little effect on C3A 

hydration. 

In the hydration of C3S, the retarding effect of admixture addition appears to be very prominent 

for all tested samples, especially for sample 2CA. For this sample, the use of admixture 

considerably inhibits the rate of C3S hydration, extending the initial setting time by almost 2 h. 

The addition of a double dose of admixture A had a significant retarding effect on all tested 

samples; with sample 2CDA affected the most. The onset of the C3S reaction for this sample is 

delayed by almost 3.5 h. 

Based on the results obtained during round 2a testing phase, it is evident that for a given dosage, 

the added admixture enhances the C3A hydration reaction in the early stages of cement 

hydration. The use of the admixture considerably retards the C3S hydration, especially in 

cements with high alkali and C3A content. 

The addition of a double maximum recommended dosage of admixture A had a detrimental 

effect on C3S hydration, significantly inhibiting the hydration process of all tested samples. 

Round 2b—Selected Cements and Blends with Admixture B. In round 2b of testing, 

calorimetry analysis was applied to evaluate the effect of sugar-based admixture on the hydration 
64 

process of the selected samples. For normal-setting cements, the addition of admixture B at the 

maximum recommended dosage had a considerable retarding effect on C3S hydration, especially 

for sample 1CB. Furthermore, the addition of this admixture enhanced the rate of C3S hydration 

for samples 1CB and 6PB compared to the C3S hydration of the same samples tested with 

additions of admixture A. 

In the case of early-stiffening cements, both 2P and 2C cements, the retarding effect of the 

admixture B is similar to the effect of addition of a single dose of admixture A. The addition of 

admixture B enhanced the C3A reaction of the 2PB sample compared to the 2P cement, but it is 

less intense than the C3A reaction of the 2PA sample. The intensity of the C3A reaction for 

sample 2CB decreased when compared to the C3A reaction of both samples 2C and 2CA. The 

use of this admixture considerably increased the rate of C3A hydration of sample 4PB, and had 

almost the similar effect as admixture A on the C3A hydration for sample 5PB. 

The addition of admixture B had a similar retarding effect on C3S hydration for samples 2CB and 

5PB as for the samples with a single dose of admixture A. In the case of sample 4PB, the 

addition of admixture B had a more pronounced effect on C3S hydration, where the onset of the 

C3S hydration occurred almost 2.5 h later than in the samples with a single dose addition of 

admixture A; however, the rate of C3S hydration is considerably enhanced compared to sample 

4PA, and only slightly less than for sample 4P. 

The calorimetry testing of sample 2PB with the addition of admixture B shows the increased rate 

of C3A hydration when compared to samples 2P and 2PDA, but less intense than for sample 

2PA. The onset of C3S hydration for this sample occurs almost at the same time as for sample 

2PA, but the rate of C3S is higher than for samples 2P, 2PA, and 2PDA. 

OBSERVATIONS 

The following list of observations resulted after examining the data obtained from the 

calorimetry tests: 

• Little relationship was observed between the initial (wetting) peak and other 

measured parameters in the pastes. This is not surprising because the data collected 

is governed by both the heat of wetting (dissolution) and the heat of reaction of the 

C3A, and it was not possible to separate the two mechanisms. 

• The data collected provided a reasonable indication of initial setting times as 

illustrated in figure 3. Early hydration rates (particularly silicates) and the effects of 

supplementary cementitious materials are clearly indicated. This method is useful in 

assessing silicate-based reactions. 

• Based on the work reported by Sandberg, the method has the potential to indicate the 

sufficiency of sulfate in the system as indicated by the position of the sulfate 

depletion hump.(14) Undersulfated systems exhibit a secondary peak to the left 

(earlier than) the silicate peak, while systems with sufficient or slight excess of 

sulfate will show a peak to the right (later than) the silicate peak. 
65 

• Hydration initiation of supplementary cementing materials can be observed as a 

second peak some time after the silicate peak. The presence of such a peak is a clear 

indication of the presence of an SCM. 

• As with many of the other methods considered, the method is useful for identifying 

change in a cementitious system to flag potential difficulties in the field. 

• The data indicate that hydration is retarded and slowed with: 

o Increasing fly ash content. 

o Increasing WRA dosage (independent of WRA type). 

ASTM is developing a procedure for running this test and providing a guide for interpreting the 

data. 

Disadvantages of the method are that it requires use of a relatively expensive instrument 

(although many cement and admixture manufacturers have purchased it), and it takes 24 h to run. 

This is a central laboratory test, but some similar, albeit less precise or sensitive, information can 

be obtained from a field-based semi-adiabatic temperature measurement system. This is 

discussed in a later section. 

Minislump 

The minislump cone test(MSCT) was developed to assess the early stiffening of cement paste 

resulting from false set, uncontrolled C3A hydration (flash set), and cement-admixture 

interactions, that is, the reactions occurring in the first 30 min of hydration. The method is being 

used for troubleshooting problems being observed in the field. The approach is to adjust 

parameters such as admixture dosage between mixes and observe changes in behavior. 

Recommendations based on these observations are often successful in reducing problems in the 

field. The test is somewhat more sensitive than can be observed in concrete, meaning that a 

system indicated as potentially problematic in the test may be satisfactory in the field. 

In the procedure, 500 g (17.6 oz) of cement or cement-blend is slowly introduced into the mixing 

jar of a blender containing 250 ml (8.5 oz) of de-ionized water and mixed at a blender speed of 

10,000 revolutions per min (rpm). The blender was equipped with a cooling system designed to 

maintain a final paste temperature of 23 ± 1 oC (73 ± 2 oF). In cases where chemical admixtures 

were used, they were added with the aid of a dropper into the mix along with cement as it was 

slowly introduced into the mix water. A mixing schedule of 30-s mix/rest/60-s mix was adopted 

to enhance the detection of the false setting tendency of cement. After 30 s of mixing, a sample 

of the paste was immediately taken for the first test at 2 min. Next, the remainder of the paste 

was returned to the blender, and at about 3 min, the paste was mixed for another 60 s. After this 

mixing, samples of the resulting paste were taken for subsequent tests at 5, 10, and 30 min. The 

paste was given a low-intensity mixing in the blender 1 min before the 10- and 30-min tests. This 

was done to minimize the effects of bleeding. 

The size of the paste pat formed after the minislump cone was lifted is expressed in the area of 

the pat (mm2

 (inches2)), and the size is an indication of the cement paste workability and flow 
66 

property. The pat areas at ages 2, 5, 10, and, 30 min are reported averages of duplicate 

determinations. The false setting tendency of the cement or blend is reported in terms of a false 

set index (FSI) that is described as the ratio of the pat area obtained at 5 min to that of the 2-min 

test. High FSI values denote the severity of the false-setting tendency of the cement or blend. 

Experience has shown that a value above 1.3 indicates false set. An index of early stiffening was 

also calculated based on the area of the pat at 30 min over the area at 5 min. A value less than 

0.85 was selected as being an indicator of rapid stiffening. The third value used in assessing the 

results was the average pat area between 5 and 30 min. Low values (less than 14,800 mm2 (23 

in2

)) indicated a stiff mix caused by a high water requirement of the system. This value was used 

for these mixes that were all at a fixed cementitious content and a fixed w/cm. 

The minislump tests in round 1 at the contractor’s facility were conducted on mixtures with and 

without admixture A because it was important to establish the effect of the admixture on the 

performance of the systems. All of the tests in the main matrix were conducted twice. The 

average variation between pairs was 625 mm2 (0.97 in2) with a standard deviation of 560 (0.87). 

All of the tests were conducted by the same operator. A limited number of tests were also 

conducted with one cement system at three different w/cm to observe the effect of w/cm. 

The sequence applied at NIST was somewhat different. The same mixes as the main matrix of 

the project were used, but the sequence of mixing and testing was different. Paste was prepared 

in the blender and the initial minislump measured. Measurements were repeated at 30, 60, 90, 

and 120 min. Before each measurement, the cement paste was mixed for 10 s with the blender. 

The data were analyzed to interpolate the time at which a 48-mm (1.9-inch) pat diameter was 

achieved. This parameter is an indicator of the silicate-related stiffening of the paste. NIST has 

also developed a mechanical lifting device to remove variability between operators in this step of 

the procedure (figure 6). 
67 

Figure 6. Device used at NIST to lift the mold for the minislump test. 

Test Results and Discussion. The results for rounds 1 and 2 are presented in tables 17 and 18. 

The contractor’s MSCT data for cement sample 1P and its blends show no indications of early 

stiffening tendency resulting from false set or C3A-related stiffening reactions. The paste pat 

sizes from 2 to 30 min are on average about 16,000 mm2 (25 in2), suggesting that the cement has 

a normal water demand (figure 7). The blend made with Class C fly ash produced the most 

workable paste as indicated by the significantly larger size of the pats in comparison with that of 

the pure cement or those of the other blends made with either Class F fly ash or granulated slag. 

The overall smaller size of the paste pats obtained with the slag blend appear to be reflective of 

the angular nature of slag particles, which has been reported to have a negative effect on the flow 

property of the paste. 
68 

 Unit conversions: 

 1 mm2

 = 0.00155 inch2

Figure 7. A plot of minislump data for mixtures tested in round 1. 

Table 17. Minislump test data for round 1. 

Mix 

Pat Area 

(mm2

 at time, min) 

False Set 

Index 

Stiffening 

Index 

 2 5 10 30 (Limit 1.3) (Limit 0.85) 

Average 

Pat Size 

(mm2

) 

1P 16,520 17,680 16,970 15,160 1.1 0.9 16,580 

1PA 15,810 19,230 17,290 15,610 1.2 1.0 17,420 

1C 17,940 20,840 19,610 16,710 1.2 0.9 19,100 

1CA 19,100 20,970 20,260 16,650 1.1 0.9 19,290 

1F 15,610 16,970 16,060 14,520 1.1 0.9 15,870 

1FA 16,970 18,390 17,290 15,480 1.1 0.9 17,100 

1S 12,840 15,810 14,520 14,320 1.2 1.1 14,900 

1SA 15,100 18000 17,100 16,260 1.2 1.1 17,160 

2P 5,810 8,520 12,260 12,260 1.5 2.1 11,030 

2PA 10,580 9,480 5,100 6,390 0.9 0.6 6,970 

2C 16,260 17,940 16,710 15,420 1.1 0.9 16,710 

2CA 16,060 17,810 15,940 12,970 1.1 0.8 15,550 

0

5000

10000

15000

20000

25000

0 10 20 30

Time, min

Area, mm2

1P 1PA 1C 1CA

1F 1FA 1S 1SA
69 

Table 17. Minislump test data for round 1 (continued). 

Mix 

Pat Area 

(mm2

 at time, min) 

False Set 

Index 

Stiffening 

Index 

 2 5 10 30 (Limit 1.3) (Limit 0.85) 

Average 

Pat Size 

(mm2

) 

2F 13,290 14,710 14,970 14,710 1.1 1.1 14,840 

2FA 15,480 17,290 15,290 14,000 1.1 0.9 15,550 

2S 8,320 13,680 12,840 12,840 1.6 1.5 13,160 

2SA 12,190 14,710 12,390 10,000 1.2 0.8 12,390 

3P 1,160 13,290 11,870 10770 11.7 9.5 12,000 

3PA 13,810 13,610 14,650 14,320 1.1 1.0 14,190 

3C 5,810 16,260 14,970 13,290 2.8 2.3 14,840 

3CA 18,260 20,520 18,650 16,650 1.1 0.9 18,580 

3F 1,230 13,290 12,450 10,970 10.6 8.7 12,260 

3FA 13,870 15,290 15,610 14,320 1.1 1.0 15,100 

3S 4,770 13,870 13,290 12,450 2.9 2.6 13,230 

3SA 13,480 16,520 14,970 13,680 1.2 1.0 15,030 

4P 14,520 18,130 16,520 14,970 1.2 1.0 16,520 

4PA 14,190 17,940 16,710 15,160 1.3 1.1 16,580 

4C 15,810 19,100 18,650 16,520 1.2 1.0 18,060 

4CA 16,390 20,000 18,970 16,520 1.2 1.0 18,520 

4F 13,680 16,520 16,060 14,710 1.2 1.1 15,740 

4FA 14,320 17,230 16,970 15,420 1.2 1.1 16,520 

4S 9,680 14,130 14,130 13,290 1.5 1.4 13,810 

4SA 11,290 15,740 15,740 14,710 1.4 1.3 15,420 

5P 14,970 16,970 16,520 13,870 1.1 0.9 15,810 

5PA 14,710 16,840 14,970 12,390 1.1 0.8 14,710 

5C 17,420 19,100 17,420 14,710 1.1 0.8 17,100 

5CA 17,100 18,840 16,650 13,350 1.1 0.8 16,320 

5F 14,320 16,520 15,160 13,480 1.2 0.9 15,030 

5FA 15,290 16,840 15,420 13,100 1.1 0.9 15,100 

5S 11,290 14,130 13,870 11,870 1.2 1.1 13,290 

5SA 12,390 16,060 14,970 12,650 1.3 1.0 14,580 

6P 5,680 18,390 17,940 15,810 3.2 2.8 17,350 

6PA 13,870 18,130 17,230 14,840 1.3 1.1 16,710 

6C 9,480 20,390 18,840 16,710 2.1 1.8 18,650 

6CA 15,740 20,390 18,520 15,420 1.3 1.0 18,060 

6F 7,100 17,680 16,260 14,970 2.5 2.1 16,320 

6FA 15,610 18,390 17,420 15,420 1.2 1.0 17,100 

6S 7,870 15,610 14,710 14,320 2.0 1.8 14,900 

6SA 13,160 17,230 15,940 14,450 1.3 1.1 15,870 

Unit conversions: 

1 mm2

 = 0.00155 inch2
70 

Table 18. Minislump test data for round 2. 

Mix 

Pat Area 

(mm2 at time, min) 

False Set 

Index 

Stiffening 

Index 

Average 

Pat Size 

(mm2

) 

Round 2a 2 5 10 30 

2P 6,580 10,580 12,770 12,390 1.1 0.9 11,940 

2C 16,060 17,550 16,970 15,480 1.2 1.0 16,710 

4P 13,810 17,230 15,940 14,650 1.2 0.9 15,940 

5P 14,320 16,390 15,290 12,710 1.1 0.9 14,770 

2PDA 7,290 14,190 11,480 7,550 1.1 0.9 11,100 

2CDA 13,940 16,580 13,940 10,710 1.1 0.9 13,740 

4PDA 10,000 15,740 13,810 10,580 1.2 1.1 13,350 

5PDA 9,940 13,290 9,480 6,650 1.2 1.1 9,810 

Round 2b 2 5 10 30 

2PB 12,000 12,390 8,710 5,290 1.1 0.9 8,770 

2CB 16,520 19,350 16,770 11,680 1.2 1.0 15,940 

4PB 13,870 16,390 14,520 12,000 1.2 0.9 14,320 

5PB 12,650 12,000 8,260 4,840 1.1 0.9 8,390 

1PB 14,650 18,520 15,940 13,350 1.1 0.9 15,940 

1CB 19,870 21,480 19,870 16,970 1.1 0.9 19,420 

6PB 18,130 19,610 17,810 14,130 1.2 1.1 17,160 

Unit conversions: 

1 mm2

 = 0.00155 inch2

As expected, sample 1P cement set much faster than the blends, and sample 1C blend showed the 

most extended setting by about 3 h. The amount of bleed water was about twice as much for the 

blends than it was for the pure cement. 

Sample 2P was the first cement to indicate false set as a result of plaster converting to gypsum, 

which caused the 5- and 10-min pat areas to be smaller than the 2-min pat (figure 8). Previous 

analysis of the cement showed it to contain mostly plaster with very little gypsum (table 2). 

Judging from the increasing size of the paste pats from 2 to 30 min, it is apparent that this 

conversion was slow and appeared to reach completion after about 10 min. The overall size of 

the paste pats of the cement and the blends made from it were slightly smaller than that of 

sample 1P and its blends, suggesting higher water demand for sample 2P cement. The early 

stiffening tendency and higher water demand of sample 2P most likely results from its high 

plaster content, and also its high C3A and alkali contents. The blend made with Class C fly ash 

also appeared to show the most workable paste mix. 

As with the previous cement, sample 2P cement set faster than its blend with sample 2C blend, 

which showed the most retardation. The bleeding capacity of the blends was similar to that of the 

pure cement. 
71 

 Unit conversions: 

 1 mm2

 = 0.00155 inch2

Figure 8. A plot of minislump data for mixtures tested in round 2. 

Sample 3P cement was another case of early stiffening resulting from plaster-to-gypsum 

conversion (figure 9). As with sample 2P cement, sample 3P cement also had a high plaster 

content; however, the conversion of plaster to gypsum in sample 3P cement appeared to occur 

much faster. It was completed in about 5 min (paste pat size is at maximum), and it appeared to 

be more severe than sample 2P cement, judging from its much higher FSI value. 

The pastes made from the blends showed similar false setting trends as the pure cement. All 

pastes made with the blends were more workable, set longer, and bled more than the pure 

cement. The paste made with the blend containing Class C fly ash was again noticeably more 

workable than the other blends. 

0

5000

10000

15000

20000

25000

0 10 20 30

Time, min

Area, mm2

2P 2PA 2C 2CA

2F 2FA 2S 2SA
72 

 Unit conversions: 

 1 mm2

 = 0.00155 inch2

Figure 9. A plot of minislump data for mixtures tested in round 3. 

The minislump data for sample 4P cement gave all indications that the cement had a low water 

demand with practically no early stiffening tendency (figure 10). Analysis of the cement showed 

it to contain mainly gypsum as the calcium sulfate source present, with only minor amounts of 

plaster. The cement was also found to be high in C3A, but it was apparent that its early hydration 

reactions were being properly controlled largely by gypsum. 

Only the blend made with Class C fly ash gave a more workable paste than the cement. The 

other blends produced pastes of about the same workability, and in the case of the sample 4S 

blend, the paste was somewhat less workable. 

As observed in the previous cements, sample 4P cement set sooner and bled less than its blends. 

0

5000

10000

15000

20000

25000

0 10 20 30

Time, min

Area, mm2

3P 3PA 3C 3CA

3F 3FA 3S 3SA
73 

 Unit conversions: 

 1 mm2

 = 0.00155 inch2

Figure 10. A plot of minislump data for mixtures tested in round 4. 

As with sample 4P cement, sample 5P cement showed no indications of early stiffening resulting 

from false set. The size of paste pats from 2 to 30 min suggested the cement had a normal water 

demand (figure 11). This is consistent with previous analysis showing the cement to contain a 

moderate amount of C3A with mostly gypsum and very little plaster. As observed in previous 

cements, the blend made with Class C fly ash gave the most workable paste mix, and the one 

containing the granulated slag was the least workable. 

Setting time was found to be earliest for the pure cement and latest for the blends containing 

Class C fly ash. Again, the pure cement bled the least with the blends showing about twice the 

bleeding capacity. 

0

5000

10000

15000

20000

25000

0 10 20 30

Time, min

Area, mm2

4P 4PA 4C 4CA

4F 4FA 4S 4SA
74 

 Unit conversions: 

 1 mm2

 = 0.00155 inch2

Figure 11. A plot of minislump data for mixtures tested in round 5. 

Sample 6P cement is another cement that shows indications of early stiffening resulting from 

false set because of the plaster-to-gypsum conversion (figure 12). However, after remixing, the 

cement paste became very fluid, indicating a normal water demand based on the very large pats 

from 5 to 30 min. Part of the reason for the very low water demand of sample 6P cement was 

likely its very low C3A content. As observed in the previous cements, the blend made with 

Class C fly ash gave the most workable mix. Both blends made with Class F fly ash and 

granulated slag were somewhat less workable than the pure cement. The lower workability of the 

slag blend could be explained in terms of the angular nature of the slag particles. For the blend 

containing Class F fly ash, one explanation may involve its finer particle size and distribution. 

As with the other previous five cements, sample 6P cement had shorter setting time and less 

bleed water than its blends. 

0

5000

10000

15000

20000

25000

0 10 20 30

Time, min

Area, mm2

5P 5PA 5C 5CA

5F 5FA 5S 5SA
75 

Unit conversions: 

1 mm2

 = 0.00155 inch2

Figure 12. A plot of minislump data for mixtures tested in round 6. 

Effects of Chemical Admixtures. The results of minislump tests conducted in rounds 3 and 4 

are shown in table 19. The use of the lignin-based chemical admixture provided some benefit of 

water reduction to only samples 1P and 3P cements and their respective blends, estimated 

roughly at around 3 percent water reduction. The rest of the cement and blends were either 

unchanged or may have suffered slight loss in early workability. Of the three cements found to 

show rapid stiffening, two cements (2P, 6P) indicate incompatibility with the chemical 

admixtures, as shown by the paste slump loss from 5 to 30 min that more resembles flash set 

than false set. Sample 3P cement, which was found to have the most severe false setting 

tendency earlier, is shown to have the most benefit with admixture addition. The positive effect 

of lignin-based admixture on sample 3P cement may be explained as the result of (1) rapid 

conversion of plaster to gypsum taking place as the paste is being mixed, or (2) the admixture is 

causing a delay in the delay of this conversion process beyond 30 min. Further observation of the 

paste at later ages beyond 30 min favors explanation (1). 

0

5000

10000

15000

20000

25000

0 10 20 30

Time, min

Area, mm2

6P 6PA 6C 6CA

6F 6FA 6S 6SA
76 

Table 19. Minislump test data for round 3 and 4. 

Mix 

Pat Area 

(mm2

 at time, min) 

False Set

Index 

Stiffening 

Index 

Average Pat 

Size 

Round 3 2 5 10 30 

5P 10,390 10,390 8,190 5,230 1.1 0.9 7,940 

5PA 12,260 12,060 9,100 6,390 1.2 1.0 9,160 

5PB 9,160 7,420 4,840 3,810 1.2 0.9 5,350 

2PA 9,740 9,740 6,130 5,350 1.1 0.9 7,100 

1PA 15,100 18,390 16,900 14,650 1.1 0.9 16,650 

1PB 16,260 18,000 15,610 12,190 1.1 0.9 15,290 

1CA 17,680 19,740 16,650 11,550 1.2 1.1 16,000 

6PA 13,100 17,680 14,900 11,160 1.2 1.1 14,580 

2CA 13,810 13,810 10,060 5,680 1.5 2.1 9,870 

2FA 12,900 12,060 9,480 6,840 0.9 0.6 9,480 

2CDA 10,060 9,290 5,100 3,350 1.1 0.9 5,870 

1CB 16,650 17,680 12,320 5,870 1.1 0.8 11,940 

Round 4 2 5 10 30 

2CA 17,550 20,520 21,030 18,520 1.1 0.9 20,000 

2FA 17,940 20,580 20,130 14,520 1.2 1 18,450 

2CDA 15,610 19,290 19,870 17,810 1.2 0.9 18,970 

1CB 21,030 23,230 22,320 20,710 1.1 0.9 22,060 

1PA 17,100 18,390 18,130 15,810 1.1 0.9 17,480 

1PB 17,230 17,810 17,940 15,740 1.1 0.9 17,160 

1CA 17,230 23,350 22,710 20,840 1.2 1.1 22,320 

6PA 13,100 17,680 14,900 11,160 1.2 1.1 14,580 

 Unit conversions: 

1 mm2

 = 0.00155 inch2

In general, the addition of lignin-based admixture caused longer setting times and more bleed 

water for the cements and their blends, which is a direct result of some retardation of the 

hydration reactions by the clinker phases, especially C3S. All blends made with Class C fly ash 

showed the longest setting time and the most bleed water. 

Further testing was done on three cements and one blend that exhibited early stiffening tendency 

to evaluate the effect of double dose of the lignin-based admixture. The results are shown in 

table 19. As the results indicate, the double dose addition of lignin-based admixture did very 

little to prevent the early stiffening tendencies of the cements and the blend. In fact, it made the 

condition worse—the double dose addition resulted in greater slump loss from 5 to 30 min when 

compared with single dose admixture addition. The double dose addition also resulted in much 

longer setting times accompanied with excessive amounts of bleed water. 

Sugar-based admixture at a dosage rate of 163 ml/100 kg (2.5 oz/cwt) was also tried on the same 

set of three cements and one blend. The results given in table 19 are very similar to those 

obtained with the lignin-based admixture. No benefit of water reduction was achieved by the 

addition of sugar-based admixture. All pastes containing sugar-based admixture showed longer 

setting times accompanied by more bleeding. When added to the normal sample 6P cement, the 

sugar-based admixture was also found to have very little benefit in providing water reduction. 
77 

Effects of Temperature. The study on the effects of temperature was carried out at 32 °C 

(90 °F) and 10 °C (50 °F), to simulate summertime and fall concreting (table 9). The cements 

and blends used for evaluation were selected on the basis of their rapid or normal stiffening 

tendencies, plus the slow setting properties found earlier. The results are shown in round 3 and 

round 4 test results. As expected, all pastes made at 32 °C (90 °F) are less workable than those 

prepared at 23 °C (70 °F). This is the result of accelerated hydration of the clinker phases, 

especially C3A. Conversely, hydration reactions are slowed at 10 °C (50 °F), resulting in pastes 

of high workability. 

At 32 °C (90 °F), the pastes took much shorter times to set as a direct result of higher reaction 

rates and formation of more hydration products. In contrast, pastes prepared at 10 °C (50 °F) 

were slower to set and were accompanied with more bleeding, which resulted from the hydration 

process being slowed down by a lower temperature. 

Effects of Class C Fly Ash. In all cases, the Class C fly ash-containing blend shows higher 

slump loss from 5 to 30 min than that of the pure cement, sample 1P. The greater slump loss of 

the blend that seems to become more severe at lower w/c ratios appears to be related to some 

early reactions outside of the cement clinker-phase hydration reactions. Earlier analysis of 

Class C fly ash showed it to contain reactive components that include C3A estimated as 11.4 

percent by weight of the fly ash. Anhydrite (CaSO4) was also detected in the fly ash at an 

estimated amount of 4 percent. With this level of C3A in the Class C fly ash coupled with the 

form of calcium sulfate (anhydrite) present, the higher slump loss observed in all 1C blend pastes 

may be related to the inadequate control of C3A hydration. 

Effects of Water-to-Cementitious Materials Ratio. Some mixes were added to address the 

issue of Class C fly ash reactivity in blends at lower w/c ratios. These paste mixes were prepared 

using w/cm=0.50, 0.42, 0.40, and 0.37. The results are shown in table 20. 

Table 20. Minislump test data for investigating effect 

of w/cm. 

w/cm 

Pat Area 

(mm2 at time, min) 

False Set

Index 

Stiffening 

Index 

Average 

Pat Size 

Mix 1C 2 5 10 30 

0.37 8,840 7,420 6,390 3,420 1.1 0.9 5740 

0.40 12,260 11,290 10,770 8,320 1.2 1.0 10,130 

0.42 14,130 13,870 12,260 9,480 1.2 0.9 11,870 

0.50 17,940 20,840 19,610 16,710 1.1 0.9 19,030 

 Unit conversions: 

1 mm2

 = 0.00155 inch2

NIST Minislump Test 

The minislump tests conducted at NIST aimed at identifying silicate-based stiffening effects 

indicate the following observations (tables 21 to 23): 
78 

• Extremely short times to reach a small (48-mm (1.9-inch) diameter) pat size were 

recorded for most combinations of Cement 2. The exceptions were with no 

admixture present and at high water-reducer dosage with Class C fly ash. 

• Shortened times were reported for the combinations of Cements 4 and 5 containing 

water reducer at 21 °C (70 °F). 

• Cements 1 and 6 showed normal/extended times. 

These observations are consistent with other test methods that indicate stiffening caused by 

silicate reactions. 

Table 21. NIST test data for round 1.

Mix 

Pat Size 

(mm at time, min) 

Time to 

reach 

48 mm, 

(min) 

Slope 

(mm/min)

 15 30 60 90 120 

1PA 79.5 71.3 67.3 60.5 57.9 * −0.187 

1CA 87.5 73.6 63.9 58.4 58.4 * −0.340 

1FA 83.1 76.5 71.4 69.4 63.1 305 −0.123 

1SA 76.4 73.4 73.4 73.3 69.1 304 −0.102 

2PA 46.0 44.0 44.0 44.0 * 13 −0.125 

2CA 57.9 50.9 48.1 * * 64 −0.198 

2FA 50.1 53.4 49.5 51.3 53.3 197 −0.013 

2SA 53.9 51.8 49.4 48.8 48.3 123 −0.072 

3PA 64.9 60.0 57.4 54.5 53.3 185 −0.110 

3CA 71.0 66.6 59.4 58.5 57.9 307 −0.071 

3FA 71.0 66.5 62.0 53.6 54.9 183 −0.132 

3SA 62.4 61.8 59.3 57.9 52.4 243 −0.073 

4PA 64.3 58.0 50.5 48.5 * 94 −0.198 

4CA 76.0 64.0 58.4 55.3 52.5 184 −0.144 

4FA 71.5 65.0 56.9 52.4 51.4 180 −0.142 

4SA 65.6 59.4 56.3 53.0 49.5 186 −0.103 

5PA 61.9 53.6 49.0 48.1 * 94 −0.160 

5CA 74.1 56.5 56.1 49.1 47.8 123 −0.206 

5FA 65.1 61.0 55.3 53.4 51.5 187 −0.108 

5SA 68.8 65.0 54.1 55.9 52.1 243 −0.094 

6PA 78.4 65.6 61.6 59.9 54.0 242 −0.128 

6CA 82.5 65.8 60.9 56.5 52.5 243 −0.129 

6FA 81.5 70.5 69.1 69.9 65.6 363 −0.094 

6SA 75.0 65.3 66.5 64.5 60.0 424 −0.064 

Note - * = No data recorded 

Unit conversions: 

1 mm2

 = 0.00155 inch2
79 

Table 22. NIST test data for round 2. 

Mix 

Pat Area 

(mm2 at time, min) 

Time to 

reach 48 

mm (min)

Slope 

(mm/min)

Round 2A 15 30 60 90 120 

2P 52.3 51.3 49.0 48.1 47.0 123 −0.047 

2C 69.9 65.5 60.6 58.1 56.0 305 −0.065 

4P 76.3 69.3 62.8 56.5 51.3 183 −0.188 

5P 70.6 63.0 60.0 53.4 48.9 125 −0.157 

2PDA 47.0 47.8 47.1 45.8 * 13 −0.034 

2CDA 74.9 70.5 61.9 56.0 52.5 423 −0.057 

4PDA 56.9 50.6 48.9 45.8 * 93 −0.126 

5PDA 57.3 48.4 46.3 * * 64 −0.193 

Round 2B 15 30 60 90 120 

2PB 46.1 44.5 * * * 13 −0.061 

2CB 62.3 51.8 47.0 45.6 * 64 −0.273 

4PB 66.9 59.6 52.8 50.8 49.5 182 −0.121 

5PB 58.5 49.8 49.0 48.0 44.8 124 −0.104 

1PB 78.3 70.4 66.5 64.8 63.0 304 −0.105 

1CB 88.1 74.5 67.3 62.5 58.5 362 −0.101 

6PB 78.8 65.8 61.0 57.6 57.0 304 −0.099 

Note - * = No data recorded 

Unit conversions: 

1mm =0.0394 inch 

1 mm2 = 0.00155 in2
80 

Table 23. NIST Test Data For Round 3 and 4.

Mix 

Pat Area 

(mm2

 at time, min) 

Time to 

reach 48 

mm 

(min) 

Slope 

(mm/min)

Round 3 15 30 60 90 120 

5P 69.9 59.6 55.3 51.3 48.5 184 −0.148 

5PA 58.0 53.6 51.1 49.5 48.4 187 −0.065 

5PB 60.0 50.8 49.5 48.3 46.4 124 −0.102 

2PA 43.3 * * * * 12 *

1PA 76.0 71.0 65.9 65.8 60.4 304 −0.110 

1PB 77.0 71.0 68.6 65.8 64.8 335 −0.086 

1CA 81.9 69.0 61.0 57.1 55.4 304 −0.082 

6PA 78.3 69.8 67.5 56.1 51.5 184 −0.205 

2CA 59.3 56.8 51.3 48.4 46.0 123 −0.123 

2FA 50.5 51.3 49.6 49.3 48.8 183 −0.029 

2CDA * * * * * * *

1CB 91.5 75.8 70.0 64.1 61.3 363 −0.249 

Round 4 15 30 60 90 120 

2CA 59.0 55.8 55.1 49.4 46.8 123 −0.100 

2FA 64.0 53.8 54.4 52.5 50.8 183 −0.059 

2CDA 93.6 84.8 77.6 68.5 61.4 365 −0.237 

1CB 90.5 74.9 72.8 64.8 60.3 303 −0.111 

1PA 81.0 75.9 72.3 66.5 60.1 244 −0.166 

1PB 82.9 73.0 68.8 66.0 62.3 244 −0.142 

1CA 93.5 82.9 71.1 67.3 62.6 302 −0.126 

6PA 87.5 81.0 76.8 70.1 62.5 186 −0.199 

Note - * = No data recorded 

Unit conversions: 

1mm =0.0394 inch 

1 mm2

 = 0.00155 in2

Rheology 

Rheological methods for cement paste were investigated for their potential to identify 

incompatibilities between pavement materials. The logic behind this approach is that the main 

incompatibility problems occur between the cement, chemical admixtures, and supplementary 

cementitious materials. The advantage is that cement paste testing needs small amounts of 

materials, and it is less labor intensive than tests performed on concrete. 

The rheology-based method to measure yield stress uses the stress-growth procedure. The 

cement paste is sheared at a very low shear rate (the lowest possible with the rheometer used) 

and the shear stress is measured. The shear stress increases linearly with time until the yield 

stress is reached (figure 13). At that point, the shear stress reaches a peak and then decreases. 

The linear portion is caused by the elastic response of the viscoelastic material. After the yield 

stress is reached, the material flows, and the reduction in shear stress is measured. The plot of the 
81 

yield stress versus the time (figure 14) will gradually increase until initial setting is reached. 

After initial setting is reached, the shear stress will increase very fast until the rheometer can no 

longer measure flow because the shear stress is too high. 

Point A, the end of the linear (elastic) portion, is the yield stress point. 

Point B, the peak point, is taken as an approximation of the yield stress 

because it is more readily identified. 

Figure 13. Stress growth measurement. 

Note: These data are presented to illustrate the method, and they 

were not produced with the project materials. 

Unit conversions: 

1 kPa = 0.145 psi 

Figure 14. Typical plots of yield stress versus time for 

accelerated, untreated, and retarded cementitious systems. 

Time

Stress

A

B

A

B

0

2000

4000

6000

8000

10000

12000

14000

0123456

Time, hours

Yield Stress, Pa

Retarded

Normal

Accelerated
82 

Figure 15. A photograph of the rheometer used at NIST. 

The cement pastes were mixed with a blender for 10 s before being placed in the rheometer 

(figure 15). The rheometer is somewhat specialized, and it may require expert operation and 

interpretation. It does have the advantage of being relatively quick to run, and a number of 

cementitious systems can be compared in a single day. This makes it useful for materials 

prequalification work. Many State DOTs reportedly own the equipment for use in testing asphalt, 

and a small interchangeable modification is required to make it suitable for use with cementitious 

pastes. As shown in figure 3, the initial setting times determined using this test method were 

generally consistent with those found by other methods. Of more interest is that the slope of the 

yield stress/time plot determined for the cementitious systems could be used to predict the 

systems that were rapid setting or very reactive (table 9, final column). The systems that were 

indicated as rapid stiffening included many of those made with cements 2, 4, and 5, without 

supplementary cementing materials. This is consistent with the calorimetry data discussed in 

detail above. The method is useful for detecting problems related to the silicate reactions. 

Mortar Cube Strength 

Mortar cubes were prepared in accordance with ASTM C 109 except that mix proportions were 

at a fixed w/cm (0.5), and water-reducing admixture was included as required in the test matrix. 

Flow was recorded but not fixed or adjusted. The cubes were tested for compressive strength at 

24 h (table 9). 

A loose correlation was observed between the 24-h cube strength and the magnitude of the 

silicate peak in calorimetry tests. This is not surprising because both effects are governed by the 

early reactivity of the silicates. The strengths may be influenced by the following conditions: 
83 

• Setting time—retardation would suppress early strength. 

• Air content—decreasing strength with increasing air. 

It was considered that there were too many confounding effects and a lack of reliability to make 

this a useful approach for indicating incompatibility. 

Air Content 

The amount of vinsol air entraining admixture required to achieve an air content of 18 percent 

was determined in accordance with ASTM C 185, except that the mix proportions were fixed as 

discussed above. 

Little correlation was found between mortar air content and other test data except the 24-h cube 

strength as discussed in table 9. 

Stiffening 

Stiffening was assessed by testing according to a modified version of ASTM C 359. 

Modifications were to use the same mix proportions as the rest of the paste work in this project, 

and room temperatures were controlled at 21, 32, or 10 °C ± 3 (70, 90, or 50 °F ± 5) and paste 

temperatures were not recorded (table 9). 

It is notable that the systems that were indicated by this test to be false setting were not always 

the same as those indicated by the minislump test. In general, the systems that were indicated to 

be potentially problematic were those containing cements 2, 4, and 5, all of which have been 

similarly problematic in other test methods including time of setting, calorimetry, and minislump 

pat area. 

A variation of this test method is being developed by the ASTM subcommittee (09-48) on 

incompatibility at ASTM for this application. Work is ongoing in this committee to refine the 

method and provide guidance on interpreting the data. 

Pore Solution Chemistry 

Following is a summary of the introduction and conclusions of the pore solution chemistry 

analyses. 

Introduction 

Depending on initial time of setting for different mixes, extractions were done on either plasticstate or hardened-state paste. Mixing procedure for the paste was adapted from that described in 

the report, Early Stiffening Test Development for Portland Cement.

(82) This method of mixing 

cement paste was also used for the minislump testing. Chemical analysis of the pore solution 

collected was conducted for sodium, potassium, calcium, and sulfate ion, as well as pH 

measurement. 
84 

Paste samples were mixed with water at w/cm of 0.5, and solutions extracted in either the plastic 

or hardened state at 5, 10, 30, 60, 360, and 1,440 min after mixing. Samples were taken from all 

four rounds of testing. 

Paste mixing: Paste was mixed in a blender at 10,000 rpm for 90 s counting from the moment all 

cement and admixture were added to the water. Mixing proportions used were 500 g (17.6 oz) of 

cementitious material, 250 ml (8.5 oz) of water, and varied amounts of WRA admixture. 

Admixtures were measured and emptied into the mixer using 5-ml (0.17-oz) plastic syringes and 

dosed at single and double dosages recommended by the manufacturer. Lignin-based WRA A 

was dosed at 325 and 650 mL/100 kg (5 and 10 oz/cwt) of cementing material. Sugar-based 

WRA B was dosed at 163 mL/100 kg (2.5 oz/cwt) of cementing material. A w/cm of 0.5 was 

used in all paste mixes. 

Because of the different effects on paste consistency experienced on initial time of setting and 

early stiffening by using different extraction conditions such as time after mixing, combination 

of materials, and mixing temperature, the solution extractions were performed either in plastic 

state where the sample was poured into disposable centrifuge tubes, or in hardened state where 

samples were cast in small cylinder molds. 

Extractions during plastic state. An analytical centrifuge machine was used to extract solution 

before the cement paste reached initial set. The centrifuge machine was equipped with a 115-

volt, 1.5-amp, 60-Hertz (Hz) motor, and it had a total capacity of six tubes. Plastic centrifuge 

tubes with a gradation scale and a total capacity of 15 ml (0.5 oz) were used. 

Minimum extraction times were determined previously to obtain between 10 and 15 ml (0.3 and 

0.5 oz) of solution. The extraction times were 1 min for very fluid paste and 3 min for less fluid 

paste. A funnel was used to put the paste in the six centrifuge tubes; and where the paste would 

not flow easily, a vibrating table was used. Twelve tubes were filled in with paste to obtain the 

desired amount of liquid from paste mixes that had not yet reached initial set but showed 

significant stiffening at 6 h after mixing. 

Extractions during hardened-state. An extraction method for squeezing solution out of 

hardened cement paste was adopted from previous research studies at Purdue University.(83) A 

die and piston manufactured of steel and designed to carry loads of up to 1,330 newtons (N) 

(300,000 lb) of force, “squeezed” the pore liquid by applying pressure to the paste specimen. 

Liquid was collected through grooves in the base and carried out into test tubes tube using 

flexible tubing flushed with nitrogen gas. Specimens used for this extraction technique were 

discs cast in 50-mm (2-inch) diameter by 19-mm (.075-inch) height disc cylinders that provided 

a tight seal. An illustration of the press die set is shown in figures 16 and 17, showing in figure 

16 the paste specimen and the cylindrical chamber before introducing the disc and applying the 

pressure. Normally four to five disc specimens were required to obtain the desired volume of 

liquid. 

Chemical analysis. After the extraction, samples were sealed and kept in the refrigerator before 

analysis the next morning. After refrigeration, samples were allowed to reach room temperature, 

pH was measured, and solutions were acidified to minimize potential changes in chemical 

composition resulting from carbonation. Samples were analyzed within the next 24 h for sulfate, 
85 

calcium, sodium, and potassium concentration. Sulfate analyses were done according to 

ASTM C 114 wet method for chemical analysis, determined by the gravimetric method after 

precipitation with reagent-grade barium chloride. Calcium, sodium, and potassium analyses were 

done using Atomic Absorption Flame Emission Spectroscopy (AAS) using a spectrometer. 

Sample preparation in most cases did not require more than 10 times dilution of the original 

volume, and in no case exceeded 100 times. Concentrations were calculated in mg/L of solution 

and used in parts per million (ppm) for data reduction and analysis. 

Figure 16. Die set for squeezing 

pore solution from hardened 

cement paste specimens. 

Figure 17. Pore fluid being 

collected from die set. 

SUMMARY 

The setting or stiffening behavior of hydrating portland cement or cements with SCMs during the 

first 10 min after mixing is generally attributed to the reactions involving C3A and the sulfate 

from the added gypsum and from alkali sulfates in the clinker. In cases when the system is not in 

balance with respect to these reactions, changes in rheology of the mixture may result, and the 

mixture may exhibit early stiffening, false set, or flash set. False set is related to precipitation of 

gypsum because of a high concentration of sulfate in the pore solution. Flash set, the result of too 

little sulfate available in the pore solution, is caused by formation of C3A hydrates instead of 

ettringite, which is the normal hydration product. 

Early after mixing, the concentration of the constituent ions in the pore solution varies according 

to the specific cement. For example, in cements high in alkali sulfates, the concentration of 

sulfate ions as well as alkali ions will be high. At the same time the hydration of the C3S will 

contribute calcium ions as well as hydroxyl ions to the pore solution. In special cases where the 
86 

concentrations of sulfate and calcium ions are high, the pore solution can be supersaturated with, 

for example, gypsum, and this may cause gypsum to precipitate. The criterion for this is whether 

the so-called solubility product for gypsum is higher than that corresponding to gypsum in 

equilibrium with the pore solution, which in this case is said to be saturated with respect to 

gypsum. The solubility product of gypsum is calculated according to the equation in figure 18. 

Kgyp=[Ca2+][SO4

2-

] 

Figure 18. Equation. Solubility product of gypsum. 

Where [Ca2+] and [SO4

2-] are the concentrations of calcium ions and sulfate ions respectively in 

the pore solution. Solubility products for other compounds can be calculated in similar ways, and 

for saturated solutions, the solubility products at a given temperature are constants specific for 

the considered compound. Strictly, another term, “activity,” should be used rather than the term 

“concentration.” “Activity” takes into consideration the presence of other ionic constituents of 

the pore solution; therefore, the term “ion activity product” (IAP) is used rather than the term 

“solubility product.” For gypsum, this term is expressed as the equation in figure 19. 

IAPgyp = (Ca2+)(SO4

2-

)

Figure 19. Equation. Ion activity product of gypsum. 

Where (Ca2+) and (SO4

2-) respectively are the activities of the calcium ions and sulfate ions of 

the pore solution, and these can be calculated from the total composition of the pore solution. 

One way to characterize the pore solution regarding possible supersaturation with, for example, 

gypsum or other constituents, is to define the saturation factor, SF, as the ratio between the actual 

IAPgyp of the pore solution and the corresponding value for the saturated condition. 

SF values larger than 1 indicates supersaturation, SF = 1 corresponds to the saturated solution, 

and for SF smaller than 1 the solution is undersaturated. A crystal cannot exist in a solution with 

SF < 1; it is not stable, and it will dissolve. In a solution with SF > 1 it will grow; it cannot 

dissolve. 

For the selected systems, the saturation factors for gypsum (CaSO4•2H2O), SFgyp, syngenite 

(K2Ca(SO4)2•H2O), SFsyn, and calcium hydroxide (Ca(OH)2), SFCH, were studied. Syngenite is a 

potassium-calcium-sulfate that can precipitate in systems with cements with high sulfate and 

potassium concentrations. 

For cement pastes of grey and white portland cement, it is known from the literature that SFgyp

and SFsyn can be larger than 1 for up to about 10 h or later and SFCH is larger than 1 for up to 28 

days or more.(84,85) The supersaturation of gypsum is related to the dehydration of gypsum to 

hemihydrate (plaster of paris) in commercial cements during grinding. The plaster is much more 

soluble than gypsum, and it can deliver sulfate to the pore solution faster than it can be consumed 

by the reaction with C3A phase. Extra sources of sulfate such as alkali sulfates also can 

contribute to supersaturation. The reason for the prolonged super saturation of calcium hydroxide 

is probably the continued hydration of C3S and C2S. 
87 

Water reducers are in many ways similar to retarders. Taylor makes references to work showing 

that calcium ion concentration and hydroxyl ion concentrations increase in pore solution when 

such chemical admixtures are used.(53) The mechanism is probably that they modify the reaction 

products by being adsorbed and allow the calcium ion concentration in solution to be higher than 

in pore solutions with the unmodified hydration product. 

For the four systems 2P, 2C, 4P and 5P (no admixture) considered “early stiffening” at 21 °C 

(70 °F), the SFgyp values for 2P, 2C, and 5P were similar ~6.5, and for 4P it was ~2.5 without any 

significant change up to 360 min. After this time, all values decreased to below 1, signaling all 

gypsum has been consumed. During the period from mixing until 360 min, the SFgyp values 

indicate supersaturation, and hence, a potential for precipitation of gypsum with possible effect 

on the workability. The supersaturation in 4P is lower than in the other systems, and it would be 

expected that this system would show less early stiffening compared to the others. 

In the SFsyn system, 4P is again the lowest—around 1 up to 10 min and then for later times 

smaller than 1, indicating no presence of syngenite. This makes sense because cement 4P is low 

in potassium. The other systems all have SFsyn higher than 10, indicating potential for 

precipitation of syngenite, which can cause the same effects as precipitation of gypsum. Because 

syngenite is a sulfate-bearing phase, it might compete with the C3A for the sulfate ion in the pore 

solution and cause flash set.(53)

Regarding calcium hydroxide the SFCH values for 4P again is the lowest of the set, with values 

from 2.5 increasing to about 10 at 360 min, after which time it decreases but maintains values>1. 

The other systems have values from around 9 increasing to 26 at 360 min. As mentioned above, 

the pore solution is expected to be supersaturated by calcium hydroxide for some time after 

mixing; but, the individual differences in supersaturation cannot be explained at this time. The 

reasons can be many—different reactivity of the clinker minerals of the cement contributing 

calcium ions and hydroxyl ions at different rates to the pore solution, effect of alkalis on the 

calcium ion concentration, or different ratios between calcium and silica in the calcium-silicatehydrate formed during the early hydration process. 

Addition of water reducers A and B (single (A) and double dosage (DA) of A and single dosage 

of B) generally resulted in an increase of the hydroxyl ion concentration of the pore solution for 

all systems and in calcium ion concentration except for 4PA and 4PDA. The SFgyp for 4PA and 

4PDA was not changed significantly, but for the other systems it increased with progressive 

addition of water reducer A. Addition of B had a similar effect as addition of a single dosage A. 

This indicates increasing tendency for early setting with increasing addition of water reducer. For 

SFsyn the addition of water reducers had similar effects. 

For SFCH, the addition of water reducer had an effect for all systems: The SFCH increased with 

increasing addition. The increases in SF values are in line with the findings reported in literature 

referred to above; however, the effect of the supersaturation with respect to calcium hydroxide 

on the early stiffening behavior is not understood. 

One set considered “Fast Stiffening”—(2PA, 5PA, 5PB, and 5P) and a set considered 

“Normal”—(1PA, 1CA, 1PB, and 6PA) at 21 °C (70 °F), were also tested at 32 °C (90 °F). Up to 

60 min after mixing, the “Fast Stiffening” systems had higher SFgyp and SFsyn values than the 
88 

“Normal.” The “Fast Stiffening” had SFgyp > 5 and the “Normal” < 3. Changing the temperature 

from 21 to 32 °C (70 to 90 °F) had only a small effect on the level of individual SF values until 

about 60 min after mixing. Then the SFgyp and SFsyn values decreased to less than 1 for the 32 °C 

(90 oF) treated systems. This indicates the following: 

• The “Fast Stiffening” systems have higher potential for precipitation of gypsum and 

syngenite with the possible effects on workability and early stiffening behavior. 

• The higher temperature accelerates hydration of C3A, and hence, the consumption of 

gypsum is at a much earlier time. For both the “Fast Stiffening” and “Normal” sets, 

this will lead to shorter setting time in general. 

The SFsyn values for the “Normal” are around or below 1 in all cases, indicating the nonexistence 

of syngenite, and hence, no negative effect of this phase on the rheology. For the SFCH no clear 

tendency was observed other than the “Fast Stiffening” systems increased at 32 °C (90 °F) 

relative to 21 °C (70 °F). 

Four systems considered “Slow Stiffening” at 21 °C (70 °F)—2CA, 2FA, 2CDA, and 1B—

together with “Normal” systems mentioned above were tested at 10 °C (50 °F). Regarding the 

gypsum the SFgyp values for the “Slow” with the exception of 1B were around 10 to 14 and the 

“Normal” slightly lower. The effect of decreasing the temperature from 21 to 10 °C (70 to 50 oF) 

was a slight increase in SF values for the “Slow Stiffening” as well as the “Normal” set up to 

360 min after mixing. With the exception of 6PA, after this time, the SFgyp values for the 

“Normal” decreased to less than 1, indicating total consumption of gypsum; but the SFgyp values 

for the “Slow Stiffening” treated at 10 °C (50°F) remained almost unchanged at their levels 

larger than 1, indicating that gypsum was still present at 1,440 min after mixing. For the “Slow 

Stiffening” set, the SFsyn behavior was similar. The values for the system 1B indicated no 

existence of syngenite either at 21 or 10 °C (70 or 50 °F), which was also the case for the 

“Normal” systems. No clear trend could be observed regarding calcium hydroxide. 

The following list of findings is based on the study of saturation factors for gypsum, syngenite, 

and calcium hydroxide: 

• Addition of water reducers results in an increase in the saturation factors for gypsum, 

syngenite, and calcium hydroxide in the systems studied. 

• For “Fast Stiffening” systems tested at 32 °C (90 °F), the saturation factors for 

gypsum and syngenite were not affected until after 60 min after mixing comparing to 

those of samples tested at 21 °C (70 °F). After 60 min the 32 °C (90 °F) saturation 

factors decreased to below 1, indicating total consumption of gypsum. When tested 

at 21 °C (70 °F), this change took place after 360 min after mixing. 

• Testing “Slow Stiffening” systems at 10 °C (50 °F) had only minor effect on the 

saturation factors for gypsum and syngenite up to 360 min after mixing when 

compared to samples tested at 21 °C (70 °F). After 360 min the saturation factors 

decreased to below 1 for samples tested at 21 °C (70 °F), indicating the presence of 

gypsum at least up to 1,440 min after mixing. 
89 

• Comparing “Fast Stiffening” systems with “Normal” showed that the levels of 

gypsum saturation factors were highest for the “Fast Stiffening” systems. The 

difference in saturation factor values might be an indicator of whether a system could 

be considered fast or normal; however, when comparing “Normal” with “Slow 

Stiffening” systems, the gypsum saturation factors for the “Slow Stiffening” are 

slightly higher than for the “Normal.” Based on the present study, it is not possible to 

characterize early stiffening behavior based solely on pore-solution chemistry. 

Slump Loss 

Concrete Slump Loss. Three slump cones were prepared after the concrete mixtures had been 

mixed. The samples were covered to prevent moisture loss, and they were kept in a room 

controlled to the temperature selected (10, 21, or 32 °C (50, 70, or 90 °F)). Slumps were 

measured 15, 30, and 60 min after initial mixing in accordance with ASTM C 143. The data 

reported are the percentage slump losses at each time (100 percent meaning that slump has 

reached 0 mm (0 inch)). 

Some mixes had a slump of zero initially; therefore, valid slump loss data were not obtained. 

These included mixes containing cements 2 and 4 at 32 °C (90 °F). All mixes at 32 °C (90 °F) 

exhibited significant slump loss reaching zero slump within 30 min. At 21°C (70 °F), mixes 

made with cements 2, 4, and 6 had reached near zero slump in 30 min. Cements 1 and 5 were 

still showing some workability at this time. The rapid slump loss of cement 6, even from a high 

initial slump, is surprising because this is not consistent with the paste and mortar test results. 

The slump loss data are not consistent with other test methods and may be questionable for the 

following reasons: 

• The slump test is only appropriate for values between 12 and 225 mm (0.5 and 9 

inches), and therefore, values less than 12 mm (0.5 inch) are not reliable. Likewise, 

the precision of the test is approximately 25 mm (1 inch), therefore, a 100 percent 

slump loss from 25 to 0 mm (1 to 0 inch) is not necessarily meaningful. A number of 

mixes had a zero slump initially making the test meaningless. In paving, low slump 

mixes are required to prevent edge slump; therefore, the usefulness of this test may 

be limited in this application. 

• The approach used here was to test specimens that were undisturbed from the time of 

initial mixing. This was done to reduce variability induced by breaking up early 

hydration bonds that would influence slump; however, this approach is not typical of 

normal field handling of concrete, which is significantly disturbed during transport 

(even in a flat bed truck), placing, and compaction. 

Mortar Flow Loss. Samples of mortar were sieved from the same concrete mixtures used to 

determine concrete slump loss. Three mortar flow cones (ASTM C 1437) were filled and 

covered until tested at 15, 30, and 60 min after initial mixing. Similar to the concrete slump loss 

data, the results are presented as percentage reduction in flow at each time. 

Cement 2 at 21.1 °C (70 °F) exhibited relatively low slump loss at either temperature or 

admixture dosage. This is consistent with the minislump observations that show high risk of false 
90 

setting that is balanced with the use of water reducing admixture. Cement 5 exhibited significant 

loss of flow at 21.1 °C (70 °F) that decreased at the higher temperature or with increasing water 

reducer dosage. Cement 4 had a moderate slump loss at 32 °C (90 °F), but otherwise reasonably 

low slump loss at the other temperatures. Cements 1 and 6 did not exhibit much loss of flow over 

the time measured. These observations are consistent with other test methods that detect 

stiffening because of silicate reactions, and they appear to be more reliable than the concrete 

slump loss tests. 

Ultrasonic P-Wave 

Theory of Wave Propagation. Longitudinal (compression) waves, transversal (shear) waves, 

and surface (Rayleigh) waves are the three common types of stress waves that propagate through 

an elastic medium. The velocity of these waves depends on the elastic properties of the medium. 

The pulse velocity V of longitudinal stress waves in a concrete is related to its elastic properties 

and density according to the relationship expressed in the equation in figure 20. 

Figure 20. Equation. Pulse velocity. 

Where 

V= Wave velocity. 

E = dynamic modulus of elasticity. 

μ = dynamic Poisson’s ratio. 

ρ = density. 

The Ultrasonic Pulse Velocity (UPV) test is a stress wave propagation method that involves 

measurement of the travel time of compression waves pulse over a known path length. Pulses of 

longitudinal stress waves are generated by an electro-acoustical transducer that is held in contact 

with one surface of the concrete under test. After traversing through the concrete, the pulses are 

received and converted into electrical energy by a second transducer located a distance L from 

the transmitting transducer. The transit time T is measured electronically. The pulse velocity V is 

calculated by dividing L by T. ASTM C 597 is the standard test method for pulse velocity 

through concrete. 

Test Procedure and Instrumentation. Concrete specimens were cast and compacted in a 

purpose-made 150- by- 150- by 300-mm (6- by 6- by 12-inch) acrylic mold. Transducers were 

then bolted on each side of the mold. An ultrasonic couplant was applied between the transducer 

and the acrylic to ensure good wave transmission. Both transducers were then connected to a 

commercial UPV device. Transit time was recorded automatically at desired intervals, and the 

wave velocity was calculated by dividing the length of the mold by the transit time. 

Test Results. The test results show that initial and final set can be determined using this 

technique. The two points are marked by a sudden change in the rate of increase of the wave 

(1 )(1 2 )

(1 )

ρ μ μ

μ

+ −

− = E V
91 

velocity. As shown in figure 3, the results are reasonably consistent with other methods used to 

assess initial setting times. 

Impedance 

Consolidation of the concrete was determined at initial mixing and after setting using the 

impedance-based apparatus described by Alexander et al.(86) There was little correlation between 

the initial impedance and the initial slump. This method does not appear to provide useful data 

regarding potential incompatibility. It is the loss of workability of a concrete as it makes it way 

to and through a paving machine that is the most common and problematic occurrence of 

“incompatibility” in pavements. A number of mechanisms can cause this phenomenon, meaning 

that a number of approaches may be required to detect them all. 

In some cases it may be a slow occurrence of false set (gypsum deposition), such as Cement 2, 

influenced by the solubility rate of the sulfate compounds. Rapid false set often may go 

unnoticed because mixing continues for some time during transport if an agitating truck is used. 

On the other hand, this problem will be significant if a dump truck is used. Early stiffening 

caused by insufficient sulfate in the system is another cause of early stiffening (flash set). Both 

of these reactions will be accelerated by high temperatures and the presence of some WRAs. 

In other cases, the rate of silicate reaction will be the issue, either accelerated by high 

temperatures, high alkali content, and high fineness; or retarded by some WRAs and earlier 

aluminate reactions reducing the amount of calcium in the pore solution. The formation of 

syngenite also appears to be a potentially significant factor. 

The following test methods appear to be appropriate for detecting the various mechanisms of 

stiffening and setting related incompatibility discussed earlier: 

• False set: minislump, stiffening. 

• Flash set: minislump, calorimetry, stiffening, time of setting, rheometer. 

• Accelerated or retarded silicate hydration: time of set, calorimetry, mortar slump 

loss, semi-adiabatic temperature monitoring. 

Selection of which tests to use should be based on urgency, availability of test equipment, cost of 

testing, and cost of failure. This is discussed further in Volume II of this report. 

TASK 2.1.2—CRACKING 

Introduction 

This task includes a suite of tests intended to evaluate the potential for early-age cracking. The 

work examined the tendency of concrete to crack under conditions of full restraint, the stresses 

that develop in the concrete under those conditions, the heat evolution, and the development of 

stiffness (as measured by modulus of elasticity). The test program also measured the 

development of the ability of the concrete to resist cracking in terms of the splitting tensile 
92 

strength and nondestructive tests suitable for field monitoring of pavement concrete. Initial and 

final setting times and compressive strengths were measured. 

The test program involved a 24-h period of intensive monitoring of the properties of the concrete 

immediately after casting. The purpose of this monitoring was to examine the development of 

the properties of interest at early ages. It is not anticipated that such an intensive test program 

would be incorporated into an evaluation of the materials and mix designs for pavement projects; 

however, it should indicate which measurements are the most critical so that these could be 

adopted as necessary. It will also allow for the correlation of the various types of measurements. 

Materials 

Materials were obtained from projects that reported incompatibility problems during 

construction. These reports were gathered during the information collection phase of this project. 

Chemical analyses of the cements are given in table 24 and the fly ashes in table 25. 

The first scenario involves a particular portland cement that appeared to be incompatible with 

one brand of lignosulfonate water reducer, but not with a comparable admixture made by another 

manufacturer. The problem was seen during hot weather concreting. The test program used the 

same brand of cement and the two water reducers. The cement had been received from the field 

and stored for some time before laboratory testing was conducted. The tests were conducted at a 

nominal 32 °C (90 °F). The mixes in this scenario were labeled WRA1 and WRA2. 

The second scenario simulates a combination of a cement with 20 percent of a Class C fly ash 

that was reported to be problematic in the field, along with a lignosulfonate admixture. An 

alternative fly ash reported to be satisfactory was used in the companion mixture. The chemical 

analyses of these materials were very similar, as shown in table 25. The C3A content of both fly 

ash samples was estimated by x-ray diffraction XRD to be similar in both materials. The mixes 

in this scenario were labeled FA1 and FA2. 

The third scenario simulates a concrete containing fly ash along with two chemical admixtures 

that at elevated temperatures exhibited false set in the field. Four mixtures were conducted, two 

at 32 °C (90 °F) using 25 percent and 4 percent fly ash by mass of cement, and the same 

mixtures prepared at 21 °C (70 °F). These mix parameters were selected to mirror those used on 

the site where the problem was observed. These mixtures were labeled 25FA90, 4FA90, 

25FA70, and 4FA70, respectively. 

All mixtures were prepared using the same aggregates comprising siliceous gravel coarse 

aggregate and siliceous fine aggregate from the same source (table 26). Cement 2 was the same 

material used in Task 2.1.1. It was identified as Cement 5 in that series. 

All WRAs were ASTM C 494 Type A, and both air entraining admixtures were nonvinsol-based 

materials. 
93 

Table 24. Oxide analyses of cements. 

Mass 

Analyte (percentage) 

Cement 1 Cement 2 Cement 3 

SiO2 19.99 20.83 26.91 

Al2O3 5.10 4.20 6.46 

Fe2O3 3.83 3.26 1.86 

CaO 62.68 62.55 54.45 

MgO 1.18 3.23 5.67 

SO3 2.42 2.75 2.64 

Na2O 0.10 0.13 0.24 

K2O 0.52 0.65 0.49 

TiO2 0.18 0.30 0.33 

P2O5 0.19 0.09 0.23 

Mn2O3 0.04 0.53 0.23 

SrO 0.06 0.05 0.05 

Cr2O3 0.01 <.01 <.01 

ZnO 0.02 0.22 0.03 

L.O.I. (950 oC) 3.74 1.45 -0.03 

Total 100.08 100.24 99.56 

Alkalies as Na2O 0.44 0.56 0.56 

Calculated Compounds per ASTM C 150-02a 

C3S 57 56 * 

C2S 15 18 * 

C3A 7 6 * 

C4AF 12 10 * 

* Cement 3 was a Type IS blended cement, making calculated Bogue values 

meaningless. 
94 

Table 25. Oxide analyses of supplementary cementing materials. 

Analyte Mass 

(percentage) 

Material Fly Ash 1 Fly Ash 2 Fly Ash 3 

SiO2 36.42 36.14 33.83 

Al2O3 19.18 18.33 17.99 

Fe2O3 6.01 5.20 6.08 

CaO 24.27 26.04 26.11 

MgO 4.57 4.84 6.12 

SO3 2.13 2.41 2.17 

Na2O 1.63 1.59 2.14 

K2O 0.51 0.47 0.39 

TiO2 1.55 1.61 1.46 

P2O5 1.18 0.98 1.33 

Mn2O3 0.04 0.03 0.03 

SrO 0.40 0.44 0.36 

Cr2O3 0.02 0.02 0.02 

ZnO 0.02 0.02 0.02 

L.O.I. (950 oC) 0.36 0.40 0.38 

Total 98.28 98.52 98.39 

Alkalies as Na2O 1.96 1.91 2.39 

Moisture 0.22 0.21 0.09 

SiO2+Al2O3+Fe2O3 61.61 59.67 57.90 

Table 26. Physical properties of aggregates.

 19-mm Coarse 

Aggregate 

9-mm Coarse 

Aggregate 

Siliceous Fine 

Aggregate 

Sieve Analysis 

Sieve Percentage Passing 

25-mm 100.0 

19-mm 94.5 

12.5-mm 0.9 

9.5-mm 0.1 100.0 

4.75-mm 0.6 99.1 

2.36-mm 0.1 89.7 

1.16-mm 0.1 75.7 

0.600-mm 48.9 

0.300-mm 13.6 

0.150-mm 1.3 

0.075-mm 0.3 

Pan 0.0 0.0 0.0 

Fineness Modulus 2.72 

Density 

Bulk Specific Gravity (SSD) 2.68 2.65 2.63 

Absorption 1.20 1.51 1.15 

Dry Rodded Unit Weight, kg/m3 1,665.00 1,680.00 1,780.00 

Unit conversions: 

1mm =0.0394 inch 

1 kg/m3

 = 1.69 pcy 
95 

MIX DESIGNS 

A total of six sets of mix proportions were prepared for testing. All mixes were based on the 

information obtained from the field where material incompatibilities had been observed. Of the 

six mixes, three mixes are labeled as “incompatible,” and the remaining three as “compatible.” 

Two of the mixes were also conducted at 21 °C (70 °F) to investigate temperature sensitivity of 

the reported incompatibility. The matrix of concrete mixtures is summarized in table 27. 

Table 27. Concrete mixtures. 

Incompatible 

Mix 

Compatible 

Mix Temperature Materials 

WRA1 WRA2 32 °C 

Cement 1 

Water reducer 1 

Water reducer 2 

Air entrainer 1 

FA1 FA2 32 °C 

Cement 2 

Fly ash 1 

Fly ash 2 

Water reducer 3 

Air entrainer 1 

25FA90 4FA90 32 °C 

25FA70 4FA70 21 °C 

Cement 3 

Fly ash 3 

Water reducer 1 

Water reducer 4 

Air entrainer 2 

Unit conversions: 

1 °C = (X – 32)/1.8 °F 

Because of the large volume of concrete required to cast all the specimens, two batches of each 

mix were made. The first batch was used to cast specimens for setting time, AASHTO ring test, 

P-wave, temperature monitoring, and compressive strength, modulus of elasticity, and splitting 

tensile strength for 1-, 3-, 7-, and 28-day testing. The second batch was used to cast specimens 

for setting time and compressive strength, modulus of elasticity, and splitting tensile strength for 

testing during the initial 24 h after the final set. 

Both batches of each mix were made on the same day to keep the variability of materials to a 

minimum. Immediately after mixing, fresh concrete properties were measured and specimens 

were cast. 

Proportioning and material selection of each mix are summarized in table 28. 
96

Table 28. Concrete mix proportions. 

Mix ID WRA1 WRA2 FA1 FA2 25FA90 4FA90 25

Temperature,  ̊C 32 32 32 32 32 32 Cement 1 1 2 2 3 3 Cement, kg/m3 356 356 281 281 267 341 Fly Ash — — 1 2 3 3 Fly Ash, kg/m3 0 0 70 70 89 15 Fine Aggregate, kg/m3 610 610 800 800 599 599 Coarse Aggregate–19 mm, kg/m3 569 569 489 489 569 569 Coarse Aggregate–9.5 mm, kg/m3 569 569 489 489 569 569 Water, kg/m3 959 959 824 824 959 959 Water Reducer 1 2 3 3 1, 4 1, 4 Water Reducer dosage (mL/100 kg) 534 980 331 331 55, 392 55, 392 Air Entraining Admixture 1 1 1 1 2 2 Air Entraining Admixture dosage (mL/100 kg) 

36 56 33 33 260 260 

Unit conversions: 

1 °C = (X – 32)/1.8 °F 1 kg/m3 = 1.69 pcy 1mm =0.0394 inch 1 mL/100 kg = 0.0154 oz/cwt. 
97 

Tests and Results 

Fresh Concrete Properties 

The following test methods were used to measure fresh concrete properties: 

• Slump—ASTM C 143. 

• Air content—ASTM C 231. 

• Unit weight—ASTM C 138. 

Mixes conducted at room temperature exhibited high slumps. As a result, slump flow, rather than 

slump, was measured. 

The fresh concrete properties are presented in table 29. 

Table 29. Fresh concrete properties. 

Slump (mm) 

Slump Flow (mm) 

Unit Weight 

(kg/m3

) 

Air Content 

Mix ID (percentage) 

Batch 1 Batch 2 Batch 1 Batch 2 Batch 1 Batch 2 

WRA1 51 64 2278 2278 7.3 7.0 

WRA2 95 95 2323 2323 5.3 5.3 

FA1 95 89 2291 2284 6.8 6.8 

FA2 114 114 2259 2278 7.2 7.0 

25FA90 222 267 2278 2284 5.1 3.7 

4FA90 248 248 2284 2281 5.1 4.5 

25FA70 (559) (610) 2259 2271 7.5 7.5 

4FA70 (559) (584) 2259 2262 7.5 7.8 

Unit conversions: 

1mm =0.0394 inch 

1 kg/m3 = 1.69 pcy 

In general, there was little variation in fresh concrete properties between two batches of the same 

mix. 

Setting Time. The time of set was measured in accordance with ASTM C 403. The results are 

presented in table 30. 

Table 30. Setting time data.

Initial Set (min) Final Set (min) Mix ID Batch 1 Batch 2 Batch 1 Batch 2 

WRA1 340 349 422 396 

WRA2 251 234 341 306 

FA1 339 354 430 460 

FA2 389 403 477 482 

25FA90 No data 298 No data 1511 

4FA90 452 464 530 539 

25FA70 844 No data 1421 No data 

4FA70 726 720 872 848 
98 

The 25FA90 mixture exhibited rapid stiffening in the mixer, followed by extremely slow and 

erratic setting behavior. Final set occurred eventually after 2.5 days. The same mixture prepared 

at 21 °C (70 °F) was also somewhat erratic. This mix was the only one that exhibited classic 

stiffening incompatibility behavior in this set of work. In these mixtures in which final set 

occurred after 1 day, initial measurements of hardened properties were not taken. 

Cracking Tendency. Cracking tendency and stress development were investigated using the 

ASTM C 1581 ring test method on samples stored at the same temperature as the mixing 

temperature. A modification to the test was that the specimens were 125 mm (5 inches) high 

rather than 150 mm (6 inches) based on the equipment available. For each mix, five rings were 

cast and monitored until cracking occurred. A summary of the results is presented in table 31. 

Table 31. Results of ASTM ring tests. 

Mix WRA1 WRA2 FA1 FA2 25FA90 4FA90 25FA70 4FA70

Average initial strain 

(millionths) 18.60 9.20 5.00 4.30 * 2.00 3.40 6.30 

Average maximum strain 

(millionths) 34.70 34.40 26.00 27.70 * 20.70 13.90 18.90 

Average strain rate factor 

(millionths per root day) 9.90 20.80 10.1 20.80 * 12.10 6.40 11.50 

Average stress rate, 

(MPa/day) 0.14 0.24 0.15 0.17 * 0.20 0.11 0.20 

Average time to crack, days 6.79 5.40 5.81 5.54 * 4.50 - 4.51 

* Sample 25FA90 did not crack. 

Unit conversions: 

1 MPa = 145.0 psi 

The results show that mix WRA2 did crack slightly earlier than WRA1, but there was little 

apparent difference between the two FA mixtures. The mixtures in the third scenario that 

exhibited setting incompatibility did not crack, while the other two cracked very early. 

Hardened Concrete Properties 

Hardened concrete properties were measured by testing concrete for compressive strength, 

modulus of elasticity, and splitting tensile strength. The measurements were conducted every 2 h 

from time of final set up to 24 h, then at 3, 7, and 28 days. Samples for longer term tests were 

stored at the mixing temperature for 24 h, then moved to standard storage.

The tests were conducted in accordance with the following methods: 

• Compressive strength–ASTM C 39. 

• Modulus of elasticity—ASTM C 469. 

• Splitting tensile strength—ASTM C 496. 

Individual test results are presented in tabular form in tables 32 through 39. Graphical 

compressive strength, modulus, and splitting tensile strength development are shown in figures 

21, 22, and 23, respectively. 
99 

Table 32. Hardened concrete properties for mix WRA1. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa Gigapascal (GPa) MPa 

2 5.7 18.4 0.7 

4 8.9 16.4 1.1 

6 12.1 18.3 1.3 

8 14.1 17.9 1.7 

10 16.1 22.8 1.8 

12 16.5 23.7 2.1 

14 18.6 24.0 2.2 

16 19.9 24.1 2.4 

18 22.1 25.6 2.2 

20 21.2 25.0 2.3 

22 21.5 26.8 2.2 

24 23.6 27.2 2.4 

72 28.1 29.6 2.9 

168 33.0 31.0 3.5 

672 41.0 34.0 4.0 

Unit conversions: 

1 MPa = 145.0 psi 

Table 33. Hardened concrete properties for mix WRA2. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

2 5.4 13.5 0.6 

4 8.8 16.5 0.9 

6 11.2 20.4 1.5 

8 13.0 19.5 1.7 

10 14.9 22.6 1.7 

12 17.6 23.3 2.1 

14 17.7 24.9 2.2 

16 18.1 23.8 2.2 

18 20.3 22.6 2.7 

20 19.8 22.8 2.3 

22 19.1 24.4 2.2 

24 21.7 27.1 2.2 

72 31.2 28.1 3.1 

168 35.2 32.1 3.7 

672 45.0 35.6 3.9 

Unit conversions: 

1 MPa = 145.0 psi 
100 

Table 34. Hardened concrete properties for mix FA1. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

2 7.0 15.0 0.9 

4 8.8 16.2 1.0 

6 10.7 18.5 1.2 

8 12.1 19.5 1.5 

10 12.5 20.0 1.9 

12 13.8 21.2 1.9 

14 15.2 20.6 2.0 

16 16.4 21.5 2.2 

18 16.3 22.1 2.2 

20 17.6 23.9 2.3 

22 18.7 22.1 2.3 

24 23.3 25.3 2.6 

72 28.2 28.3 3.0 

168 37.8 32.8 3.7 

672 7.0 15.0 0.9 

Unit conversions: 

1 MPa = 145.0 psi 

Table 35. Hardened concrete properties for mix FA2. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

2 6.1 13.6 1.0 

4 8.3 15.7 1.1 

6 9.4 18.4 1.3 

8 10.8 18.4 1.6 

10 12.3 19.0 1.8 

12 14.1 21.3 2.0 

14 14.3 25.1 1.9 

16 15.1 22.5 2.1 

18 15.7 22.9 2.2 

20 17.7 23.6 2.2 

22 18.4 20.8 2.1 

24 18.6 22.0 2.3 

72 22.8 26.3 2.6 

168 28.3 30.8 3.0 

672 36.8 32.1 3.6 

Unit conversions: 

1 MPa = 145.0 psi 
101 

Table 36. Hardened concrete properties for mix 25FA90. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

72 1.4 7.7 0.2 

168 13.5 21.2 1.6 

672 41.7 32.3 4.4 

Unit conversions: 

1 MPa = 145.0 psi 

Table 37. Hardened concrete properties for mix 4FA90. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

2 2.1 9.1 0.3 

4 2.5 10.9 0.3 

6 3.2 13.8 0.4 

8 4.0 13.9 0.5 

10 4.3 15.3 0.6 

12 5.9 13.6 0.8 

14 7.2 16.2 0.9 

16 7.7 17.7 1.0 

18 9.2 18.1 1.1 

20 10.2 18.5 1.2 

22 10.9 19.4 1.4 

24 11.7 18.4 1.6 

72 22.2 25.5 2.3 

168 30.9 30.5 3.4 

1176 44.8 35.7 4.1 

Unit conversions: 

1 MPa = 145.0 psi 

Table 38. Hardened concrete properties for mix 25FA70. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

48 1.0 6.1 0.2 

72 2.6 12.1 0.4 

168 7.1 15.8 0.9 

672 16.9 21.5 2.2 

1416 36.5 31.8 4.0 

Unit conversions: 

1 MPa = 145.0 psi 
102 

Table 39. Hardened concrete properties for mix 4FA70. 

Age Compressive 

Strength 

Modulus of 

Elasticity 

Splitting Tensile 

Strength 

Hours MPa GPa MPa 

2 1.4 11.0 0.2 

4 2.3 9.7 0.3 

6 2.6 9.4 0.4 

8 2.7 12.0 0.4 

10 2.8 10.9 0.4 

12 3.2 11.1 0.4 

14 3.7 11.0 0.6 

16 4.1 12.1 0.6 

18 4.4 13.3 0.6 

20 5.0 16.7 0.8 

22 5.4 15.1 0.8 

24 5.7 15.6 0.8 

72 14.2 23.9 1.8 

168 22.1 33.1 2.6 

672 40.7 29.6 4.3 

Unit conversions: 

1 MPa = 145.0 psi 

Unit conversions: 

1 mm2

 = 0.00155 inch2

Figure 21. Compressive strength development. 

0

10

20

30

40

50

0 7 14 21 28

Time, days

Compressive Strength, MPa

WRA1 WRA2

FA1 FA2

25FA90 4FA90

25FA70 4FA70
103 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 22. Modulus of elasticity development. 

Unit conversions: 

1 mm2

 = 0.00155 inch2 

Figure 23. Splitting tensile strength development. 

0

10

20

30

40

50

0 7 14 21 28

Time, days

Modulus of Elasitcity, GPa

WRA1 WRA2

FA1 FA2

25FA90 4FA90

25FA70 4FA70

0

1

2

3

4

5

0 7 14 21 28

Time, days

Split Tensile Strength, MPa

WRA1 WRA2

FA1 FA2

25FA90 4FA90

25FA70 4FA70
104 

The graphs in figures 21, 22, and 23 show that the 28-day properties of the incompatible 

mixtures and their respective compatible pairs are similar. Differences are observed in the 7-day 

data for the mixtures in scenario 3. Properties for the mixtures containing 25 percent fly ash are 

significantly lower than for the corresponding mixtures containing 4 percent fly ash. This is not 

unexpected based on trends reported in the literature. 

Heat Evolution. Thermocouples were used to record the temperature rise of samples stored in 

semi-adiabatic conditions. This was achieved by casting the thermocouples into 100- by 200-mm 

(4- by 8-inch) cylinders that were stored inside a similarly sized Dewar flask. Temperatures were 

monitored for up to 36 h. The data are presented graphically in figures 24, 25, 28, 29, 32, 33, 37, 

and 38. 

Ultrasonic P-waves. Ultrasonic P-wave testing was conducted on all of the mixtures. The test is 

discussed in detail under Task 2.1.1. The data are presented graphically in figures 25, 28, 29, 32, 

33, 37, and 38. 

Results Comparison 

The following discussion is based on comparing the results for each pair of mixtures. 

Scenario 1—Influence of Chemical Admixtures, WR1 and WRA2 

The properties measured for the two mixtures are presented in figures 24 to 27. In an attempt to 

correlate the development of strength with the time of cracking, a parameter was calculated by 

dividing the compressive strength by the modulus of elasticity at each age. The results of the 

calculation (fc/E) have no units and may be considered equivalent to a strain. They are plotted in 

figures 26 and 27. It is notable that both of the mixtures cracked when this factor (fc/E) had a 

value of approximately 1 MPa/GPa (pounds per square inch per thousand pounds per square inch 

(psi/ksi)). 

The results of the tests indicate that the risk of cracking as reflected by the ring test data is 

somewhat higher for the WRA2 mix, based on the higher stress rates and shorter time to 

cracking. This is in contrast to the field reports that WRA1 was the more problematic. The initial 

strain in the WRA1 mix was double that of the WRA2 mix. This parameter is described by the 

test method as being caused by early-age autogenous shrinkage and heat of hydration. The 

maximum temperature for both mixtures was similar. This indicates similar heats of hydration. 

The same cement and w/cm was used in both mixtures, which are considered the controlling 

parameters for autogenous shrinkage. The differences result more from the timing of early 

hydration in that setting, which was somewhat earlier in the WRA1 mix than the WRA2 mix. 

The differences in hydration rates would be strongly associated with the chemistry of the 

different admixtures. A high initial strain would be expected to increase the risk of cracking, 

depending on the rate of subsequent strain development. 
105 

Figure 24. Early age properties for mix WRA1. 

Figure 25. Early age properties for mix WRA2. 

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

Set Time

Strength

Modulus

Split

Temperature

Final set

Initial 

set

WRA1

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

P-Wave Set Time

Strength Modulus

Split Temperature

Final set

Initial set

WRA2
106 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 26. Long-term properties for mix WRA1. 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 27. Long-term properties for mix WRA2. 

WRA1

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.0

0.3

0.6

0.9

1.2

1.5

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E

WRA2

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.0

0.3

0.6

0.9

1.2

1.5

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E
107 

Long-term properties of the two mixes were similar, highlighting the issue that incompatibility is 

often related more to early properties that influence constructability than later properties that 

influence serviceability of the concrete. 

Scenario 2—Influence of Fly Ashes, FA1 and FA2 

Figure 28. Early age properties for mix FA1. 

Figure 29. Early age properties for mix FA2. 

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

P-Wave

Set Time

Strength

Modulus

S lit

Initial set Final set

FA1

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

P-Wave Set Time

Strength Modulus

Split Temperature

Final set Initial set

FA2
108 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 30. Long-term properties for mix FA1. 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 31. Long-term properties for mix FA2. 

FA1

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0

0.3

0.6

0.9

1.2

1.5

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E

FA2

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.00

0.30

0.60

0.90

1.20

1.50

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E
109 

Very little difference was observed in any of the properties measured using these two sets of 

materials (figures 28 to 31). This is not surprising because the chemistries of both fly ashes were 

very similar. This supports the contention that chemical analysis of the materials in a mixture 

may be a good first step in identifying potential incompatibility. 

The fc/E parameter again showed a reasonable correlation with cracking occurring when a value 

of approximately 1 psi/ksi was reached. 

Scenario 3a—Influence of Fly Ashes at High Temperature, 25FA90 and 4FA90. 

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

P-Wave

Set Time

Strength

Modulus

Split

Temperature

Initial set

25FA90

Figure 32. Early age properties for mix 25FA90. 
110 

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

P-Wave Set Time

Strength Modulus

Split Temperature

Final set Initial set

4FA90

Figure 33. Early age properties for mix 4FA90. 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 34. Long-term properties for mix 25FA90. 

25FA90

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.00

0.30

0.60

0.90

1.20

1.50

fc/E, MPa/GPa

Strength

Modulus

Fc/E
111 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 35. Long-term properties for mix 4FA90. 

The 25FA90 mixture exhibited classic stiffening and setting incompatibility resulting from the 

chemistry of the cementitious materials. The mixture was observed to stiffen significantly in the 

mixer as is typical of flash set. This is caused by uncontrolled hydration of the C3A in the cement 

causing early stiffening. The mixture then did not set for about 21⁄2 days (figures 32 and 34). 

Again, this is typical of a system where the calcium in solution is at a lower concentration 

because it has been consumed in the early C3A hydration. This retards C3S hydration and slows 

or stops setting. It is also notable that the 28-day strength of this mixture was greater than the 

other mixtures in this series. It is not uncommon for mixtures to gain high early strengths if early 

hydration is slowed. 

The same materials were submitted for calorimetry and minislump testing to observe whether 

these tests reported similar information, as would be expected from the Task 2.1.1 work. The 

minislump data (table 40) indicate that there was extreme loss of workability within a short 

period of time. Removing one of the admixtures mitigated the degree of stiffening. The 

calorimetry plot is consistent with the observations of the concrete because there is a large initial 

peak, followed by little heat generation for the remainder of the 72 h that the test was run 

(figure 36). 

4FA90

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.00

0.30

0.60

0.90

1.20

1.50

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E
112 

Figure 36. Conduction calorimetry plot of paste system for mixture 

25FA90 conducted at 32 °C (90 °F). 

Table 40. Results of minislump tests conducted on 25FA90 pastes.

Area 

(mm^2) 

2 min 5 min 10 min 30 min

False set 

Index 

Stiffening

Index 

25FA90 paste system 

without one admixture 9,480 7,870 6,190 3,870 0.8 0.4 

25FA90 paste system 10,000 5,810 2,900 0 0.6 0.0 

Unit conversions: 

1 mm2

 = 0.00155 inch2

This mixture did not crack, again supporting the contention that systems that set and stiffen 

quickly are at higher risk of cracking than slower reacting systems. 

The mixture prepared using a lower fly ash dosage did not exhibit the stiffening incompatibility 

and performed in a manner similar to the mixtures tested in the other scenarios (figures 33 

and 35). 

0.0

0.5

1.0

1.5

2.0

2.5

0 5 10 15 20 25 30 35 40 45

Time of Hydration (hours)

Heat (mV)

25FA90
113 

Scenario 3b—Influence of Fly Ashes at Normal Temperature, 25FA70 and 4FA70 

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30

Hours

P-Wave Set Time

Strength Modulus

Split Temperature

Final set

Initial set

25FA70

Figure 37. Early age properties for mix 25FA70. 

Figure 38. Early age properties for mix 4FA70. 

0 2 4 6 8 10 12 14 16 18 20 22 24 26 28 30 32 34 36 38 40

Hours

P-Wave Set Time

Strength Modulus

Split Temperature

Final set

Initial set

4FA70
114 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 39. Long-term properties for mix 25FA70. 

Unit conversions: 

1 MPa = 145.0 psi 

Figure 40. Long-term properties for mix 4FA70. 

25FA70

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.00

0.30

0.60

0.90

1.20

1.50

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E

4FA70

0

10

20

30

40

50

0 168 336 504 672

Hours

Strength, MPa or E, GPa

0.00

0.30

0.60

0.90

1.20

1.50

Fc/E, MPa/GPa

Strength

Modulus

Crack

Fc/E
115 

The mixture containing the high fly ash dosage prepared at 21 °C (70 °F) was also significantly 

retarded and did not crack, although the effects were less marked than the same mix prepared at 

32 °C (90 °F) (figures 37 and 39). The low fly ash mixture prepared at 21 °C (70 °F) was not 

affected by the change in temperature (figures 38 and 40). Both mixtures prepared at 21 °C 

(70 °F) exhibited considerably more workability than the same mixtures made at 32 °C (90 °F). 

This is likely related to the observed rapid stiffening in the high temperature mixtures. 

Summary 

The following observations may be drawn from the work conducted in this task: 

• The risk of cracking is associated with the chemistry of the reactive materials. 

• Systems that are less reactive or more slowly reactive appear to be at lower risk of 

cracking. There is some value in monitoring setting times of mixtures. 

• The ASTM ring exhibited poor correlation with reported field observations. The 

difference between field reports and laboratory data are probably because not all of 

the same materials were used in the laboratory tests as in the field. 

• It would appear that monitoring the parameter fc/E for the first 24 h may provide 

useful data on when cracking is likely to occur. More work is required to validate 

this approach. 

TASK 2.1.3—AIR VOID SYSTEM 

Introduction 

Concrete strength and durability issues related to problematic air void systems can be costly. 

Unfortunately, air void problems are usually not identified until analyses are conducted on 

hardened concrete. To save time and money, these problems must be identified much earlier. 

Currently, the most widely accepted method being used to evaluate the air void system of fresh 

concrete is to obtain the total air content of a mixture, often using the pressure meter. Basing 

acceptance on total air content can be misleading. Total air measurements of fresh concrete may 

meet the limits outlined in job specifications, but that does not guarantee that those mixes will 

contain a satisfactory air void system and perform as intended. The total air content of fresh 

concrete provides no identification of the distribution, size, or spacing of the air bubbles, which 

are the parameters critical to performance. Clustering of air voids around aggregate particles and 

poor spacing factors are examples of problems that occur in otherwise ordinary concrete, but 

they cannot be identified in the fresh state using currently recognized methods. The purpose of 

this task was to evaluate tests that could be used to identify problematic air void systems in fresh 

concrete. 

Materials 

Air entraining admixtures are reputed to have problematic interactions when combined with 

some types of water-reducing admixtures. The most common problems associated with these 
116 

interactions include requiring increased dosage of air-entraining admixtures (AEA), decreased 

total air contents, and increased spacing factors. 

A total of 10 AEAs were procured and evaluated. The selection of AEAs was based primarily on 

the recent experience of the State highway departments in South Dakota, Michigan, Delaware, 

and New Jersey. Admixtures were obtained from the major chemical companies in the concrete 

industry. Vinsol resins as well as various synthetic admixtures were included in the program. 

Specific properties and classifications of these admixtures are presented in table 41. The 

chemical compositions of the materials are presented in table 42. 

Table 41. Air entraining admixtures and related properties. 

Admixture Physical Properties 

Identification 

Admixture 

Classification pH Specific Gravity Solids by mass (%) 

A vinsol resin 12.49 1.045 13.78 

B vinsol resin 12.7 1.050 17.49 

C vinsol resin 12.34 1.030 13.51 

D resin/rosin 10.5 1.010 5.97 

E resin/rosin 11.75 1.018 6.99 

F resin/rosin 11.06 1.015 12.51 

G alpha sulfonate 10.8 1.01 6.66 

H tall oil 9.92 1.020 6.58 

I benzene sulfonate 10.18 1.011 6.04 

J fatty acid 9.92 1.020 11.38 

 

Table 42. Cementitious materials composition and fineness. 

Composition 

High alkali 

cement 

(% mass ) 

Class C 

fly ash (A) 

(% mass) 

Class C 

fly ash (B) 

(% mass) 

Class F 

fly ash 

(% mass) 

SiO2 19.24 36.14 38.45 52.56 

Al2O3 5.61 18.33 19.59 20.26 

Fe2O3 2.28 5.20 5.73 11.46 

CaO 62.27 26.04 15.83 4.29 

MgO 2.36 4.84 4.02 1.00 

SO3 4.41 2.41 2.54 0.64 

Na2O 0.28 1.59 7.41 1.32 

K2O 0.97 0.47 0.83 1.92 

TiO2 0.30 1.61 1.32 0.97 

P2O5 0.17 0.98 0.54 0.28 

Mn2O3 0.21 0.03 0.04 0.05 

SrO 0.07 0.44 0.80 0.08 

Cr2O3 * 0.02 0.02 0.02 

ZnO * 0.02 0.01 0.04 

L.O.I. (950 oC) 1.54 0.40 0.31 4.22 

Total 99.71 98.52 97.45 99.1 
117 

Table 42. Cementitious materials composition and fineness (continued). 

Composition 

High alkali 

cement 

(% mass ) 

Class C 

fly ash (A) 

(% mass) 

Class C 

fly ash (B) 

(% mass) 

Class F 

fly ash 

(% mass) 

Total alkalies as Na2Oequiv. 0.91 1.91 7.96 2.58 

Blaine fineness, kg/m2 352 * * * 

Phases: 

C3S 54 * * * 

C2S 15 * * * 

C3A 11 13.7 * * 

C4AF 7 * * * 

SiO2+Al2O3+Fe2O3 * 59.67 63.8 84.3 

* = No data 

Two types of WRAs (sugar-based and lignin-based) were procured for analysis in this study. 

Both admixtures met ASTM C 494 requirements for Type A water-reducing admixture. The 

cementitious materials used in this study included a high alkali Type I cement, two Class C fly 

ashes, and a Class F fly ash. Except for one of the Class C fly ashes, these were materials used in 

other tasks of this study. A rounded siliceous coarse aggregate and siliceous fine aggregate were 

used in the concrete analysis portion of this study. The gradations of the coarse and fine 

aggregates are shown in tables 43 and 44 respectively. 

Table 43. Coarse aggregate grading. 

Sieve size 

(mm) 

Rounded siliceous 

(% passing) 

Crushed dolomitic 

(% passing) 

25.00 100.0 100 

19.00 99.0 92 

12.50 42.0 47 

9.50 41.0 25 

4.75 0.4 9 

Unit conversions: 

1mm =0.0394 inch 

Table 44. Fine Aggregate Grading 

Sieve size 

(mm) 

Passing 

(%) 

4.750 99.00 

2.360 90.00 

1.180 76.00 

0.600 49.00 

0.300 14.00 

0.150 1.30 

0.075 0.30 

Fineness Modulus 2.72 

Unit conversions: 

1mm =0.0394 inch 
118 

Work Plan 

The testing program of this study consisted of three stages. In the first stage, a foam drainage 

analysis was conducted where AEAs were blended with various raw materials to generate foams. 

The stability of these foams was rated on the basis of how much and how fast water drained from 

the foam structures. The second and third stages comprised testing of concrete mixtures. The 

second stage focused on testing fresh concrete properties; the third stage dealt with the testing 

and analysis of hardened concrete at early ages. The three-stage testing program was used to 

determine if a correlation among the various air content determination methods could be 

discerned to identify air void problems at the earliest possible stage in construction. 

Stage 1—Foam Drainage Analysis 

The foam drainage test was developed in the late 1980s to provide a preliminary means of 

evaluating the stability of entrained air void systems developed from commercially available 

AEAs.(81) The test was meant to identify poorly performing admixtures before their use in 

concrete. The method consists of rapidly blending an air entrainer with water to generate foam. 

Other concrete raw materials and admixtures have also been blended with air entrainers to 

evaluate how those materials influence the stability of the foam and the resulting air void 

system.(68) After it is mixed, the foam is poured into a graduated cylinder and the rate at which 

water drains from the foam is recorded for 60 min. 

A stable air void system will usually have a lower drainage rate and retain more water than an 

unstable system.(68,81) The rate of drainage depends on the hydrodynamic characteristics of the 

foam, which include the size and shape of bubbles and the mobility of the liquid-air interface. 

Over the years, this test has been slightly modified by other researchers. The foam drainage test 

procedures used in this study were based on the work conducted by the South Dakota DOT.(68)

For this study, a total of 50 tests were conducted. Foam drainage characteristics for 10 

admixtures were analyzed for the following amounts and combinations of raw materials: 

• 300 ml (10 oz) water, 10 ml (0.33 oz) AEA. 

• 250 ml (8.5 oz) water, 10 ml (0.33 oz) AEA, 50 ml (1.7 oz) WRA. 

• 300 ml (10 oz) water, 10 ml (0.33 oz) AEA, 5 g (0.18 oz) cement. 

• 250 ml (8.5 oz) water, 10 ml (0.33 oz) AEA, 50 ml (1.7 oz) WRA, 4 g (0.14 oz) 

cement, 1 g (0.04 oz) Class C fly ash. 

• 250 ml (8.5 oz) water, 10 ml (0.33 oz) AEA, 50 ml (1.7 oz) WRA, 4 g (0.14 oz) 

cement, 1 g (0.04 oz) Class F fly ash. 

The procedure for conducting this test is illustrated in figure 41. Water, admixtures, and 

cementitious materials are added to the blender. The mixture is blended for 10 s and the resulting 

foam is immediately poured into a 1,000 ml (34 oz) graduated cylinder. Then the level of the 

foam/water interface is recorded as a function of time. All tests are carried out for 1 h. 
119 

Figure 41. Foam drainage procedure. 

A 50 ml (1.7 oz) dosage of water reducer compared to the 10 ml (0.33 oz) air entrainer dosage 

was chosen to reflect the relative difference in the standard concrete dosages of the two types of 

admixtures. For tests using water reducers, the total water was dropped to 250 ml (8.5 oz) to 

maintain the 300 ml (10 oz) liquid level before the addition of air entrainer. 

The amount of water drained as a function of time is fitted to an equation shown in figure 42 and 

the values of V0 and –1/k are calculated. 

Figure 42. Equation. Foam drainage. 

Where 

Vd is the amount of liquid drained from the foam at time t. 

1/k is a parameter specific to the system being tested. 

V0 may be considered the amount of water drained from the foam at the end of the test (yintercept on a plot of V versus 1/t). 

V0 and 1/k are determined by plotting the amount of drained water versus 1/t. The slope of the 

line is –1/k and V0 is the intercept. When comparing admixtures, the more useful parameter is –

1/k, which indicates the rate of drainage of fluid from the foam. The higher the value of –1/k, the 

slower the drainage rate and the more stable the foam is considered to be. Such admixtures are 

expected to produce more stable foams than those producing foams that do not retain water as 

effectively. The percent of water drained is calculated using the equation in figure 43. 

x 100

310

(310 - V ) % Drained 100 - 0 =

Figure 43. Equation. Percent drained. 

kt

Vd V 1 = 0 −
120 

Admixtures with significant differences in the –1/k values and in the percentage of water drained 

from the foam (percentage drained) are expected to have different air void systems and different 

performance. 

Based on the results obtained from the foam drainage analysis, 3 of the 10 admixtures were 

selected for further analyses in the second and third stages. The selection of admixtures was also 

based on having at least one vinsol-based product, no two products from the same manufacturer, 

and three different chemical compositions. Admixtures B, D, and H were the 3 admixtures 

chosen—a vinsol resin (control), a resin/rosin, and a tall oil-based air entrainer, respectively. 

Stage 2—Fresh Concrete Properties and Air Void Analyzer Investigation 

In the second stage, the focus of the investigation shifted to evaluating the effects of air 

entraining admixtures on the fresh properties of concrete. A correlation among test results for 

this stage would be essential because the goal of this study is to develop the ability to identify air 

void problems in concrete before placement. 

The fresh properties of the concrete were evaluated in accordance with the following American 

Association of State Highway and Transportation Officials (AASHTO) standards: 

• AASHTO T 119, “Slump of Hydraulic Cement Concrete.” 

• AASHTO T 152, “Air Content of Freshly Mixed Concrete by the Pressure Method.” 

• AASHTO T 121, “Mass per Cubic Meter (Cubic Foot), Yield and Air Content 

(Gravimetric) of Concrete.” 

Air void Analyzer Test. A promising technique was developed in Europe in the early 1990s as 

an alternative method for measuring the air void parameters of concrete. The commercially 

available equipment for this test is known as the Air Void Analyzer (AVA). The main advantage 

of this technique is that the test is conducted on fresh concrete and takes less than 30 min to 

complete. The method is based on the fact that large bubbles rise through a column of liquid 

faster than small bubbles do, and therefore, bubble size can be accurately inferred from how long 

it takes the bubble to rise. A mortar is extracted from a concrete sample taken from the as-placed 

concrete and injected by means of a syringe into the base of the AVA. The mortar sample is 

stirred into a viscous liquid to release the air voids. The air bubbles rise through the viscous 

liquid and water in the glass cylinder, and then they are gathered on a glass bell (petri dish). The 

petri dish is suspended from a bracket attached to a sensitive balance. Knowing the viscosity of 

the system and using Stoke’s Law, it is possible to compute the size of the air bubbles with time 

and calculate the air void parameters. 

This method is used to determine three parameters: 

• Air content. 

• Spacing factor. 

• Specific surface. 
121 

Measurement of air void parameters of concrete at the fresh state is the optimum procedure for 

evaluating the air void system of concrete. The AVA is the only method available at this time for 

such measurements, although its reliability is still to be proven. 

For this project, the mortar samples used in the AVA test were obtained from one of two 150- by 

150- by 530-mm (6- by 6- by 21-inch) beams cast from each mix. In the case of mixes 12 and 13 

(vibration effect), the sample was collected from the top 50 mm (2 inches). The information 

obtained from this test included total air content and spacing factor. These values were obtained 

for correlation with the same parameters obtained from the Stage 3 ASTM C 457 analysis on 

hardened concrete. 

Concrete Mix Regimen and Design. The selected mix compositions used in the second stage 

are presented in table 45. As shown in the table, a variety of admixtures, materials, and mixing 

conditions were chosen to simulate the field conditions under which unstable air void systems or 

coalescence of air voids around aggregates have been observed. These selections were based on 

a literature review, field experience, and information from personal contacts. The goal of such 

selections was to provide realistic conditions to evaluate the ability of the proposed tests to 

identify air void problems in the fresh concrete system. 

As shown in table 45, the concrete mixtures were as follows: 

• Three mixes using the three selected AEAs. These mixes will be prepared at normal 

laboratory temperature and contain a single dose of WRA (mixes 1 to 3). 

• One mix with no WRA (mix 4). 

• One mix with a double dose of WRA (mix 5). 

• One mix with a single dose of a different WRA (mix 6). 

• Two mixes using coarse sand (mixes 7 to 8). 

• Three mixes containing a single dose of three different supplementary cementing 

materials (mixes 9 to 11). 

• Two mixes subjected to excessive vibration (mixes 12 and 13). 
122 

Table 45. Concrete test matrix used in stages 2 and 3 of subtask 2.1.3. 

Mix 

No. 

AEA 

Identification 

Sand 

Gradation 

WaterReducer

WaterReducer 

Dosage 

Temperature Pozzolans Consolidation

1 B (vinsol) Normal A Normal Normal None Normal 

Vibration 

2 H (tall oil) Normal A Normal Normal None Normal 

Vibration 

3 D 

(resin/rosin) Normal A Normal Normal None Normal 

Vibration 

4 H Normal None Not 

applicable High (32 oC) None Normal 

Vibration 

5 H Normal A High High (32 oC) None Normal 

Vibration 

6 H Normal B Normal Normal None Normal 

Vibration 

7 H Coarse A Normal Normal None Normal 

Vibration 

8 D Coarse A Normal Normal None Normal 

Vibration 

9 H Normal A Normal Normal 20% (C) 

fly ash A 

Normal 

Vibration 

10 H Normal A Normal Normal 20% (C) 

fly ash B 

Normal 

Vibration 

11 H Normal A Normal High (32 oC) 20% (F) 

fly ash 

Normal 

Vibration 

12 D Normal A Normal Normal None Excessive 

Vibration 

13 B Normal A Normal Normal None Excessive 

Vibration 

The base concrete mixture used for the second stage is shown in table 46. The base mix 

contained 335 kg/m3 (564 pcy) of ASTM Type I cement and had a water-cement ratio of 0.42. 

Changes in the base mix occurred in mixes 7–11. A coarse sand gradation was specified for 

mixes 7 and 8. The fine aggregate source for these mixes was not changed. Instead, the fine 

aggregate was sieved and manually reconstructed to obtain a fineness modulus of 2.55 to 

differentiate from its natural value of 2.97 (used in all other mixtures). Mixes 9–11 required the 

addition of various fly ashes to the base mix design. In these mixes the fly ashes were added as a 

percentage replacement by weight of cement. 

Mixing procedures were altered from those specified in AASHTO T 126, “Making and Curing 

Concrete Test Specimens in the Laboratory,” to simulate field mixing technique typical of 

paving concrete. The modification was that a 2-min mixing cycle was used. 

The dosage of air entrainer was varied for each mixture to obtain air contents in the range of 6 ± 

1 percent. A fixed dosage of WRA was applied in all mixtures except for mixes 4 and 6. No 

water reducer was added in mix 4, and in mix 6 the dosage was doubled. Because of the 
123 

variability of mixture conditions, the dosage of water reducer that provided an approximate 

100-mm (4-inch) slump for mix 1 was used as the fixed dosage for the rest of the program. 

Table 46. Base concrete mixture. 

Material kg/m3 Pounds per cubic yard 

Cement 335 564 

Fine aggregate, SSD 715 1205 

Coarse aggregate, SSD 1103 1860 

Water 141 237 

Approximate w/c 0.42 0.42 

Stage 3—Hardened Concrete Analysis 

In this stage of the investigation, the properties of hardened concrete were determined to evaluate 

the validity of correlations to the fresh property tests established in the first and second stages. 

Stage 3 tests were conducted on the same concrete mixtures made during the Stage 2 study (see 

table 46). These tests were as follows: 

• Compressive strength: Six 100- by 200-mm (4- by 8-inch) cylinders were tested for 

compressive strength in accordance with AASHTO T 22, “Compressive Strength of 

Cylindrical Concrete Specimens,” at the ages of 7 and 28 days. 

• ASTM C 457, “Microscopical Determination of Parameters of the System in 

Hardened Concrete.” A specimen was cut from the 150- by 150- by 530-mm (6- by 

6- by 21-inch) beam for this test. The cut was through the cross-section to show the 

variation in system between the top and bottom of the beam. 

• Characterization of flocculation of air voids around coarse aggregates. The same 

specimens prepared for ASTM C 457 were used to assess clustering. 

In cases where flocculation or clustering of air voids around coarse aggregates was witnessed, a 

technique developed in a past PCA study was used to rate the severity of the phenomenon.(68)

According to the PCA study, a visual reference shown in figures 44 through 47 was developed to 

standardize the determination of clustering severity around individual aggregates. This reference 

standard is composed of four categories to differentiate between no clustering, minor, moderate, 

and severe air void clustering. Each category was assigned a numeric value of 0 to 3. A rating of 

0 implies that no clustering exists. Minor clustering (Rating 1) involves the intermittent 

occurrence of clustering of entrained air voids around the periphery of coarse aggregate particles. 

For moderate clustering (Rating 2), most or all of an aggregate is surrounded by a layer of 

entrained air voids. Severe clustering (Rating 3) is defined as several layers of entrained air voids 

surrounding a single aggregate particle. 

According to the method outlined in the PCA study, only coarse aggregate particles greater than 

0.25 inch were given a rating.(69) Because lapped sections of concrete were being evaluated, the 

nominal size of an aggregate evaluated in the cut plane of those samples was unknown. An 

aggregate that appeared small on the lapped surface could have been the tip of a much larger 
124 

particle. It is not known if a relationship between the size of a clustered aggregate particle and 

the magnitude of the resultant compressive strength loss exists; therefore, all aggregate diameters 

6 mm (0.25 inch) and larger were given consideration. 

Note: Millimeter scale 

Figure 44. Rating 0–No clustering present. 

Visual rating guide for analysis of air void 

clustering severity (PCA R&D 

Serial No. 2789). 

Figure 45. Rating 1, Minor clustering 

Visual rating guide for analysis of air void 

clustering severity (PCA R&D 

Serial No. 2789). 
125 

Figure 46. Rating 2, Moderate clustering. 

Visual rating guide for analysis of air void 

clustering severity (PCA R&D 

Serial No. 2789). 

Figure 47. Rating 3, severe clustering. 

Visual rating guide for analysis 

of air void clustering severity 

(PCA R&D Serial No. 2789). 

An example analysis and calculation of the average clustering rating for a lapped concrete 

sample is presented in figure 48. Table 47 shows the corresponding calculations. To improve the 

consistency of ratings, samples were marked off 2.54 cm (1 inch) from the top and bottom and 

the central 10.16-cm (4-inch) section was analyzed for clustering. As shown in figure 48, each 

coarse aggregate particle was assigned to one of the four clustering categories. Then the number 

of aggregates in each category was multiplied by the category or number (0 to 3). Finally, the 

totals from each category were averaged over the number of particles examined. 
126 

Unit conversions: 

1 inch = 2.54 cm 

Figure 48. Example of clustering rating for a cylinder. 

Table 47. Corresponding calculations 

for average clustering rate. 

Clustering Rating Aggregates Affected Calculation 

0–None 39 0 × 39 = 0 

1–Minor 24 1 × 24 = 24 

2–Moderate 2 2 × 2 = 4 

3–Severe 0 3 × 0 = 0 

Sum 65 28 

Clustering rate = 28/65 = 0.43

0

0

0

1

0

0

2

0

0

0

1

0

0

2 1

0

0

0

0

0

0

0

0

0

1

0

0

1

1

0

0

0

1

1

0

1

1

0

0

1

1

1

0

0

0

0

1

0 1

0

0 1

0

0

1

1

1

0

0

1

0

1

0

1

1
127 

Results 

Stage 1—Foam Drainage Analysis 

The foam drainage results for the 10 admixtures included in this study are presented in table 48. 

Results for V0, −1/k, and percentage drained were ranked based on a scale of 1 to 10, with 10 

being the best and 1 being the worst performer. Admixtures B, D, and H were selected for 

concrete analysis based on variations in their foam stability to determine if similar air void 

stability issues could be predicted in concrete mixtures. These three admixtures consisted of the 

top, middle, and worst performers among the group based on their overall ranking. The overall 

rankings shown in table 48 were determined by averaging all the individual performances 

(Vo, −1/k, and percentage drained) for each admixture. 

Table 48. Foam drainage results. 

Admixture Admixture Test

ID Classification Condition V0 -1/k r

2

% drained V0 -1/k % drained Overall

AEA 301.0 6.5 0.445 97.1 2 1 1

AEA+C 269.0 390.1 0.932 86.8 4 7 4

AEA+WR 303.0 330.2 0.986 97.7 1 3 1

AEA+C+WR+C-ASH 232.0 615.2 0.982 74.8 9 4 9

AEA+C+WR+F-ASH 235.0 714.7 0.978 75.8 10 8 10

AEA 285.0 285.2 0.993 91.9 8 6 8

AEA+C 210.0 531.9 0.956 67.7 9 9 9

AEA+WR 228.0 905.4 0.944 73.5 8 5 8

AEA+C+WR+C-ASH 239.0 713.4 0.968 77.1 7 7 7

AEA+C+WR+F-ASH 245.0 794.4 0.985 79.0 8 10 8

AEA 301.0 348.7 0.974 97.1 1 8 2

AEA+C 102.0 1191.0 0.793 32.9 10 10 10

AEA+WR 212.0 955.3 0.942 68.4 10 9 10

AEA+C+WR+C-ASH 252.0 623.9 0.983 81.3 5 5 5

AEA+C+WR+F-ASH 250.0 661.8 0.979 80.6 4 5 6

AEA 293.0 101.4 0.991 94.5 5 4 5

AEA+C 253.0 182.9 0.986 81.6 8 5 8

AEA+WR 233.0 928.6 0.965 75.2 7 6 7

AEA+C+WR+C-ASH 249.0 697.1 0.984 80.3 6 6 6

AEA+C+WR+F-ASH 250.0 715.6 0.978 80.6 5 9 4

AEA 281.0 64.7 0.973 90.6 10 3 10

AEA+C 264.0 81.6 0.973 85.2 5 3 5

AEA+WR 267.0 1030.0 0.959 86.1 5 10 5

AEA+C+WR+C-ASH 236.0 817.9 0.981 76.1 8 10 8

AEA+C+WR+F-ASH 240.0 712.7 0.982 77.4 9 7 9

AEA 291.0 120.4 0.969 93.9 7 5 7

AEA+C 259.0 232.0 0.970 83.5 6 6 6

AEA+WR 239.0 938.4 0.946 77.1 6 7 6

AEA+C+WR+C-ASH 252.0 713.5 0.988 81.3 4 8 4

AEA+C+WR+F-ASH 247.0 639.1 0.971 79.7 7 4 7

AEA 298.0 734.8 0.920 96.1 4 10 4

AEA+C 299.0 420.7 0.960 96.5 1 8 1

AEA+WR 291.0 467.0 0.904 93.9 3 4 3

AEA+C+WR+C-ASH 302.0 488.2 0.961 97.4 1 3 1

AEA+C+WR+F-ASH 299 334.1 0.928 96.5 2 3 2

AEA 300 297.5 0.945 96.8 3 7 3

AEA+C 288 33.4 0.964 92.9 2 2 2

AEA+WR 294 76.8 0.875 94.8 2 2 2

AEA+C+WR+C-ASH 299 30 0.963 96.5 2 1 2

AEA+C+WR+F-ASH 304 29.47 0.947 98.1 1 1 1

AEA 282.0 51.2 0.897 91.0 9 2 9

AEA+C 257.0 87.4 0.985 82.9 7 4 7

AEA+WR 227.0 938.7 0.932 73.2 9 8 9

AEA+C+WR+C-ASH 228.0 800.9 0.978 73.5 10 9 10

AEA+C+WR+F-ASH 250.0 696.0 0.983 80.6 6 6 5

AEA 293.0 408.1 0.952 94.5 6 9 6

AEA+C 281.0 21.7 0.976 90.6 3 1 3

AEA+WR 288.0 23.5 0.925 92.9 4 1 4

AEA+C+WR+C-ASH 289.0 89.2 0.976 93.2 3 2 3

AEA+C+WR+F-ASH 290.0 69.0 0.981 93.5 3 2 3

Notes: * Rankings based on a scale of 1 to 10, with 10 being the best and 1 being the worst performer.

Foam Drainage Statistics 

resin/rosin

vinsol

benzene 

sulfonate

vinsol

fatty acid

resin/rosin

vinsol

alpha sulfonate

E

F

G

H

A

B

C

D

5

2

tall oil 1

resin/rosin

9

3

Rank*

I

J

4

10

7

6

8
128 

Stage 2—Fresh Concrete Properties and Air Void Analyzer Investigation 

The fresh properties including slump, air, and unit weight of the 13 concrete mixtures are 

presented in table 49. Table 49 also includes the air void system properties determined using the 

AVA. 

The correlation between fresh air contents generated using the pressure meter (ASTM C 231) 

and AVA is shown in figure 49. 

Total Fresh Air Content - Pressure Meter vs. AVA

0

1

2

3

4

5

6

7

8

9

02468

Pressure Meter, %

AVA, %

Figure 49. Correlation between pressure meter and AVA-generated fresh air contents. 

Stage 3—Hardened Concrete Analysis 

Hardened properties for the 13 concrete mixtures are presented in table 50. The data includes 

compressive strengths results and petrographic air void parameters. Compressive strengths of 

these mixes were evaluated at ages of 7 and 28 days. Petrographic analyses were performed on 

the hardened concrete samples to determine their total air void contents, spacing factors, and 

evidence of air void clustering. 
129

Table 49. Fresh concrete properties. 

Concrete Mix Variables Fresh P

Mix No. AEA Type Sand Gradation Water Reducer Water- Reducer Dosage Temperature Pozzolans Consolidation Slump (mm) Unit weight (kg/m3) A

(%

1 B Normal A Normal Normal None Normal 

Vibration 

90 2,355 6

2 H Normal A Normal Normal None Normal 

Vibration 

160 2,348 7

3 D Normal A Normal Normal None Normal 

Vibration 

95 2,342 6

4 H Normal None Not 

applicable

32 °C None Normal 

Vibration 

50 2,347 6

5 H Normal A Normal 32 °C None Normal 

Vibration 

75 2,340 6

6 H Normal B High Normal None Normal 

Vibration 

175 2,344 6

7 H Coarse A Normal Normal None Normal 

Vibration 

20 2,372 5

8 D Coarse A Normal Normal None Normal 

Vibration 

25 2,372 5

9 H Normal A Normal Normal 20% (C) 

fly ash A 

Normal Vibration 

120 2,327 6

10 H Normal A Normal Normal 20% (C) 

fly ash B 

Normal Vibration 

125 2,360 5

11 H Normal A Normal 32 °C 20% (F) fly 

ash 

Normal Vibration 

65 2,327 6

12 D Normal A Normal Normal None Excessive 

Vibration 

75 2,315 6

13 B Normal A Normal Normal None Excessive 

Vibration 

120 2,363 6

Unit conversions: 

1 kg/m3 = 1.69 pcy 
130

Table 50. Hardened concrete properties. 

 Concrete Mix Variables Hardened 

Mix 

No. 

AEA 

Type 

Sand 

Gradation 

Water 

Reducer 

WaterReducer Dosage 

Temperature Pozzolans Consolidation 

Strength 

7 Day 

(MPa) 

Strength 

28 Day 

(MPa) 

Air 

(%) 

Sp

Fa

(m

1 B Normal A Normal Normal None Normal 

Vibration 

30.0 33.9 5.8 0

2 H Normal A Normal Normal None Normal 

Vibration 

24.0 31.9 5.5 0

3 D Normal A Normal Normal None Normal 

Vibration 

24.2 32.5 6.4 0

4 H Normal None Not 

applicable

32 °C None Normal 

Vibration 

25.6 29.7 5.5 0

5 H Normal A Normal 32 °C None Normal 

Vibration 

30.7 36.4 5.1 0

6 H Normal B High Normal None Normal 

Vibration 

21.8 27.6 6.1 0

7 H Coarse A Normal Normal None Normal 

Vibration 

32.5 36.7 4.5 0

8 D Coarse A Normal Normal None Normal 

Vibration 

32.1 35.8 4.9 0

9 H Normal A Normal Normal 20% (C) 

fly ash A 

Normal Vibration 

25.6 38.7 3.3 0

10 H Normal A Normal Normal 20% (C) 

fly ash B 

Normal Vibration 

28.5 38.0 4.7 0

11 H Normal A Normal 32 °C 20% (F) fly 

ash 

Normal Vibration 

26.0 33.9 4.7 0

12 D Normal A Normal Normal None Excessive 

Vibration 

24.3 33.9 5.8 0

13 B Normal A Normal Normal None Excessive 

Vibration 

26.4 34.9 5.1 0

Unit conversions: 

1mm =0.0394 inch 1 MPa = 145.0 psi 
131 

Correlations between air void parameters generated from the pressure meter, petrographic, and 

AVA analyses are presented in the following figures. Figure 50 presents the correlation between 

total air void contents generated by ASTM C 457 and pressure meter analyses. Figure 51 

presents the correlation between total air void contents generated by ASTM C 457 and the AVA 

analyses. The spacing factor correlation between the ASTM C 457 and AVA analyses is shown 

in figure 52. Finally, the air content versus spacing factor relationship for the ASTM C 457 and 

AVA analyses are shown in figure 53. 

Figure 50. Correlation of total air contents between pressure 

meter and ASTM C 457. 

Figure 51. Correlation of total air contents between AVA 

and ASTM C 457. 

0

2

4

6

8

10

0 2 4 6 8 10

ASTM C 457, %

Pressure Meter, %

0

2

4

6

8

10

0 2 4 6 8 10

ASTM C 457, %

AVA, %
132 

 Unit conversions: 

 1 mm =0.0394 inch 

Figure 52. Correlation between AVA and ASTM C 457 generated 

spacing factors. 

Figure 53. Spacing factor versus air content relationship for 

ASTM C 457 and AVA. 

0.00

0.10

0.20

0.30

0.40

0.50

0.60

0.00 0.10 0.20 0.30 0.40 0.50 0.60

ASTM C 457, mm 

AVA, mm

0.000

0.100

0.200

0.300

0.400

0.500

0.600

0.0 2.0 4.0 6.0 8.0 10.0

Air Content

Spacing Factor

AVA

457
133 

Summary 

The foam drainage test was used to screen admixtures in this study. The test method was used to 

evaluate the effects of various concrete raw materials on the stability of foams generated from 

different air entraining admixtures. Foam drainage parameters for the 10 admixtures evaluated in 

this study were ranked on a scale from 1 to 10, where 1 represented the worst performer and 10 

represented the most stable admixture under all conditions. The overall rankings shown in 

table 48 were determined by averaging all the individual performances (Vo, -1/k, and percentage 

drained) for each admixture. The best, middle, and worst performers or admixtures B, D, and H 

respectively were chosen for further evaluation in concrete mixtures to determine if a similar link 

to concrete air void quality existed. It was notable that some admixtures appeared to be sensitive 

to the presence of supplementary cementing materials and water reducing admixture (E), while 

others were not. Also of interest was that some air entraining admixtures appeared to perform 

well in this test when tested alone, but were less satisfactory when tested with cementitious 

systems (F), or vice versa (A, B). It is advisable that if this test is used in the field, the full 

system should be tested and not the AEA alone. 

Concrete mixtures reported to have produced poor air void systems in the field were chosen to 

evaluate these admixtures. The 13 concrete mixtures chosen for evaluation are shown in table 45. 

The most unstable admixture was used in 8 of the 13 mixtures, while the top performer was used 

in two of the mixtures for comparison. Little correlation was observed in the effects of the 

variables changed in this test matrix. 

According to most authorities, spacing factor and specific surface values calculated from an 

ASTM C 457 petrographic analysis can determine the potential freeze/thaw durability of a 

concrete mixture. Concrete mixtures with a spacing factor below 0.200 mm (0.008 in) and 

specific surface greater than 24 mm2

/mm3 (600 inch2/inch3) are thought to be freeze/thaw 

durable. Reviewing the ASTM C 457 results for the 13 concrete mixtures presented in table 50, 

only mix 10 failed the parameters discussed above. 

Mix 10 was made using the most unstable admixture (H) as identified by the foam drainage test; 

however, this was the only mixture of the eight made with admixture H that was found to be 

outside the range of recognized air void parameters. It would appear that there is little correlation 

between the foam drainage test and the other parameters measured in this work. There is still 

potential value in the test as being an indicator of the stability of an air void system with time in 

the fresh concrete. These properties were not investigated as part of the concrete work here, but 

there are reports from the field of air content of a fresh mix changing with continued transporting 

and handling. This test would be a useful indicator in such an application. The test was also 

shown to be sensitive to changes in cementitious materials and may also have value as a monitor 

of system uniformity. 

A review the correlations between air void parameters obtained using the pressure meter (ASTM 

C 231), AVA, and ASTM C 457 analyses show considerable scatter in the AVA data. The 

correlation of total air contents between the pressure meter and AVA shown in figure 49 is much 

more scattered when compared to the similar relationship between the ASTM C 457 and pressure 

meter presented in figure 50. The correlation between ASTM C 457 and AVA spacing factors 

shown in figure 52 shows significant scatter. There are reports that the instrument is being 
134 

successfully used as a quality management tool. It may be that the test is appropriate for use in a 

situation where the same, or similar, mixes are repeatedly tested from batch to batch. In that case 

it is more the repeatability of the results that is important than the absolute numbers obtained. 

These limited data indicate the test may not be immediately appropriate for testing a variety of 

mixtures without some form of calibration. 

Of the 13 concrete mixtures made, only 3 showed signs of air void clustering when analyzed 

according to the clustering rating system. All three of these mixtures were made using the most 

unstable admixture (H). In addition, two of the three mixtures where clustering occurred were 

mixed at 32.2 oC (90 oF). This supports the belief that clustering is more prone to occur during 

the summer months when mixing temperatures are generally higher. The third mixture in which 

clustering occurred was made with a high dosage of water reducer. 

Another test that was not conducted as part of this work has a history of being useful. The test is 

the foam index test. When used as a quick indicator of variability in cementitious materials 

(particularly fly ash), it has potential as a field materials acceptance test. 
135

CHAPTER 4. SUMMARY 

INTRODUCTION 

As indicated in the preceding sections, a large number of mechanisms and effects contribute to 

so-called incompatibility. Many of these are complex and interrelated. This means that there is 

no simple means of providing a reliable measure of the risk of incompatibility. Some test 

methods are suitable for indicating risk of problems in the first 30 min because of 

aluminate/sulfate balance issues, while others are suitable for detecting later silicate hydration 

problems, and none is ideal for both. 

There is a general trend that the lower-cost rugged tests are more prone to scatter and less 

sensitive than the more expensive delicate tests. Many of the tests take a long time to conduct, 

which is problematic for field application where an answer may be required in a few hours. 

One of the interesting aspects of interpreting the data from the laboratory work conducted was 

that there was no clearly marked system identified as “incompatible” with a companion sample 

labeled “compatible.” Part of the work in assessing test methods to identify incompatibility was 

to use the same test methods to assess the apparent incompatibility of the test mixtures. 

It was also observed that in many of the tests, there was no threshold that clearly indicated 

whether any given system was incompatible or not. A result that may be considered poor for one 

system may be considered acceptable for another. The greatest value of many of these tests is in 

monitoring the uniformity of a system over time. A marked change in a test result would indicate 

potential problems that would need to be investigated using other means. This tracking would 

need to be based knowing the acceptable ranges for that system, for the environment in which it 

is being used. 

In seeking to develop a test protocol, there is some value in understanding and summarizing the 

multiple and complex mechanisms that are at play when considering the wide-ranging problem 

of incompatibility. 

EARLY SETTING AND EXCESSIVE RETARDATION 

Hydraulic cement systems stiffen, set, and harden by a series of nonreversible chemical reactions 

with water, a process called hydration. This process is complex, and it still is the subject of 

extensive research. A discussion of the broad principles follows. 

Cement Chemistry 

Portland cement and cementitious materials comprise the same family of chemical elements. 

Chemical analyses of cementitious materials by X-ray fluorescence report the elements as 

oxides. This is for convenience only because these elements are not all likely to be present as 

pure oxides. The same convention is followed below. 

Calcium oxide. Normally comprises 60 to 65 percent of cement by mass, while silica normally 

contributes about 20 percent. These combine to form the so-called “silicates,” C2S and C3S. The 
136

hydration products (the compounds formed when they react with water) of C2S and C3S are 

similar to each other, albeit in different proportions. Hydration of silicates also produces some 

heat (figure 54). Calcium silicate hydrate (CSH) is the primary compound that gives hydrated 

cement paste the strength and impermeability that makes concrete useful in construction. 

Calcium hydroxide (CH) forms hexagonal crystals that do not contribute significantly to 

strength, but can be readily dissolved by acids and soft water. 

C3S, also known as “alite,” is the compound that contributes to setting and early strength 

development of concrete. The contribution normally begins a few hours after mixing. C2S, also 

known as “belite,” is the primary compound that contributes to later strength development of 

concrete. The contribution is considered to begin about a week after mixing. Portland cements 

currently contain approximately 60 percent C3S and 20 percent C2S. 

Alumina. Included in the mixture introduced into a cement kiln because it helps to reduce the 

burning temperatures required to make cement. Iron oxide is also normally present in the raw 

materials. Alumina combines with calcium and iron oxide to form two aluminate compounds: 

C3A and C4AF. Typical portland cements contain approximately 5–8 percent C3A and 8–12 

percent C4AF. C4AF reactions do not contribute significantly to the properties of concrete except 

the gray color. C3A reacts very rapidly when mixed with water and generates a large amount of 

heat (figure 54), unless it is controlled by the presence of calcium and sulfate. 

Calcium sulfate. Added to clinker during grinding at about 5 percent dosage to control the initial 

reaction of C3A. The dosage is carefully optimized because the strength of a cement is influenced 

by the amount of sulfate, and incompatibility (including uncontrolled stiffening and setting) can 

occur if the of amounts of C3A and sulfate are out of balance. Calcium sulfate is normally 

present in three forms, depending on the amount of water tied to the compounds. These are 

described in table 51. 

Table 51. Compounds of calcium sulfate in cement. 

Compound Shorthand Notation 

Anhydrous calcium sulfate (anhydrite) CS ̄

Calcium sulfate dihydrate (gypsum) CS ̄H2

Calcium sulfate hemihydrate (plaster 

or bassanite) CS ̄H1⁄2

The reaction products of C3A and sulfate are complex and change with time from mainly 

amorphous hydrates to form more crystalline hydrates over time, such as ettringite and 

monosulfoaluminate hydrate (figure 54). The formation of syngenite also appears to be a 

potentially significant factor. 

Hydration Reactions and Development of Microstructure 

Hydration begins as soon as cementitious materials come in contact with water. The particles 

partially dissolve and the various components start to react at various rates. 
137

There is no single mechanism behind the wide range of effects that are occurring. Many of the 

mechanisms are complex and interactive and may require expert evaluation if they occur in the 

field. Following are discussions of some of the chemical reactions that are occurring. 

Early Reactions. Cement hydration in the first 15 min is a delicate balance between the C3A in 

the cement, and sulfate in solution slowing the C3A reaction (figure 54). If there is insufficient 

sulfate in solution, the C3A begins to react immediately to form calcium aluminate hydrate, 

which can cause flash (immediate and permanent) set if it is not controlled. C3A hydrates at a 

more controlled rate in the presence of sulfate to form ettringite while there is sulfate in solution. 

When the sulfates are consumed, ettringite continues to react to form monosulfate (figure 54). 

On the other hand, too much sulfate in solution may precipitate out as gypsum, causing false 

(temporary) set. These reactions are the basis of many incompatibility problems. 

The amount of sulfate in solution is dependent not only on the amount of sulfate ion in the 

cement, but the form in which it occurs. Cement that has overheated in the mill may contain 

excess amounts of relatively fast dissolving plaster (CaSO4·1⁄2H2O). Cement manufacturers will 

normally target a balance of plaster and gypsum (CaSO4·2H2O) suitable for the reactivity of a 

given clinker type and cement fineness, and they will optimize the sulfate content to balance the 

setting time of the concrete. 

Addition of a supplementary cementitious material that contains additional calcium aluminates 

(typically high-calcium fly ash) can mean that the aluminate/sulfate balance can be 

compromised, causing the problems discussed above. 

The fineness of the cement will also influence the reaction rates. The finer the cement is, the 

greater the risk of uncontrolled C3A reactions with other ingredients in the concrete. 

Some chemical admixtures will interfere with C3A hydration and the solubility of calcium and 

sulfate in the pore solution; thus, they may significantly affect the workability of the concrete in 

the first few minutes. Type A water reducers tend to accelerate aluminate hydration and retard 

silicate hydration. Some chemical admixtures may reduce early slump when used with some 

cementitious combinations. 
138

Unit conversions: 

1 J/g/h (joule per gram per hour) = 0.008 calories per ounce per hour 

Figure 54. Reactions in hydrating cement. 

The solubility and reactivity of all of the compounds are also strongly influenced by temperature, 

with higher temperatures generally increasing solubility (except calcium) and accelerating 

reaction rates. These changes can affect the balance of the system and change stiffening rates and 

setting times. 

Later reactions. After a dormant period of 1 to 3 h, the silicates (C3S and later the C2S) start to 

hydrate. They form fibrous growths of calcium-silicate-hydrate (CSH) that gradually spread and 

merge with the growth from other cement particles or adhere to aggregate particles. This build up 

of new solid compounds results in progressive stiffening, hardening, and strength development. 

This reaction proceeds as long as the system contains water, explaining the need for curing. 

Increasing alkali content and cement fineness, along with increasing temperature will increase 

reactivity of the silicate components and decrease setting times. Increasing reactivity will also 

tend to increase the rate of gain of stiffness, which may increase the risk of cracking. 

The presence of some chemical admixtures will affect the reaction rates, often retarding setting. 

Type A water-reducing admixtures may retard silicate hydration. 

The saturation of calcium may also affect the hydration of C3S, which in turn is influenced by the 

reactions in early stages of hydration discussed above. Insufficient calcium in solution (that is, if 

Troubleshooting presentations

Gypsum

CS ? Gypsum deposition (False set)

Gypsum depletion

Aluminate reactions

C3A + CH + 12H ? C 4AH13 ** Hopefully never (flash set)

C3A + 3CS + 26H ? C 3A•3CS•H32 (Ettringite) **

2C3A + C3A•3CS•H32 + 4H ? 4(C 3A•CS•H12) (Monosulfate)

Silicate reactions

2C3S + 6H ? CSH + 3CH *

2C2S + 4H ? CSH + CH * Later

* Retarded by sugar / lignin

** Accelerated by sugar / lignin

0

5

10

15

20

25

0:00 6:00 12:00 18:00 0:00

Time of hydration (h)

J/g/h

Working time

Initial set

Final set

"Sulfate depletion"

(ettringite to monosulfate

conversion)

Strength 

development
139

it has been consumed in early C3A hydration) will slow or stop silicate hydration, leading to 

retardation of the concrete or failure to set. 

Dimensional Stability and Cracking 

Concrete, and all of the components within it, tend to grow and shrink with changing 

temperatures, moisture conditions, and in some cases chemical reactions. By nature of its 

composition, concrete is mixed with water, some of which is consumed in hydration and some of 

which may leave the system by bleeding or evaporation as the concrete is allowed to dry. 

Hydrated cement paste is generally the phase that changes the most with changing moisture 

content, which is why it is recommended that the paste content of a mixture be minimized within 

constraints imposed by other requirements such as strength or impermeability. 

The space occupied by the reagents of cement hydration is less than that of the hydrated system. 

This results in so called chemical shrinkage, and autogenous shrinkage (the amount of chemical 

shrinkage that can be measured). This phenomenon is greatest in systems with low w/cm. 

Other chemical reactions including alkali aggregate reaction and sulfate attack may cause 

dimensional change in concrete, but these are outside the scope of this project. 

All of the materials in concrete expand and shrink with changing temperature and moisture 

content. The consequences of these dimensional changes are a function of other properties of the 

concrete including restraint, stiffness, strength, and creep. A freestanding object that is not 

restrained internally or externally will shrink without damage; however, external restraint is 

almost always applied to concrete elements by their support systems and connections to adjacent 

elements. Internal restraint is also imposed by the different components (aggregates, paste) 

having different stiffness values and likely different amounts of dimensional movement. Such 

restraint will result in cracking. 

The amount of stress set up in a shrinking, restrained material is a direct function of its stiffness 

(modulus of elasticity) with stiffer materials resulting in higher stresses. Creep helps to mitigate 

the amount of stress. The risk of cracking is governed by the balance of imposed stress and the 

material strength. 

Adding to the complexity of this issue is that all of these properties are changing with time as the 

concrete hydrates, with the changes occurring rapidly at early ages and slowing with age, and 

with the changes occurring at different rates for the different properties. The rate of hydration 

will be influenced by the temperature and chemistry of the reactive materials. The rate of drying 

(and associated shrinkage) will also be influenced by the temperature and the environment to 

which the concrete is exposed. The rates and degree of temperature change are governed by the 

dimensions of the element, the environment, and the chemistry and degree of hydration. 

Computer models are available to assess the risk of cracking in concrete pavements based on 

these parameters. Part of the work conducted in this project has been to determine the relative 

rates of change of strength and stiffness of the concrete mixtures tested. 

The current standard test for concrete shrinkage (ASTM C 157) does not provide any 

information about the dimensional movement of concrete for the first 24 h, and limited 
140

information before drying is allowed to start; however, such information is required if early age 

cracking is to be better understood and prevented. The ring shrinkage test provides a controlled 

method of tracking shrinkage-related stresses in a concrete under restraint from the time that the 

concrete is placed in the mold. 

Air Void System 

It is important that a proper air void system be provided to concrete if it is to be protected from 

frost damage. Such a system may be considered as a uniform distribution of a large number of 

small air bubbles, the critical parameter being the maximum distance from any point in the paste 

to the nearest bubble. 

The quality of an air void system is strongly influenced by the chemistry of the cementitious 

materials, particularly the carbon content of fly ash, if present. Different air-entraining 

admixtures will also produce different air void systems, with some materials being strongly 

influenced by the presence of other chemical admixtures and supplementary cementing 

materials. The grading of the fine aggregate will also influence development of the system along 

with the amount of mixing energy provided. It is easier to entrain air in a mixture with a higher 

slump than in one with a lower slump. The air void system of a concrete will also change with 

continued handling, placing, and compacting effort. 

It is desirable that the spacing factor be determined in concrete, particularly in the fresh state to 

allow early decisions regarding its acceptability. It may also be preferred to measure it in the 

final position to allow for the effects of handling; however, there are no proven means of 

conducting this determination at present, making it important to be able to correlate final spacing 

factor with other, more easily measured parameters such as total air content measured using a 

pressure meter. 

PROTOCOL 

The protocol has been developed on the premise of developing as much information as possible 

in a prequalification phase. This work would include calibrating the more sensitive central 

laboratory tests with the equivalent field tests using materials that are likely to be used in the 

field and under environments likely to be experienced in the field. The work may also include 

preparing alternative mix proportions and practices to accommodate changes in environment or 

changes in materials sources. Tests in the field would be based on the more portable tests being 

conducted regularly, primarily to monitor the uniformity of the materials and the final mixture as 

discussed above. 

Most of the tests conducted in this work have some value, and the extent of prequalification and 

field testing will need to be based on the availability of equipment and the relative cost of testing 

compared to the cost and risk of failures. A typical example is the determination of setting time, 

which can be achieved by up to six different techniques, any of which is acceptable, and the 

selection of which should be based on the other requirements and conditions at the site. 

It is likely that a relatively simple suite of field tests conducted regularly will provide much of 

the reassurance needed that a concrete mixture will perform satisfactorily: 
141

• Foam index. 

• Foam drainage. 

• Slump loss. 

• Unit weight. 

• Semi-adiabatic temperature monitoring. 

• Setting time. 

• Chemistry of reactive materials. 

Obtaining information of the materials’ chemistry in the detail required for individual batches 

may be problematic. For a large project with significant costs associated with failure, 

negotiations may be made with the suppliers to conduct the reviews as part of the existing quality 

control and to provide certification that a set of critical parameters such as C3A content has not 

changed by more than X percent between loads. 

The protocol is presented in volume II. 

IMPLEMENTATION PLAN 

It is important the information generated in this project be implemented in the construction 

industry to reduce the occurrence of incompatibility and its attendant costs. Because many of the 

test methods are already standardized or in use, the primary need for guidelines and an 

implementation plan is to increase awareness about this work and the accompanying protocols 

among the makers and users of concrete. The intended audience of this report is State 

departments of transportation representatives, as well as contractors and ready-mix suppliers 

involved in pavement construction. 

In addition, it is suggested that the recommended test methods that have not been standardized 

should be submitted to relevant authorities for adoption. 

Publications 

The findings of this work will be disseminated in publications. In addition to the project report, a 

TechBrief publication summarizing the findings will be published by the Federal Highway 

Administration (FHWA) and a technical paper will be available for consideration in applicable 

journals. 

Presentations 

The topic of this project has been the subject of at least six presentations already made at the 

Transportation Research Board (TRB) and several state and local ACPA symposia. A prepared 

presentation is provided in Microsoft® PowerPoint® format along with this report. 

Standards 

The test methods that are not currently standardized have been prepared in AASHTO format and 

should be submitted to AASHTO or ASTM, or both, for adoption.

143

ACKNOWLEDGEMENTS 

The authors wish to acknowledge the work of the following people in completing the work 

described in this report: 

From the CTLGroup: 

Katie Amelio 

Pat Berry 

Barb Betke 

Javed Bhatty 

Fred Blaul 

Phil Brindisi 

Roberto Celestin 

Luis Duval 

Ken MacLeod 

Greg Miller 

Mohamad Nagi 

Agata Pyc 

Brian Szczerowski 

Shiraz Tayabji 

From Braun Intertec: 

Rachel Detwiler 

From NIST: 

Max Peltz 

John Winpigler 

DISCLAIMER 

Commercial equipment, instruments, and materials mentioned in this paper are identified to 

foster understanding. Such identification does not imply recommendation or endorsement by the 

authors or NIST, nor does it imply that the materials or equipment identified are necessarily the 

best available for the purpose. 

MATCHING FUNDS 

CTLGroup was required to provide a minimum of a 20 percent match of the Federal funding 

toward the project. The matching funds were obtained by reaching agreement with the Portland 

Cement Association. No specific task was solely funded by PCA, but rather, a proportion of 

every payment due through the duration of the project was invoiced to PCA. PCA’s total 

contribution was $110,000 of the total estimated project cost of $451,245.

145

REFERENCES 

1. Gress, D., Early Distress in Concrete Pavements, Federal Highway Administration, 

FHWA-SA-97-045, Washington, DC, January 9, 1997, pp. 53. 

2. Whiting, D., Addendum to NCHRP Report 258, Control of Air Content in Concrete, 

Appendix F, State-of-the-Art Report, Portland Cement Association, Skokie, IL, 1983, 

263 pp. 

3. Stark, D.C., Effect of Vibration on the Air void System and Freeze-Thaw Durability of 

Concrete, PCA Research & Development Bulletin RD092.01TT, Portland Cement 

Association, Skokie, IL, 1986. 

4. Tymkowicz, S. and Steffes, R., Vibration Study for Consolidation of Portland Cement 

Concrete, Report No. MLR-95-4, Iowa Department of Transportation, January 1997, 

94 pp. 

5. Jennings, H., Johnson, D.L., Moss, G.M., and Saak, A.W. Pooled Fund Study of 

Premature Rigid Deterioration, Iowa Department of Transportation Research Project H1063, Northwestern University Technological Institute, Evanston, IL, April 1997, 94 pp. 

6. Powers, T.C., The Properties of Fresh Concrete, John Wiley & Sons, New York, 1968. 

7. Whiting, D.A. and Nagi, M.A., Manual on Control of Air Content in Concrete, EB116, 

Portland Cement Association, Skokie, IL, 1998. 

8. Stutzman, P.E. Deterioration of Iowa Highway Concrete Pavements: A Petrographic 

Study, NISTIR 6399, National Institute of Standards and Technology, December 1999, 

72 pp. 

9. Simon, M.J.; Jenkins, R.B.; and Hover, K.C. “The Influence of Immersion Vibration on 

the Void System of Air Entrained Concrete,” Durability of Concrete: G.M. Idorn 

International Symposium, Toronto, ON, Canada, ACI SP-131, Jens Holm and Mette 

Geiker, Eds., American Concrete Institute, 1992, pp. 99–126. 

10. Kosmatka, S.H., Kerkhoff, B. and Panarese, W.C., Design and Control of Concrete 

Mixtures, 14th Edition, EB001.14T, Portland Cement Association, Skokie, IL, 2002, 

355 pp. 

11. Senbetta, E. and Malchow, G. “Studies of Control of Durability of Concrete Through 

Proper Curing,” Concrete Durability, Katharine and Bryant Mather International 

Conference, ACI SP-100, J.M. Scanlon, Ed., American Concrete Institute, 1987, 

pp. 73–87. 

12. Hansen, W.C., “False Set in Portland Cement,” Proceedings of the 4th International 

Symposium on the Chemistry of Cement, Washington DC, 1960, pp. 387–428. 
146

13. Neville, A., “The Question of Concrete Durability: We Can Make Good Concrete 

Today,” Concrete International, Vol. 22, No. 7, July 2000, pp. 21–26. 

14. Sandberg, P.J. and Roberts, L.R., “Cement-Admixture Interaction Related to Aluminate 

Control,” Jr. ASTM International, Vol. 2, No. 6, June 1, 2005, pp.1–14. 

15. Wadso, L., “Unthermostated Multichannel Heat Conduction Calorimeter,” Cement, 

Concrete, and Aggregates, Lund, Sweden, Vol. 26, No. 2, December 2004, pp.1–7. 

16. Aitcin, P.C., Jolicoeur, C, and MacGregor, J.G., “Superplasticizers: How They Work and 

Why They Occasionally Don’t,” Concrete International, Vol. 16, No. 5, May 1994, 

pp. 45–52. 

17. Helmuth, R.A., “Fly Ash in Cement and Concrete,” Portland Cement Association, 

Skokie, IL, 1987. 

18. Ferraris C., Obla K., Hill R., “The Influence of Mineral Admixtures on the Rheology of 

Cement Paste and Concrete,” Cement and Concrete Research, Vol. 31, No. 2, 2001, 

pp. 245–255. 

19. Bhattacharja, S. and Tang, F. J., “Rheology of Cement Paste in Concrete with Different 

Mix Designs and Interlaboratory Evaluation of the Mini-Slump Cone Test,” PCA R&D 

Serial No. 2412, Portland Cement Association, Skokie, IL, 2000. 

20. Hackley V.A., Ferraris C. F., “Guide to Rheological Nomenclature: Measurements in 

Ceramic Particulate Systems,” NIST Special Publication 946, January 2001, pp. 35. 

21. Kantro, D.L., Influence of Water-Reducing Admixtures on the Properties of Cement 

Paste—A Miniature Slump Test, PCA R & D Bulletin, RD079.01T, Portland Cement 

Association, Skokie, IL, 1980, pp. 95–102. 

22. Helmuth, R.A., Hills, L.M., Whiting, D.A., and Bhattacharja, S., “Abnormal Concrete 

Performance in the Presence of Admixtures,” PCA R & D Serial No. 2006, Portland 

Cement Association, Skokie, IL, 1995. 

23. Ferraris C.F., “Measurement of the Rheological Properties of Cement Paste: A New 

Approach,” International RILEM Conference on the Role of Admixtures in High 

Performance Concrete, J.G. Cabrera and R. Rivera-Villareal, Eds., Monterrey, Mexico 

March 21–26, 1999b, pp. 333–342. 

24. Ferraris, C.F. and Gaidis, J.M., “Connection between Rheology of Concrete and 

Rheology of Cement paste,” ACI Materials Journal, Vol. 88, No. 4, 1992, pp. 388–393. 

25. Ferraris, C.F., “Measurements of Rheological Properties of High Performance Concrete: 

State of the Art Report,” Journal of Research of the National Institute of Standards and 

Technology, Vol. 104, No. 5, 1996, pp. 461–478. 
147

26. Wong, G.S., Alexander, A.M., Haskins, R., Poole, T.S., Malone, P.G., and Wakeley, L., 

Portland-Cement Concrete Rheology and Workability: Final Report, FHWA-RD-00-025, 

Federal Highway Administration, McLean, VA, April 2001. 

27. Wang J.N., Kennedy T.W., McGennis R.B., “Volumetric and Mechanical Performance 

Properties of Superpave Mixtures,” Journal of Materials In Civil Engineering, Vol. 12, 

No. 3, August 2000, pp.238–244. 

28. Struble, L.J. and Ji, X., “Rheology,” Handbook of Analytical Techniques in Concrete 

Science and Technology, Principles, Techniques, and Applications, Ed. Ramachandran, 

V.S. and J.J. Beaudoin, Noyes Publications, Park Ridge, NJ, William Andrew Publishing, 

Norwich, New York, 2001, pp. 333–367. 

29. Tattersall, G.H. and Baker, P.H., “The Effect of Vibration on the Rheological Properties 

of Fresh Concrete,” Magazine of Concrete Research, Vol. 40, No, 143, 1988 pp. 79–89. 

30. De Larrard, F., Hu C., Szitkar, J.C., Joly, M., Claux, F. and Sedran, T., “A New 

Rheometer for Soft-to-Fluid Fresh Concrete,” Laboratoire Central des Ponts et Chaussees 

(LCPC) internal report, 1995. 

31. Popovics, S., Fundamentals of Portland Cement Concrete: A Quantitative Approach, 

John Wiley & Sons, 1982. 

32. Aldea, C.M., Ghandehar, M., Shah, S.P., and Karr, A., “Estimation of Water Flow 

through Cracked Concrete under Load,” ACI Materials Journal, Vol. 97, No. 5, 

September–October 2000, pp. 567–575. 

33. Chatterji, S., “Probable Mechanisms of Crack Formation at Early Ages of Concretes,” 

International Conference on Concrete of Early Ages, RILEM, 1982, pp. 35–38. 

34. Springenschmid, R., Breitenbücher, R., and Mangold, M., “Practical Experience with 

Concrete Technological measures to Avoid Cracking,” Thermal Cracking in Concrete at 

Early Ages, RILEM Proceedings 25, R. Springenschmid, Ed. E&FN Spon, 1995, 

pp. 377–384. 

35. Springenschmid, R. and Breitenbücher, R. “Influence of Constituents, Mix Proportions 

and Temperature on Cracking Sensitivity of Concrete,” Prevention of Thermal Cracking 

in Concrete at Early Ages, RILEM Report 15, R. Springenschmid, Ed. E&FN Spon, 

1998, pp. 40–50. 

36. Powers, T.C., “Void Spacing as a Basis for Producing Air-Entrained Concrete,” ACI 

Journal, RX049, Portland Cement Association, Skokie, IL, Vol. 50, May 1954, pp. 741–

760. 

37. Krauss, P.D. and Rogalla, E.A., Transverse Cracking in Newly Constructed Bridge 

Decks, National Cooperative Highway Research Board Report 380, National Academy 

Press, Washington, DC, 1996, p. 126. 
148

38. Holt, E.E., “Where Did These Cracks Come From?” Concrete International, Vol. 22, 

No. 9, September 2000, pp. 57–60. 

39. Bernander, S., “Practical Measures to Avoiding Early Age Thermal Cracking in Concrete 

Structures,” Chapter 9, Prevention of Thermal Cracking in Concrete at Early Ages,

RILEM Report 15, R. Springenschmid, Ed. E&FN Spon, 1998, pp. 255–314. 

40. Van Breugel, K., “Prediction of Temperature Development in Hardening Concrete,” 

Prevention of Thermal Cracking in Concrete at Early Ages, RILEM Report 15, R. 

Springenschmid, Ed. E&FN Spon, 1998, pp. 51–75. 

41. Roper, H. and Anderson, T., “Laboratory and Site Studies of Early Dimensional Changes 

and Crack Development,” International Conference on Concrete of Early Ages, RILEM, 

1982, pp. 63–69. 

42. Thomas, M.D.A. and Mukherjee, P.K., “The Effect of Slag on Thermal Cracking in 

Concrete,” Thermal Cracking in Concrete at Early Ages, RILEM Proceedings 25, R. 

Springenschmid, Ed. E&FN Spon, 1995, pp. 197–204. 

43. Chan, Y.W.; Liu, C.Y.; and Lu, Y.S., “Effects of Slag and Fly Ash on the Autogenous 

Shrinkage of High Performance Concrete,” Autogenous Shrinkage of Concrete, Ei-ichi 

Tazawa, Ed., E & FN Spon, London, UK and New York, 1999, pp. 221–228. 

44. Ziegeldorf, S., Müller, H.S., Plöehn, J., and Hilsdorf, H.K., “Autogenous Shrinkage and 

Crack Formation in Young Concrete,” International Conference on Concrete of Early 

Ages, RILEM, Vol. I, 1982, pp. 83–88. 

45. Sellevold, E., Bjøntegaard, Ø., Justnes, H., and Dahl, P.A. “High Performance Concrete: 

Early Volume Change and Cracking Tendency,” Thermal Cracking in Concrete at Early 

Ages, RILEM Proceedings 25, R. Springenschmid, Ed. E&FN Spon, 1995, pp. 229–236. 

46. Whiting, D.A. and Detwiler, R.J. “Silica Fume Concrete for Bridge Decks,” National 

Cooperative Highway Research Program Report 410, Transportation Research Board, 

National Academy Press, Washington, DC, 1998, pp.47. 

47. Breitenbücher, R. and Mangold, M., “Minimization of Thermal Cracking in Concrete 

Members at Early Ages,” Thermal Cracking in Concrete at Early Ages, RILEM 

Proceedings 25, R. Springenschmid, Ed. E&FN Spon, 1995, pp. 205–212. 

48. Japan Concrete Institute Technical Committee on Autogenous Shrinkage of Concrete, 

Committee Report, Autogenous Shrinkage of Concrete, Ei-ichi Tazawa, Ed., London and 

New York: E & FN Spon, 1999, pp. 1–62. 

49. Holt, E.E. and Leivo, M.T. “Autogenous Shrinkage at Very Early Ages,” Autogenous 

Shrinkage of Concrete, Ei-ichi Tazawa, Ed., E & FN Spon, London, UK and New York, 

1999, pp. 135–142. 
149

50. Rapoport, J.R., J.S. Popovics, S.V. Kolluru, and Shah, S.P., “Using Ultrasound to 

Monitor Stiffening Process of Concrete with Admixtures,” ACI Materials Journal, 

Vol. 97, No. 6 (November–December 2000) pp. 675–683. 

51. See, H.T., Attiogbe, E.K., and Miltenberger, M.A., “Shrinkage Cracking Characteristics 

of Concrete Using Ring Specimens,” ACI Materials Journal, Vol. 100, No. 3, May-June 

2003. pp. 239–245. 

52. Hossain, A.; Pease, B.; and Weiss, J., “Quantitative Early-Age Stress Development and 

Cracking in Low W/C Concrete Using the Restraining Ring Test with Acoustic 

Emission,” Transportation Research Board, 82nd Annual Meeting, Compendium of 

Papers CD ROM, January 12–16, 2003. 

53. Taylor, H.F.W., Cement Chemistry, Academic Press, New York, 1990 pp. 233–234. 

54. Plante, P., Pigeon, M. and Foy, C. “The Influence of Water-Reducers on the Production 

and Stability of the Air void System in Concrete,” Cement and Concrete Research, Vol. 

19, No. 4, 1989, pp. 621–633. 

55. Stott, D., Rezansoff, T. and Sparling, B.F., “Loss of Freeze-Thaw Durability of Concrete 

Containing Accelerating Admixtures,” Canadian Journal of Civil Engineering, Vol. 21, 

No. 4, 1994, pp. 605–613. 

56. Attiogbe, E.K., Nmai, C.K., and Gay, F.T., “Air-Void System Parameters and FreezeThaw Durability of Concrete Containing Superplasticizers,” Concrete International, 

American Concrete Institute, Vol. 14, No. 7, July 1992, pp. 57–61. 

57. “Manufacturing Air-Entrained Concrete,” Betonwerk Fertigteil Technik (BFT), Vol. 1, 

2002, pp. 46–52. 

58. Pigeon, M., Plante, P., Pleau, R. and Banthia, N., “The Influence of Soluble Alkalies on 

the Production and Stability of the Air void System in Superplasticized and 

Nonsuperplasticized Concrete,” ACI Materials Journal, Vol. 89, No.1, 1992, pp. 24–31. 

59. Personal communication from David Stark, Construction Technology Laboratories, to 

Peter Taylor (2002). 

60. Gebler, S.H. and Klieger, P., “Effect of Fly Ash on the Air void Stability of Concrete,” 

Portland Cement Association, Skokie, IL, 1986, 40 pp. 

61. Langan, B.W., Joshi, R.C. and Ward, M.A., “Strength and Durability of Concrete 

Containing 50% Portland Cement Replacement by Flyash and Other Materials,” 

Canadian Journal of Civil Engineering, Vol. 17, No. 1, 1990, pp. 19–27. 

62. Saucier, F., Pigeon, M. and Cameron, G., “Air Void Stability, Part V: Temperature, 

General Analysis and Performance Index,” ACI Materials Journal, Vol. 88, No. 1, 

January-February, 1991, pp. 25–37. 
150

63. Gardner, T.J.; Beushausen, H-D., and Alexender, M.G., “The Effect of Elevated 

Temperatures on the Properties of Concrete,” BFT, Vol. 70, No. 5, 2004 pp. 6–13. 

64. Pang, Y.; Lou, H., Qiu, X., and Yang, D., “Influences of Modified Lignosulfonate 

Superplasticizer on Cement Hydration and the Durability of Concrete,” Journal of 

Sichuan University (Engineering Science Edition), Chengdu, China, Vol. 37, No. 1, 

January 2005, pp. 74–77. 

65. Khayat, K. H. and Assaad, J., “Air Void Stability in Self-Consolidating Concrete,” ACI 

Materials Journal, Vol. 99, No. 4, July/August 2002, pp. 408–416. 

66. Nagi, M. and Whiting, D., “Achieving and Verifying Air Content in Concrete,” Research 

and Development Bulletin RP324, Portland Cement Association, Skokie, IL, 1994, 40 pp. 

67. Hover, K.C., “Some Recent Problems with Air-Entrained Concrete,” Cement, Concrete, 

and Aggregates, Vol.11, No. 1, 1989, pp. 73–80. 

68. Cross, W., Duke, E., Kellar, J. and Johnston, D., Investigation of Low Compressive 

Strengths of Concrete Paving, Precast and Structural Concrete, South Dakota 

Department of Transportation Report SD98-03-F, 2000, 78 pp. 

69. Kozikowski, Jr. R.L., Vollmer, D.B.; Taylor, P.C., and Gebler, S.H., “Factors Affecting 

the Origin of Air Void Clustering,” PCA R&D Serial No. 2789, Portland Cement 

Association, Skokie, IL, 22 pp, 2005. 

70. Higginson, E.C., “Some Effects of Vibration and Handling on Concrete Containing 

Entrained Air,” Journal of the American Concrete Institute, Vol. 24, No. 1, 1952, 

pp. 1–12. 

71. Mehta, P.K., Concrete: Structure, Properties, and Materials, Prentice-Hall, Inc., 

Englewood Cliff, NJ, 1986, 449 pp. 

72. Torrans, P.H. and Ivey, D.L., The Void Spacing Indicator, Texas Transportation Institute, 

Research Report No. 103–3, 1969, 42 pp. 

73. Johansen, P.E., “Characterization of the Air void System in Concrete by a Vibration 

Test,” RILEM-ABEM International Symposium on Concrete Admixtures, Topic V, 1967, 

pp. 7–29. 

74. Henrichsen, J.V., “Quality Assurance of Air void Structures in Concrete,” International 

Symposium on Non-Destructive Testing in Civil Engineering, (NDT-CE) 26.28.09, 

German Society for Non-Destructive Testing (DGZfP), Berlin, Germany, 

September,1995, 8 pp. 

75. Germann Instruments, Evanston, IL, Personal Communication. 

76. Magura, D.D., Air void Analyzer Evaluation, Report No. FHWA-SA-96-062, Federal 

Highway Administration, Washington, DC, 1996. 
151

77. Redmond, Michael “Air void Analyzer,” Priority Technology Program, Final Report, 

State of Maine, Department of Transportation, 1999, 7 pp. 

78. Zhang, Z., Ansari, F., and Vitillo, N., “Automated Determination of Entrained Air Void 

Parameters in Hardened Concrete,” ACI Materials Journal, Vol. 102, No. 1, 

January/February 2005, pp. 42–48. 

79. Bruere, G.M., “Air Entrainment in Cement and Silica Paste,” Journal of the American 

Concrete Institute, Vol. 26, No. 9, 1955, pp. 905–920. 

80. Dodson, V., “Air-Entraining Admixtures,” Concrete Admixtures, Chapter 6,Van 

Nostrand Reinhold, London, UK, 1990, pp. 129–158. 

81. Gutmann, P.F., “Bubble Characteristics as They Pertain to Compressive Strength and 

Freeze-Thaw Durability,” Bonding in Cementitious Composites, Materials Research 

Society Symposium Proceedings, Materials Research Society, Pittsburgh, PA. Vol. 114,

1988, pp. 271–277. 

82. Tang, F. J. and Bhattacharja, S., Early Stiffening Test Development for Portland Cement, 

Portland Cement Association R&D Serial No. 1999, 1996, 31 pp., 1996. 

83. Barneyback, R.S. Jr.; “Alkali-Silica Reaction in Portland Cement Concrete,” Ph.D. 

Thesis, Purdue University, Lafayette, IN, 1987. 

84. Gartner, Ellis M., Tang, Fulvio J., and Weiss, Stuart J., “Saturation Factors for Calcium 

Hydroxide and Calcium Sulfates in Fresh Portland Cement Pastes,” Journal of the 

American Ceramic Society, Vol. 68, No. 12, 1985, pp. 667–673. 

85. Rothstein, D., Thomas J., Christensen, B.J., Jennings, H.M., “Solubility Behavior of Ca-, 

S-, Al-, and Si-bearing Solid Phases in Portland Cement Pore Solutions as a Function of 

Hydration Time,” Cement and Concrete Research, Vol. 32, No. 10, 2002, pp. 1663–

1671. 

86. Alexander, A.M., Haskins, R.W, Sari, A., Soroushian, P., and Hsu, J-W., “New 

Technologies for Improving the Consolidation of Concrete,” U.S. Army Corps of 

Engineers, Waterways Experiment Station, CPAR-SL-97-2, September 1997. 
HRDI-12/08-06(1M200)E

Recycled

Recyclable